#------------------------------------------------------------------------------
#$Date: 2016-03-22 11:56:50 +0200 (Tue, 22 Mar 2016) $
#$Revision: 178925 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/54/4115473.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4115473
loop_
_publ_author_name
'Svilen Bobev'
'Slavi C. Sevov'
_publ_contact_author
;
Slavi C. Sevov
Department of Chemistry and Biochemistry
251 Nieuwland Science Hall
University of Notre Dame
Notre Dame, IN 46556-5670
USA
;
_publ_contact_author_email       ssevov@nd.edu
_publ_contact_author_fax         'Intl. Code + (219)631-6652'
_publ_contact_author_phone       'Intl. Code + (219)631-5891'
_publ_section_title
;
 Clathrate III of Group 14 Exists After All
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              3389
_journal_page_last               3390
_journal_paper_doi               10.1021/ja010010f
_journal_volume                  123
_journal_year                    2001
_chemical_formula_moiety         Cs3.75Na0.36Sn20.29
_chemical_formula_sum            'Cs3.75 Na0.36 Sn20.29'
_chemical_formula_weight         2914.67
_chemical_name_common            clathrate-III
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           136
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4n 2n'
_symmetry_space_group_name_H-M   'P 42/m n m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   23.5566(9)
_cell_length_b                   23.5566(9)
_cell_length_c                   12.1040(9)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      19.66
_cell_measurement_theta_min      13.94
_cell_volume                     6716.7(6)
_computing_cell_refinement       CAD4_(Enraf-Nonius,_1977)
_computing_data_collection       CAD4_(Enraf-Nonius,_1977)
_computing_data_reduction        SDS_Package_(Enraf-Nonius,_1985)
_computing_molecular_graphics    'SHELXTL (Siemens, 1994)'
_computing_publication_material  'SHELXTL (Siemens, 1994)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  Enraf_Nonius_CAD4
_diffrn_measurement_method       omega-2theta
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0475
_diffrn_reflns_limit_h_max       26
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       38
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            7865
_diffrn_reflns_theta_full        34.98
_diffrn_reflns_theta_max         34.98
_diffrn_reflns_theta_min         2.08
_diffrn_standards_interval_count 200
_diffrn_standards_interval_time  120
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    18.780
_exptl_absorpt_correction_T_max  0.3150
_exptl_absorpt_correction_T_min  0.2115
_exptl_absorpt_correction_type   psi-scan
_exptl_absorpt_process_details   'average of 5 psi-scan reflections'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    5.765
_exptl_crystal_description       bar
_exptl_crystal_F_000             9797
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.08
_refine_diff_density_max         4.679
_refine_diff_density_min         -5.884
_refine_diff_density_rms         0.611
_refine_ls_extinction_coef       0.000003(1)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.204
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     151
_refine_ls_number_reflns         7865
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.204
_refine_ls_R_factor_all          0.1037
_refine_ls_R_factor_gt           0.0824
_refine_ls_shift/su_max          0.005
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0120P)²+724.7363P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1534
_refine_ls_wR_factor_ref         0.1611
_reflns_number_gt                6298
_reflns_number_total             7865
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja010010f_2.cif
_cod_data_source_block           CAD4
_cod_database_code               4115473
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-y+1/2, x+1/2, z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'y, x, -z'
'-y, -x, -z'
'-x, -y, -z'
'x, y, -z'
'y-1/2, -x-1/2, -z-1/2'
'-y-1/2, x-1/2, -z-1/2'
'x-1/2, -y-1/2, z-1/2'
'-x-1/2, y-1/2, z-1/2'
'-y, -x, z'
'y, x, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Sn1 Sn 0.81530(4) 0.44728(4) 0.18183(8) 0.01726(18) Uani 1 1 d .
Sn2 Sn 0.26434(6) 0.26434(6) 0.0000 0.0130(3) Uani 1 4 d S
Sn3 Sn 0.14584(6) 0.29541(6) 0.0000 0.0145(2) Uani 1 2 d S
Sn4 Sn 0.39406(4) 0.39406(4) 0.11822(11) 0.0157(2) Uani 1 2 d S
Sn5 Sn 0.65595(6) 0.43004(6) 0.0000 0.0156(2) Uani 1 2 d S
Sn6 Sn 0.73486(4) 0.50961(5) 0.31016(9) 0.01968(19) Uani 1 1 d .
Sn7 Sn 0.86268(4) 0.63322(4) 0.18947(8) 0.01734(18) Uani 1 1 d .
Sn8 Sn 0.05872(6) 0.20870(7) 0.0000 0.0181(3) Uani 1 2 d S
Sn9 Sn 0.0000 0.5000 0.2500 0.0121(3) Uani 1 4 d S
Sn10 Sn 0.31388(4) 0.31388(4) 0.19712(12) 0.0180(2) Uani 1 2 d S
Sn11 Sn 0.90213(4) 0.52479(4) -0.11929(8) 0.01455(16) Uani 1 1 d .
Sn12 Sn 0.63142(5) 0.49547(4) 0.19543(9) 0.02016(19) Uani 1 1 d .
Sn13 Sn 0.23057(7) 0.61621(8) 0.0000 0.0245(3) Uani 1 2 d S
Sn14 Sn 0.04004(9) 0.04004(9) 0.1734(3) 0.0402(6) Uani 0.79 2 d SP
Sn15 Sn 0.76627(5) 0.62749(5) 0.33195(12) 0.0298(3) Uani 1 1 d .
Sn16 Sn 0.09286(12) 0.09286(12) 0.0000 0.0168(6) Uani 0.52 4 d SP
Sn17 Sn 0.2000(3) 0.7274(3) 0.0000 0.0203(11) Uani 0.24 2 d SP
Na1 Na 0.2404(8) 0.7596(8) 0.0000 0.033(7) Uani 0.52 4 d SP
Na2 Na 0.0697(16) 0.0697(16) 0.087(5) 0.009(9) Uiso 0.11 2 d SP
Cs1 Cs 0.89535(11) 0.10465(11) 0.0000 0.0605(9) Uani 1 4 d S
Cs2 Cs 0.17812(8) 0.17812(8) 0.24320(18) 0.0505(6) Uani 1 2 d S
Cs3 Cs 0.37319(7) 0.96984(9) 0.0000 0.0379(4) Uani 1 2 d S
Cs4 Cs 0.75015(5) 0.56577(6) 0.0000 0.0173(2) Uani 1 2 d S
Cs5 Cs 0.0000 0.0000 0.5000 0.0208(5) Uani 1 8 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Sn Sn -0.6537 1.4246 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Sn7 Sn1 Sn11 107.04(4) 12_756 10
Sn7 Sn1 Sn6 110.49(4) 12_756 .
Sn11 Sn1 Sn6 106.96(4) 10 .
Sn7 Sn1 Sn13 102.61(5) 12_756 9_665
Sn11 Sn1 Sn13 113.63(5) 10 9_665
Sn6 Sn1 Sn13 115.77(5) . 9_665
Sn7 Sn1 Cs4 177.73(4) 12_756 .
Sn11 Sn1 Cs4 70.79(3) 10 .
Sn6 Sn1 Cs4 71.07(3) . .
Sn13 Sn1 Cs4 77.92(4) 9_665 .
Sn7 Sn1 Cs2 74.36(4) 12_756 11_666
Sn11 Sn1 Cs2 176.22(5) 10 11_666
Sn6 Sn1 Cs2 75.51(5) . 11_666
Sn13 Sn1 Cs2 62.59(5) 9_665 11_666
Cs4 Sn1 Cs2 107.77(4) . 11_666
Sn7 Sn1 Cs3 72.77(4) 12_756 13_676
Sn11 Sn1 Cs3 74.51(4) 10 13_676
Sn6 Sn1 Cs3 61.03(4) . 13_676
Sn13 Sn1 Cs3 171.74(5) 9_665 13_676
Cs4 Sn1 Cs3 106.98(4) . 13_676
Cs2 Sn1 Cs3 109.27(4) 11_666 13_676
Sn7 Sn1 Cs3 69.75(3) 12_756 7
Sn11 Sn1 Cs3 63.06(3) 10 7
Sn6 Sn1 Cs3 168.70(5) . 7
Sn13 Sn1 Cs3 74.54(4) 9_665 7
Cs4 Sn1 Cs3 108.38(3) . 7
Cs2 Sn1 Cs3 114.74(5) 11_666 7
Cs3 Sn1 Cs3 109.41(4) 13_676 7
Sn7 Sn1 Na1 72.3(2) 12_756 9_665
Sn11 Sn1 Na1 129.28(13) 10 9_665
Sn6 Sn1 Na1 121.0(2) . 9_665
Sn13 Sn1 Na1 31.03(17) 9_665 9_665
Cs4 Sn1 Na1 108.5(2) . 9_665
Cs2 Sn1 Na1 47.48(14) 11_666 9_665
Cs3 Sn1 Na1 142.50(13) 13_676 9_665
Cs3 Sn1 Na1 70.2(2) 7 9_665
Sn3 Sn2 Sn3 119.38(8) 7 .
Sn3 Sn2 Sn10 106.685(19) 7 10
Sn3 Sn2 Sn10 106.684(19) . 10
Sn3 Sn2 Sn10 106.685(19) 7 .
Sn3 Sn2 Sn10 106.684(19) . .
Sn10 Sn2 Sn10 110.65(8) 10 .
Sn3 Sn2 Cs4 70.43(3) 7 15_665
Sn3 Sn2 Cs4 170.18(6) . 15_665
Sn10 Sn2 Cs4 68.49(3) 10 15_665
Sn10 Sn2 Cs4 68.49(3) . 15_665
Sn3 Sn2 Cs4 170.18(6) 7 9_665
Sn3 Sn2 Cs4 70.43(3) . 9_665
Sn10 Sn2 Cs4 68.49(3) 10 9_665
Sn10 Sn2 Cs4 68.49(3) . 9_665
Cs4 Sn2 Cs4 99.75(5) 15_665 9_665
Sn3 Sn2 Cs2 69.36(4) 7 10
Sn3 Sn2 Cs2 69.36(4) . 10
Sn10 Sn2 Cs2 78.97(5) 10 10
Sn10 Sn2 Cs2 170.38(7) . 10
Cs4 Sn2 Cs2 116.75(2) 15_665 10
Cs4 Sn2 Cs2 116.75(2) 9_665 10
Sn3 Sn2 Cs2 69.36(4) 7 .
Sn3 Sn2 Cs2 69.36(4) . .
Sn10 Sn2 Cs2 170.38(7) 10 .
Sn10 Sn2 Cs2 78.97(5) . .
Cs4 Sn2 Cs2 116.75(2) 15_665 .
Cs4 Sn2 Cs2 116.75(2) 9_665 .
Cs2 Sn2 Cs2 91.41(8) 10 .
Sn7 Sn3 Sn7 107.12(6) 2_665 9_665
Sn7 Sn3 Sn2 102.57(4) 2_665 .
Sn7 Sn3 Sn2 102.57(4) 9_665 .
Sn7 Sn3 Sn8 111.48(4) 2_665 .
Sn7 Sn3 Sn8 111.48(4) 9_665 .
Sn2 Sn3 Sn8 120.45(6) . .
Sn7 Sn3 Cs4 64.55(3) 2_665 9_665
Sn7 Sn3 Cs4 64.55(3) 9_665 9_665
Sn2 Sn3 Cs4 67.85(5) . 9_665
Sn8 Sn3 Cs4 171.70(6) . 9_665
Sn7 Sn3 Cs2 170.45(5) 2_665 10
Sn7 Sn3 Cs2 80.40(4) 9_665 10
Sn2 Sn3 Cs2 69.54(4) . 10
Sn8 Sn3 Cs2 69.93(5) . 10
Cs4 Sn3 Cs2 115.29(5) 9_665 10
Sn7 Sn3 Cs2 80.40(4) 2_665 .
Sn7 Sn3 Cs2 170.45(5) 9_665 .
Sn2 Sn3 Cs2 69.54(4) . .
Sn8 Sn3 Cs2 69.93(5) . .
Cs4 Sn3 Cs2 115.30(5) 9_665 .
Cs2 Sn3 Cs2 91.54(6) 10 .
Sn7 Sn3 Cs3 72.37(4) 2_665 7_455
Sn7 Sn3 Cs3 72.37(4) 9_665 7_455
Sn2 Sn3 Cs3 170.85(6) . 7_455
Sn8 Sn3 Cs3 68.70(5) . 7_455
Cs4 Sn3 Cs3 103.00(4) 9_665 7_455
Cs2 Sn3 Cs3 116.18(3) 10 7_455
Cs2 Sn3 Cs3 116.18(3) . 7_455
Sn7 Sn3 Na2 132.5(5) 2_665 10
Sn7 Sn3 Na2 112.2(5) 9_665 10
Sn2 Sn3 Na2 93.9(2) . 10
Sn8 Sn3 Na2 28.4(3) . 10
Cs4 Sn3 Na2 159.0(4) 9_665 10
Cs2 Sn3 Na2 45.5(5) 10 10
Cs2 Sn3 Na2 64.2(5) . 10
Cs3 Sn3 Na2 95.1(2) 7_455 10
Sn7 Sn3 Na2 112.2(5) 2_665 .
Sn7 Sn3 Na2 132.5(5) 9_665 .
Sn2 Sn3 Na2 93.9(2) . .
Sn8 Sn3 Na2 28.4(3) . .
Cs4 Sn3 Na2 159.0(4) 9_665 .
Cs2 Sn3 Na2 64.2(5) 10 .
Cs2 Sn3 Na2 45.5(5) . .
Cs3 Sn3 Na2 95.1(2) 7_455 .
Na2 Sn3 Na2 21.3(11) 10 .
Sn12 Sn4 Sn12 106.32(6) 15_665 2_665
Sn12 Sn4 Sn10 111.10(4) 15_665 .
Sn12 Sn4 Sn10 111.10(4) 2_665 .
Sn12 Sn4 Sn4 109.29(3) 15_665 10
Sn12 Sn4 Sn4 109.29(3) 2_665 10
Sn10 Sn4 Sn4 109.68(4) . 10
Sn12 Sn4 Cs4 72.91(3) 15_665 15_665
Sn12 Sn4 Cs4 176.30(5) 2_665 15_665
Sn10 Sn4 Cs4 72.41(3) . 15_665
Sn4 Sn4 Cs4 67.92(2) 10 15_665
Sn12 Sn4 Cs4 176.30(5) 15_665 9_665
Sn12 Sn4 Cs4 72.91(3) 2_665 9_665
Sn10 Sn4 Cs4 72.41(3) . 9_665
Sn4 Sn4 Cs4 67.92(2) 10 9_665
Cs4 Sn4 Cs4 107.61(5) 15_665 9_665
Sn12 Sn4 Cs5 70.15(3) 15_665 3_554
Sn12 Sn4 Cs5 70.15(3) 2_665 3_554
Sn10 Sn4 Cs5 177.61(6) . 3_554
Sn4 Sn4 Cs5 67.93(2) 10 3_554
Cs4 Sn4 Cs5 106.30(3) 15_665 3_554
Cs4 Sn4 Cs5 106.30(3) 9_665 3_554
Sn12 Sn4 Cs1 70.43(4) 15_665 3_545
Sn12 Sn4 Cs1 70.43(4) 2_665 3_545
Sn10 Sn4 Cs1 70.86(6) . 3_545
Sn4 Sn4 Cs1 179.46(5) 10 3_545
Cs4 Sn4 Cs1 112.35(3) 15_665 3_545
Cs4 Sn4 Cs1 112.35(3) 9_665 3_545
Cs5 Sn4 Cs1 111.53(6) 3_554 3_545
Sn12 Sn4 Na2 78.7(5) 15_665 12_666
Sn12 Sn4 Na2 29.7(6) 2_665 12_666
Sn10 Sn4 Na2 112.6(4) . 12_666
Sn4 Sn4 Na2 130.2(5) 10 12_666
Cs4 Sn4 Na2 150.7(6) 15_665 12_666
Cs4 Sn4 Na2 101.2(5) 9_665 12_666
Cs5 Sn4 Na2 69.5(4) 3_554 12_666
Cs1 Sn4 Na2 49.4(5) 3_545 12_666
Sn12 Sn4 Na2 29.7(6) 15_665 11_666
Sn12 Sn4 Na2 78.7(5) 2_665 11_666
Sn10 Sn4 Na2 112.6(4) . 11_666
Sn4 Sn4 Na2 130.2(5) 10 11_666
Cs4 Sn4 Na2 101.2(5) 15_665 11_666
Cs4 Sn4 Na2 150.7(6) 9_665 11_666
Cs5 Sn4 Na2 69.5(4) 3_554 11_666
Cs1 Sn4 Na2 49.4(5) 3_545 11_666
Na2 Sn4 Na2 49.7(11) 12_666 11_666
Sn5 Sn5 Sn12 103.67(3) 15_665 .
Sn5 Sn5 Sn12 103.67(3) 15_665 10
Sn12 Sn5 Sn12 110.33(6) . 10
Sn5 Sn5 Sn13 112.83(5) 15_665 9_665
Sn12 Sn5 Sn13 112.80(4) . 9_665
Sn12 Sn5 Sn13 112.80(4) 10 9_665
Sn5 Sn5 Cs4 169.76(3) 15_665 .
Sn12 Sn5 Cs4 71.03(3) . .
Sn12 Sn5 Cs4 71.03(3) 10 .
Sn13 Sn5 Cs4 77.41(5) 9_665 .
Sn5 Sn5 Cs5 69.161(19) 15_665 3_554
Sn12 Sn5 Cs5 66.30(3) . 3_554
Sn12 Sn5 Cs5 66.30(3) 10 3_554
Sn13 Sn5 Cs5 178.01(6) 9_665 3_554
Cs4 Sn5 Cs5 100.60(4) . 3_554
Sn5 Sn5 Cs2 69.30(2) 15_665 4_554
Sn12 Sn5 Cs2 172.56(5) . 4_554
Sn12 Sn5 Cs2 74.49(4) 10 4_554
Sn13 Sn5 Cs2 69.11(4) 9_665 4_554
Cs4 Sn5 Cs2 116.30(3) . 4_554
Cs5 Sn5 Cs2 112.02(4) 3_554 4_554
Sn5 Sn5 Cs2 69.30(2) 15_665 11_666
Sn12 Sn5 Cs2 74.49(4) . 11_666
Sn12 Sn5 Cs2 172.56(5) 10 11_666
Sn13 Sn5 Cs2 69.11(4) 9_665 11_666
Cs4 Sn5 Cs2 116.30(3) . 11_666
Cs5 Sn5 Cs2 112.02(4) 3_554 11_666
Cs2 Sn5 Cs2 100.16(8) 4_554 11_666
Sn5 Sn5 Na1 73.66(9) 15_665 9_665
Sn12 Sn5 Na1 124.44(3) . 9_665
Sn12 Sn5 Na1 124.44(3) 10 9_665
Sn13 Sn5 Na1 39.16(10) 9_665 9_665
Cs4 Sn5 Na1 116.58(9) . 9_665
Cs5 Sn5 Na1 142.82(9) 3_554 9_665
Cs2 Sn5 Na1 52.16(5) 4_554 9_665
Cs2 Sn5 Na1 52.16(5) 11_666 9_665
Sn5 Sn5 Na2 74.60(16) 15_665 4_554
Sn12 Sn5 Na2 133.2(6) . 4_554
Sn12 Sn5 Na2 33.2(3) 10 4_554
Sn13 Sn5 Na2 110.5(6) 9_665 4_554
Cs4 Sn5 Na2 102.35(18) . 4_554
Cs5 Sn5 Na2 69.9(6) 3_554 4_554
Cs2 Sn5 Na2 48.6(6) 4_554 4_554
Cs2 Sn5 Na2 139.4(3) 11_666 4_554
Na1 Sn5 Na2 100.5(5) 9_665 4_554
Sn5 Sn5 Na2 74.60(16) 15_665 11_666
Sn12 Sn5 Na2 33.2(3) . 11_666
Sn12 Sn5 Na2 133.2(6) 10 11_666
Sn13 Sn5 Na2 110.5(6) 9_665 11_666
Cs4 Sn5 Na2 102.35(18) . 11_666
Cs5 Sn5 Na2 69.9(6) 3_554 11_666
Cs2 Sn5 Na2 139.4(3) 4_554 11_666
Cs2 Sn5 Na2 48.6(6) 11_666 11_666
Na1 Sn5 Na2 100.5(5) 9_665 11_666
Na2 Sn5 Na2 135.7(9) 4_554 11_666
Sn12 Sn6 Sn1 104.15(5) . .
Sn12 Sn6 Sn8 98.17(5) . 11_666
Sn1 Sn6 Sn8 106.81(5) . 11_666
Sn12 Sn6 Sn15 112.31(5) . .
Sn1 Sn6 Sn15 111.98(5) . .
Sn8 Sn6 Sn15 121.40(5) 11_666 .
Sn12 Sn6 Cs4 69.82(4) . .
Sn1 Sn6 Cs4 66.40(3) . .
Sn8 Sn6 Cs4 162.99(5) 11_666 .
Sn15 Sn6 Cs4 75.18(4) . .
Sn12 Sn6 Cs3 174.52(4) . 13_676
Sn1 Sn6 Cs3 80.49(4) . 13_676
Sn8 Sn6 Cs3 77.52(4) 11_666 13_676
Sn15 Sn6 Cs3 67.90(4) . 13_676
Cs4 Sn6 Cs3 115.11(4) . 13_676
Sn12 Sn6 Cs1 73.61(4) . 11_676
Sn1 Sn6 Cs1 177.75(5) . 11_676
Sn8 Sn6 Cs1 73.75(4) 11_666 11_676
Sn15 Sn6 Cs1 69.18(6) . 11_676
Cs4 Sn6 Cs1 112.43(3) . 11_676
Cs3 Sn6 Cs1 101.75(4) 13_676 11_676
Sn12 Sn6 Na2 48.7(7) . 11_666
Sn1 Sn6 Na2 120.8(6) . 11_666
Sn8 Sn6 Na2 50.2(7) 11_666 11_666
Sn15 Sn6 Na2 126.7(6) . 11_666
Cs4 Sn6 Na2 118.4(7) . 11_666
Cs3 Sn6 Na2 126.5(7) 13_676 11_666
Cs1 Sn6 Na2 57.9(6) 11_676 11_666
Sn12 Sn6 Cs2 64.72(4) . 11_666
Sn1 Sn6 Cs2 68.13(4) . 11_666
Sn8 Sn6 Cs2 61.19(4) 11_666 11_666
Sn15 Sn6 Cs2 176.70(5) . 11_666
Cs4 Sn6 Cs2 102.10(4) . 11_666
Cs3 Sn6 Cs2 115.21(5) 13_676 11_666
Cs1 Sn6 Cs2 110.60(6) 11_676 11_666
Na2 Sn6 Cs2 52.8(6) 11_666 11_666
Sn12 Sn6 Na2 69.3(5) . 4
Sn1 Sn6 Na2 129.1(5) . 4
Sn8 Sn6 Na2 33.4(6) 11_666 4
Sn15 Sn6 Na2 117.1(5) . 4
Cs4 Sn6 Na2 138.9(5) . 4
Cs3 Sn6 Na2 105.5(5) 13_676 4
Cs1 Sn6 Na2 50.4(5) 11_676 4
Na2 Sn6 Na2 21.8(11) 11_666 4
Cs2 Sn6 Na2 63.7(5) 11_666 4
Sn1 Sn7 Sn11 108.76(4) 11_676 10
Sn1 Sn7 Sn3 103.99(5) 11_676 9_665
Sn11 Sn7 Sn3 108.18(4) 10 9_665
Sn1 Sn7 Sn15 104.49(5) 11_676 .
Sn11 Sn7 Sn15 113.41(5) 10 .
Sn3 Sn7 Sn15 117.25(5) 9_665 .
Sn1 Sn7 Cs4 177.14(4) 11_676 .
Sn11 Sn7 Cs4 71.14(3) 10 .
Sn3 Sn7 Cs4 73.48(4) 9_665 .
Sn15 Sn7 Cs4 78.02(4) . .
Sn1 Sn7 Cs3 74.29(4) 11_676 13_676
Sn11 Sn7 Cs3 75.30(4) 10 13_676
Sn3 Sn7 Cs3 176.51(4) 9_665 13_676
Sn15 Sn7 Cs3 60.77(4) . 13_676
Cs4 Sn7 Cs3 108.31(4) . 13_676
Sn1 Sn7 Cs3 71.30(3) 11_676 15_765
Sn11 Sn7 Cs3 62.52(3) 10 15_765
Sn3 Sn7 Cs3 71.11(4) 9_665 15_765
Sn15 Sn7 Cs3 171.59(4) . 15_765
Cs4 Sn7 Cs3 106.39(3) . 15_765
Cs3 Sn7 Cs3 110.83(4) 13_676 15_765
Sn1 Sn7 Cs2 69.62(4) 11_676 2_665
Sn11 Sn7 Cs2 168.06(5) 10 2_665
Sn3 Sn7 Cs2 61.87(4) 9_665 2_665
Sn15 Sn7 Cs2 78.10(5) . 2_665
Cs4 Sn7 Cs2 109.86(4) . 2_665
Cs3 Sn7 Cs2 114.64(4) 13_676 2_665
Cs3 Sn7 Cs2 106.50(4) 15_765 2_665
Sn1 Sn7 Na1 77.8(3) 11_676 3_655
Sn11 Sn7 Na1 143.7(2) 10 3_655
Sn3 Sn7 Na1 104.37(11) 9_665 3_655
Sn15 Sn7 Na1 34.1(3) . 3_655
Cs4 Sn7 Na1 104.0(2) . 3_655
Cs3 Sn7 Na1 72.37(11) 13_676 3_655
Cs3 Sn7 Na1 146.2(3) 15_765 3_655
Cs2 Sn7 Na1 48.2(2) 2_665 3_655
Sn16 Sn8 Sn6 111.36(5) . 3_544
Sn16 Sn8 Sn6 111.36(5) . 12_656
Sn6 Sn8 Sn6 106.26(6) 3_544 12_656
Sn16 Sn8 Sn3 118.44(9) . .
Sn6 Sn8 Sn3 104.23(4) 3_544 .
Sn6 Sn8 Sn3 104.23(4) 12_656 .
Sn16 Sn8 Na2 21.3(8) . 10
Sn6 Sn8 Na2 90.0(8) 3_544 10
Sn6 Sn8 Na2 119.4(9) 12_656 10
Sn3 Sn8 Na2 128.1(7) . 10
Sn16 Sn8 Na2 21.3(8) . .
Sn6 Sn8 Na2 119.4(9) 3_544 .
Sn6 Sn8 Na2 90.0(8) 12_656 .
Sn3 Sn8 Na2 128.1(7) . .
Na2 Sn8 Na2 35.6(18) 10 .
Sn16 Sn8 Cs2 68.93(6) . .
Sn6 Sn8 Cs2 171.16(5) 3_544 .
Sn6 Sn8 Cs2 81.31(3) 12_656 .
Sn3 Sn8 Cs2 68.94(4) . .
Na2 Sn8 Cs2 90.1(7) 10 .
Na2 Sn8 Cs2 64.3(9) . .
Sn16 Sn8 Cs2 68.94(6) . 10
Sn6 Sn8 Cs2 81.32(3) 3_544 10
Sn6 Sn8 Cs2 171.16(5) 12_656 10
Sn3 Sn8 Cs2 68.94(4) . 10
Na2 Sn8 Cs2 64.3(9) 10 10
Na2 Sn8 Cs2 90.1(7) . 10
Cs2 Sn8 Cs2 90.79(5) . 10
Sn16 Sn8 Cs3 168.04(9) . 7_455
Sn6 Sn8 Cs3 62.93(4) 3_544 7_455
Sn6 Sn8 Cs3 62.93(4) 12_656 7_455
Sn3 Sn8 Cs3 73.52(5) . 7_455
Na2 Sn8 Cs3 150.5(7) 10 7_455
Na2 Sn8 Cs3 150.5(7) . 7_455
Cs2 Sn8 Cs3 118.47(4) . 7_455
Cs2 Sn8 Cs3 118.47(4) 10 7_455
Sn16 Sn8 Cs1 73.93(9) . 1_455
Sn6 Sn8 Cs1 69.06(4) 3_544 1_455
Sn6 Sn8 Cs1 69.06(4) 12_656 1_455
Sn3 Sn8 Cs1 167.63(7) . 1_455
Na2 Sn8 Cs1 63.5(7) 10 1_455
Na2 Sn8 Cs1 63.5(7) . 1_455
Cs2 Sn8 Cs1 118.70(5) . 1_455
Cs2 Sn8 Cs1 118.70(5) 10 1_455
Cs3 Sn8 Cs1 94.11(6) 7_455 1_455
Sn11 Sn9 Sn11 107.864(18) 4_465 10_455
Sn11 Sn9 Sn11 112.74(4) 4_465 3_545
Sn11 Sn9 Sn11 107.864(19) 10_455 3_545
Sn11 Sn9 Sn11 107.864(19) 4_465 9_665
Sn11 Sn9 Sn11 112.74(4) 10_455 9_665
Sn11 Sn9 Sn11 107.864(18) 3_545 9_665
Sn11 Sn9 Cs3 169.03(2) 4_465 7_455
Sn11 Sn9 Cs3 67.66(3) 10_455 7_455
Sn11 Sn9 Cs3 78.22(3) 3_545 7_455
Sn11 Sn9 Cs3 66.58(3) 9_665 7_455
Sn11 Sn9 Cs3 66.58(3) 4_465 5_545
Sn11 Sn9 Cs3 169.03(2) 10_455 5_545
Sn11 Sn9 Cs3 67.66(3) 3_545 5_545
Sn11 Sn9 Cs3 78.22(3) 9_665 5_545
Cs3 Sn9 Cs3 119.518(19) 7_455 5_545
Sn11 Sn9 Cs3 78.22(3) 4_465 15_665
Sn11 Sn9 Cs3 66.58(3) 10_455 15_665
Sn11 Sn9 Cs3 169.03(2) 3_545 15_665
Sn11 Sn9 Cs3 67.66(3) 9_665 15_665
Cs3 Sn9 Cs3 90.84(3) 7_455 15_665
Cs3 Sn9 Cs3 119.518(19) 5_545 15_665
Sn11 Sn9 Cs3 67.66(3) 4_465 13_576
Sn11 Sn9 Cs3 78.22(3) 10_455 13_576
Sn11 Sn9 Cs3 66.58(3) 3_545 13_576
Sn11 Sn9 Cs3 169.03(2) 9_665 13_576
Cs3 Sn9 Cs3 119.518(19) 7_455 13_576
Cs3 Sn9 Cs3 90.84(3) 5_545 13_576
Cs3 Sn9 Cs3 119.518(18) 15_665 13_576
Sn4 Sn10 Sn15 108.12(4) . 15_665
Sn4 Sn10 Sn15 108.12(4) . 2_665
Sn15 Sn10 Sn15 108.28(7) 15_665 2_665
Sn4 Sn10 Sn2 105.00(6) . .
Sn15 Sn10 Sn2 113.52(4) 15_665 .
Sn15 Sn10 Sn2 113.52(4) 2_665 .
Sn4 Sn10 Cs4 65.06(3) . 15_665
Sn15 Sn10 Cs4 75.43(3) 15_665 15_665
Sn15 Sn10 Cs4 173.16(6) 2_665 15_665
Sn2 Sn10 Cs4 69.08(3) . 15_665
Sn4 Sn10 Cs4 65.06(3) . 9_665
Sn15 Sn10 Cs4 173.16(6) 15_665 9_665
Sn15 Sn10 Cs4 75.43(3) 2_665 9_665
Sn2 Sn10 Cs4 69.08(3) . 9_665
Cs4 Sn10 Cs4 100.29(4) 15_665 9_665
Sn4 Sn10 Na1 135.9(4) . 11_566
Sn15 Sn10 Na1 55.34(7) 15_665 11_566
Sn15 Sn10 Na1 55.34(7) 2_665 11_566
Sn2 Sn10 Na1 119.1(4) . 11_566
Cs4 Sn10 Na1 129.69(3) 15_665 11_566
Cs4 Sn10 Na1 129.69(3) 9_665 11_566
Sn4 Sn10 Cs2 167.35(6) . .
Sn15 Sn10 Cs2 78.77(4) 15_665 .
Sn15 Sn10 Cs2 78.77(4) 2_665 .
Sn2 Sn10 Cs2 62.36(5) . .
Cs4 Sn10 Cs2 107.80(3) 15_665 .
Cs4 Sn10 Cs2 107.80(3) 9_665 .
Na1 Sn10 Cs2 56.7(4) 11_566 .
Sn4 Sn10 Cs1 73.16(5) . 3_545
Sn15 Sn10 Cs1 67.35(4) 15_665 3_545
Sn15 Sn10 Cs1 67.35(4) 2_665 3_545
Sn2 Sn10 Cs1 178.16(7) . 3_545
Cs4 Sn10 Cs1 109.86(4) 15_665 3_545
Cs4 Sn10 Cs1 109.86(4) 9_665 3_545
Na1 Sn10 Cs1 62.8(4) 11_566 3_545
Cs2 Sn10 Cs1 119.48(6) . 3_545
Sn1 Sn11 Sn7 105.17(4) 10 10
Sn1 Sn11 Sn9 107.56(4) 10 9_665
Sn7 Sn11 Sn9 106.36(4) 10 9_665
Sn1 Sn11 Sn11 105.43(3) 10 10
Sn7 Sn11 Sn11 107.35(3) 10 10
Sn9 Sn11 Sn11 123.635(19) 9_665 10
Sn1 Sn11 Cs4 66.75(3) 10 .
Sn7 Sn11 Cs4 66.24(3) 10 .
Sn9 Sn11 Cs4 167.62(3) 9_665 .
Sn11 Sn11 Cs4 68.722(15) 10 .
Sn1 Sn11 Cs3 174.06(4) 10 15_765
Sn7 Sn11 Cs3 79.64(4) 10 15_765
Sn9 Sn11 Cs3 73.88(3) 9_665 15_765
Sn11 Sn11 Cs3 69.473(16) 10 15_765
Cs4 Sn11 Cs3 112.96(4) . 15_765
Sn1 Sn11 Cs3 79.48(4) 10 7
Sn7 Sn11 Cs3 175.17(4) 10 7
Sn9 Sn11 Cs3 73.02(3) 9_665 7
Sn11 Sn11 Cs3 69.738(16) 10 7
Cs4 Sn11 Cs3 115.23(4) . 7
Cs3 Sn11 Cs3 95.64(4) 15_765 7
Sn1 Sn11 Cs3 69.45(4) 10 13_675
Sn7 Sn11 Cs3 68.47(4) 10 13_675
Sn9 Sn11 Cs3 64.91(3) 9_665 13_675
Sn11 Sn11 Cs3 171.44(2) 10 13_675
Cs4 Sn11 Cs3 102.74(3) . 13_675
Cs3 Sn11 Cs3 115.98(3) 15_765 13_675
Cs3 Sn11 Cs3 114.94(3) 7 13_675
Sn14 Sn12 Sn6 114.80(7) 11_666 .
Sn14 Sn12 Sn4 107.38(7) 11_666 2_665
Sn6 Sn12 Sn4 103.71(5) . 2_665
Sn14 Sn12 Sn5 117.34(7) 11_666 .
Sn6 Sn12 Sn5 107.07(5) . .
Sn4 Sn12 Sn5 105.27(5) 2_665 .
Sn14 Sn12 Na2 24.7(8) 11_666 11_666
Sn6 Sn12 Na2 92.4(7) . 11_666
Sn4 Sn12 Na2 125.8(9) 2_665 11_666
Sn5 Sn12 Na2 118.9(7) . 11_666
Sn14 Sn12 Cs5 75.04(6) 11_666 3_554
Sn6 Sn12 Cs5 168.66(4) . 3_554
Sn4 Sn12 Cs5 66.79(3) 2_665 3_554
Sn5 Sn12 Cs5 71.08(3) . 3_554
Na2 Sn12 Cs5 98.2(7) 11_666 3_554
Sn14 Sn12 Cs4 172.18(7) 11_666 .
Sn6 Sn12 Cs4 68.93(3) . .
Sn4 Sn12 Cs4 64.81(4) 2_665 .
Sn5 Sn12 Cs4 66.28(4) . .
Na2 Sn12 Cs4 161.0(8) 11_666 .
Cs5 Sn12 Cs4 100.62(3) 3_554 .
Sn14 Sn12 Cs2 79.33(7) 11_666 11_666
Sn6 Sn12 Cs2 78.84(4) . 11_666
Sn4 Sn12 Cs2 170.45(5) 2_665 11_666
Sn5 Sn12 Cs2 65.28(4) . 11_666
Na2 Sn12 Cs2 62.8(9) 11_666 11_666
Cs5 Sn12 Cs2 109.52(3) 3_554 11_666
Cs4 Sn12 Cs2 108.38(4) . 11_666
Sn14 Sn12 Cs1 66.57(7) 11_666 11_676
Sn6 Sn12 Cs1 69.74(4) . 11_676
Sn4 Sn12 Cs1 73.60(4) 2_665 11_676
Sn5 Sn12 Cs1 176.00(6) . 11_676
Na2 Sn12 Cs1 64.2(7) 11_666 11_676
Cs5 Sn12 Cs1 111.54(3) 3_554 11_676
Cs4 Sn12 Cs1 109.95(5) . 11_676
Cs2 Sn12 Cs1 115.73(4) 11_666 11_676
Sn14 Sn12 Na2 34.8(4) 11_666 4
Sn6 Sn12 Na2 80.1(4) . 4
Sn4 Sn12 Na2 120.9(6) 2_665 4
Sn5 Sn12 Na2 130.4(5) . 4
Na2 Sn12 Na2 14.8(8) 11_666 4
Cs5 Sn12 Na2 109.9(4) 3_554 4
Cs4 Sn12 Na2 148.7(3) . 4
Cs2 Sn12 Na2 68.5(6) 11_666 4
Cs1 Sn12 Na2 52.2(4) 11_676 4
Sn14 Sn12 Na2 36.0(4) 11_666 12_666
Sn6 Sn12 Na2 117.0(5) . 12_666
Sn4 Sn12 Na2 72.2(4) 2_665 12_666
Sn5 Sn12 Na2 135.3(4) . 12_666
Na2 Sn12 Na2 54.6(13) 11_666 12_666
Cs5 Sn12 Na2 67.1(5) 3_554 12_666
Cs4 Sn12 Na2 136.4(4) . 12_666
Cs2 Sn12 Na2 115.2(4) 11_666 12_666
Cs1 Sn12 Na2 48.3(4) 11_676 12_666
Na2 Sn12 Na2 55.6(10) 4 12_666
Sn17 Sn13 Sn1 113.74(9) . 9_665
Sn17 Sn13 Sn1 113.74(9) . 2_665
Sn1 Sn13 Sn1 100.05(7) 9_665 2_665
Sn17 Sn13 Sn5 127.53(16) . 9_665
Sn1 Sn13 Sn5 98.74(5) 9_665 9_665
Sn1 Sn13 Sn5 98.74(5) 2_665 9_665
Sn17 Sn13 Na1 19.3(4) . .
Sn1 Sn13 Na1 123.04(15) 9_665 .
Sn1 Sn13 Na1 123.04(15) 2_665 .
Sn5 Sn13 Na1 108.3(4) 9_665 .
Sn17 Sn13 Cs2 78.08(10) . 12_666
Sn1 Sn13 Cs2 167.19(7) 9_665 12_666
Sn1 Sn13 Cs2 78.42(3) 2_665 12_666
Sn5 Sn13 Cs2 69.16(5) 9_665 12_666
Na1 Sn13 Cs2 66.7(2) . 12_666
Sn17 Sn13 Cs2 78.08(10) . 3_554
Sn1 Sn13 Cs2 78.42(3) 9_665 3_554
Sn1 Sn13 Cs2 167.19(7) 2_665 3_554
Sn5 Sn13 Cs2 69.16(5) 9_665 3_554
Na1 Sn13 Cs2 66.7(2) . 3_554
Cs2 Sn13 Cs2 100.20(6) 12_666 3_554
Sn17 Sn13 Cs4 170.69(15) . 9_665
Sn1 Sn13 Cs4 61.43(4) 9_665 9_665
Sn1 Sn13 Cs4 61.43(4) 2_665 9_665
Sn5 Sn13 Cs4 61.78(4) 9_665 9_665
Na1 Sn13 Cs4 170.0(4) . 9_665
Cs2 Sn13 Cs4 107.58(5) 12_666 9_665
Cs2 Sn13 Cs4 107.58(5) 3_554 9_665
Sn17 Sn13 Cs3 71.62(15) . 15_665
Sn1 Sn13 Cs3 69.62(4) 9_665 15_665
Sn1 Sn13 Cs3 69.62(4) 2_665 15_665
Sn5 Sn13 Cs3 160.85(7) 9_665 15_665
Na1 Sn13 Cs3 90.9(4) . 15_665
Cs2 Sn13 Cs3 120.74(4) 12_666 15_665
Cs2 Sn13 Cs3 120.74(4) 3_554 15_665
Cs4 Sn13 Cs3 99.08(5) 9_665 15_665
Na2 Sn14 Sn14 133(2) . 2
Na2 Sn14 Sn16 3(2) . .
Sn14 Sn14 Sn16 129.97(9) 2 .
Na2 Sn14 Sn12 100.5(14) . 6_455
Sn14 Sn14 Sn12 109.40(6) 2 6_455
Sn16 Sn14 Sn12 102.75(9) . 6_455
Na2 Sn14 Sn12 100.5(14) . 12_656
Sn14 Sn14 Sn12 109.40(6) 2 12_656
Sn16 Sn14 Sn12 102.75(9) . 12_656
Sn12 Sn14 Sn12 97.92(11) 6_455 12_656
Na2 Sn14 Na2 26.1(19) . 10
Sn14 Sn14 Na2 107.4(9) 2 10
Sn16 Sn14 Na2 22.6(9) . 10
Sn12 Sn14 Na2 116.2(5) 6_455 10
Sn12 Sn14 Na2 116.2(5) 12_656 10
Na2 Sn14 Na2 117(3) . 2
Sn14 Sn14 Na2 15.9(8) 2 2
Sn16 Sn14 Na2 114.0(8) . 2
Sn12 Sn14 Na2 118.3(4) 6_455 2
Sn12 Sn14 Na2 118.3(4) 12_656 2
Na2 Sn14 Na2 91.4(12) 10 2
Na2 Sn14 Cs5 155(2) . .
Sn14 Sn14 Cs5 71.35(4) 2 .
Sn16 Sn14 Cs5 158.67(12) . .
Sn12 Sn14 Cs5 64.50(6) 6_455 .
Sn12 Sn14 Cs5 64.50(6) 12_656 .
Na2 Sn14 Cs5 178.7(10) 10 .
Na2 Sn14 Cs5 87.3(8) 2 .
Na2 Sn14 Cs1 81.8(12) . 9_655
Sn14 Sn14 Cs1 71.85(4) 2 9_655
Sn16 Sn14 Cs1 79.89(6) . 9_655
Sn12 Sn14 Cs1 76.53(4) 6_455 9_655
Sn12 Sn14 Cs1 174.32(9) 12_656 9_655
Na2 Sn14 Cs1 68.0(5) 10 9_655
Na2 Sn14 Cs1 64.3(4) 2 9_655
Cs5 Sn14 Cs1 111.40(5) . 9_655
Na2 Sn14 Cs1 81.8(12) . 1_455
Sn14 Sn14 Cs1 71.85(4) 2 1_455
Sn16 Sn14 Cs1 79.89(6) . 1_455
Sn12 Sn14 Cs1 174.32(9) 6_455 1_455
Sn12 Sn14 Cs1 76.53(4) 12_656 1_455
Na2 Sn14 Cs1 68.0(5) 10 1_455
Na2 Sn14 Cs1 64.3(4) 2 1_455
Cs5 Sn14 Cs1 111.40(5) . 1_455
Cs1 Sn14 Cs1 108.99(9) 9_655 1_455
Na2 Sn14 Cs2 57(2) . .
Sn14 Sn14 Cs2 169.60(5) 2 .
Sn16 Sn14 Cs2 60.43(9) . .
Sn12 Sn14 Cs2 64.60(6) 6_455 .
Sn12 Sn14 Cs2 64.60(6) 12_656 .
Na2 Sn14 Cs2 83.0(9) 10 .
Na2 Sn14 Cs2 174.5(8) 2 .
Cs5 Sn14 Cs2 98.24(7) . .
Cs1 Sn14 Cs2 113.26(5) 9_655 .
Cs1 Sn14 Cs2 113.26(5) 1_455 .
Na2 Sn14 Na2 93(2) . 9
Sn14 Sn14 Na2 40.8(7) 2 9
Sn16 Sn14 Na2 89.2(7) . 9
Sn12 Sn14 Na2 128.43(19) 6_455 9
Sn12 Sn14 Na2 128.43(19) 12_656 9
Na2 Sn14 Na2 66.6(15) 10 9
Na2 Sn14 Na2 24.9(13) 2 9
Cs5 Sn14 Na2 112.2(7) . 9
Cs1 Sn14 Na2 56.21(14) 9_655 9
Cs1 Sn14 Na2 56.21(14) 1_455 9
Cs2 Sn14 Na2 149.6(7) . 9
Sn17 Sn15 Sn10 99.42(13) 3_655 2_665
Sn17 Sn15 Sn7 112.74(14) 3_655 .
Sn10 Sn15 Sn7 99.09(5) 2_665 .
Sn17 Sn15 Sn6 134.61(12) 3_655 .
Sn10 Sn15 Sn6 104.12(5) 2_665 .
Sn7 Sn15 Sn6 101.20(5) . .
Sn17 Sn15 Na1 18.43(19) 3_655 3_655
Sn10 Sn15 Na1 81.08(10) 2_665 3_655
Sn7 Sn15 Na1 117.8(4) . 3_655
Sn6 Sn15 Na1 139.5(4) . 3_655
Sn17 Sn15 Cs3 86.76(13) 3_655 13_676
Sn10 Sn15 Cs3 173.45(6) 2_665 13_676
Sn7 Sn15 Cs3 80.33(4) . 13_676
Sn6 Sn15 Cs3 69.73(4) . 13_676
Na1 Sn15 Cs3 105.01(8) 3_655 13_676
Sn17 Sn15 Cs4 159.82(12) 3_655 .
Sn10 Sn15 Cs4 64.51(4) 2_665 .
Sn7 Sn15 Cs4 61.36(4) . .
Sn6 Sn15 Cs4 64.25(4) . .
Na1 Sn15 Cs4 143.98(5) 3_655 .
Cs3 Sn15 Cs4 109.91(4) 13_676 .
Sn17 Sn15 Cs1 76.78(14) 3_655 11_676
Sn10 Sn15 Cs1 75.41(4) 2_665 11_676
Sn7 Sn15 Cs1 169.93(6) . 11_676
Sn6 Sn15 Cs1 72.50(5) . 11_676
Na1 Sn15 Cs1 70.1(4) 3_655 11_676
Cs3 Sn15 Cs1 104.15(4) 13_676 11_676
Cs4 Sn15 Cs1 108.58(4) . 11_676
Sn17 Sn15 Cs2 63.30(11) 3_655 2_665
Sn10 Sn15 Cs2 66.27(4) 2_665 2_665
Sn7 Sn15 Cs2 67.00(4) . 2_665
Sn6 Sn15 Cs2 162.02(5) . 2_665
Na1 Sn15 Cs2 56.4(3) 3_655 2_665
Cs3 Sn15 Cs2 118.98(5) 13_676 2_665
Cs4 Sn15 Cs2 97.79(4) . 2_665
Cs1 Sn15 Cs2 116.98(4) 11_676 2_665
Na2 Sn16 Na2 108(5) 10 .
Na2 Sn16 Sn14 4(2) 10 10
Na2 Sn16 Sn14 104(2) . 10
Na2 Sn16 Sn14 104(2) 10 .
Na2 Sn16 Sn14 4(2) . .
Sn14 Sn16 Sn14 100.06(18) 10 .
Na2 Sn16 Sn8 106.4(10) 10 .
Na2 Sn16 Sn8 106.4(10) . .
Sn14 Sn16 Sn8 107.90(3) 10 .
Sn14 Sn16 Sn8 107.90(3) . .
Na2 Sn16 Sn8 106.4(10) 10 7
Na2 Sn16 Sn8 106.4(10) . 7
Sn14 Sn16 Sn8 107.90(3) 10 7
Sn14 Sn16 Sn8 107.90(3) . 7
Sn8 Sn16 Sn8 122.84(15) . 7
Na2 Sn16 Cs2 172(2) 10 .
Na2 Sn16 Cs2 80(2) . .
Sn14 Sn16 Cs2 175.99(13) 10 .
Sn14 Sn16 Cs2 83.95(8) . .
Sn8 Sn16 Cs2 70.60(6) . .
Sn8 Sn16 Cs2 70.60(6) 7 .
Na2 Sn16 Cs2 80(2) 10 10
Na2 Sn16 Cs2 172(2) . 10
Sn14 Sn16 Cs2 83.95(8) 10 10
Sn14 Sn16 Cs2 175.99(13) . 10
Sn8 Sn16 Cs2 70.60(6) . 10
Sn8 Sn16 Cs2 70.60(6) 7 10
Cs2 Sn16 Cs2 92.05(10) . 10
Na2 Sn16 Cs1 66.9(14) 10 9_655
Na2 Sn16 Cs1 66.9(14) . 9_655
Sn14 Sn16 Cs1 64.76(7) 10 9_655
Sn14 Sn16 Cs1 64.76(7) . 9_655
Sn8 Sn16 Cs1 166.99(11) . 9_655
Sn8 Sn16 Cs1 70.16(5) 7 9_655
Cs2 Sn16 Cs1 117.44(2) . 9_655
Cs2 Sn16 Cs1 117.44(2) 10 9_655
Na2 Sn16 Cs1 66.9(14) 10 1_455
Na2 Sn16 Cs1 66.9(14) . 1_455
Sn14 Sn16 Cs1 64.76(7) 10 1_455
Sn14 Sn16 Cs1 64.76(7) . 1_455
Sn8 Sn16 Cs1 70.16(5) . 1_455
Sn8 Sn16 Cs1 166.99(11) 7 1_455
Cs2 Sn16 Cs1 117.44(2) . 1_455
Cs2 Sn16 Cs1 117.44(2) 10 1_455
Cs1 Sn16 Cs1 96.83(9) 9_655 1_455
Na2 Sn16 Na2 43(2) 10 9
Na2 Sn16 Na2 65(3) . 9
Sn14 Sn16 Na2 39.0(6) 10 9
Sn14 Sn16 Na2 61.1(6) . 9
Sn8 Sn16 Na2 118.00(9) . 9
Sn8 Sn16 Na2 118.00(9) 7 9
Cs2 Sn16 Na2 145.0(6) . 9
Cs2 Sn16 Na2 122.9(6) 10 9
Cs1 Sn16 Na2 49.35(11) 9_655 9
Cs1 Sn16 Na2 49.35(11) 1_455 9
Na2 Sn16 Na2 65(3) 10 2
Na2 Sn16 Na2 43(2) . 2
Sn14 Sn16 Na2 61.1(6) 10 2
Sn14 Sn16 Na2 39.0(6) . 2
Sn8 Sn16 Na2 118.00(9) . 2
Sn8 Sn16 Na2 118.00(9) 7 2
Cs2 Sn16 Na2 122.9(6) . 2
Cs2 Sn16 Na2 145.0(6) 10 2
Cs1 Sn16 Na2 49.35(11) 9_655 2
Cs1 Sn16 Na2 49.35(11) 1_455 2
Na2 Sn16 Na2 22.1(11) 9 2
Na1 Sn17 Sn17 6.4(13) . 15_665
Na1 Sn17 Sn15 117.8(7) . 4_464
Sn17 Sn17 Sn15 114.48(13) 15_665 4_464
Na1 Sn17 Sn15 117.8(7) . 11_576
Sn17 Sn17 Sn15 114.48(13) 15_665 11_576
Sn15 Sn17 Sn15 99.7(2) 4_464 11_576
Na1 Sn17 Sn13 113.3(14) . .
Sn17 Sn17 Sn13 119.64(15) 15_665 .
Sn15 Sn17 Sn13 102.96(17) 4_464 .
Sn15 Sn17 Sn13 102.96(17) 11_576 .
Na1 Sn17 Cs2 69.8(9) . 12_666
Sn17 Sn17 Cs2 74.00(8) 15_665 12_666
Sn15 Sn17 Cs2 167.6(2) 4_464 12_666
Sn15 Sn17 Cs2 83.89(6) 11_576 12_666
Sn13 Sn17 Cs2 64.64(10) . 12_666
Na1 Sn17 Cs2 69.8(9) . 3_554
Sn17 Sn17 Cs2 74.00(8) 15_665 3_554
Sn15 Sn17 Cs2 83.89(6) 4_464 3_554
Sn15 Sn17 Cs2 167.6(2) 11_576 3_554
Sn13 Sn17 Cs2 64.64(10) . 3_554
Cs2 Sn17 Cs2 90.23(13) 12_666 3_554
Na1 Sn17 Cs1 80.9(13) . 9_665
Sn17 Sn17 Cs1 74.59(8) 15_665 9_665
Sn15 Sn17 Cs1 68.53(13) 4_464 9_665
Sn15 Sn17 Cs1 68.53(13) 11_576 9_665
Sn13 Sn17 Cs1 165.8(2) . 9_665
Cs2 Sn17 Cs1 123.58(10) 12_666 9_665
Cs2 Sn17 Cs1 123.58(10) 3_554 9_665
Na1 Sn17 Cs3 172.0(14) . 15_665
Sn17 Sn17 Cs3 165.63(8) 15_665 15_665
Sn15 Sn17 Cs3 58.40(13) 4_464 15_665
Sn15 Sn17 Cs3 58.40(13) 11_576 15_665
Sn13 Sn17 Cs3 74.73(15) . 15_665
Cs2 Sn17 Cs3 115.36(10) 12_666 15_665
Cs2 Sn17 Cs3 115.36(10) 3_554 15_665
Cs1 Sn17 Cs3 91.03(12) 9_665 15_665
Sn17 Na1 Sn17 167(3) 15_665 .
Sn17 Na1 Sn13 47.4(10) 15_665 15_665
Sn17 Na1 Sn13 145.3(17) . 15_665
Sn17 Na1 Sn13 145.3(17) 15_665 .
Sn17 Na1 Sn13 47.4(10) . .
Sn13 Na1 Sn13 97.8(7) 15_665 .
Sn17 Na1 Sn15 43.8(5) 15_665 6_465
Sn17 Na1 Sn15 128.9(11) . 6_465
Sn13 Na1 Sn15 76.58(9) 15_665 6_465
Sn13 Na1 Sn15 142.4(3) . 6_465
Sn17 Na1 Sn15 128.9(11) 15_665 4_464
Sn17 Na1 Sn15 43.8(5) . 4_464
Sn13 Na1 Sn15 142.4(3) 15_665 4_464
Sn13 Na1 Sn15 76.58(9) . 4_464
Sn15 Na1 Sn15 129.6(8) 6_465 4_464
Sn17 Na1 Sn15 43.8(5) 15_665 13_575
Sn17 Na1 Sn15 128.9(11) . 13_575
Sn13 Na1 Sn15 76.58(9) 15_665 13_575
Sn13 Na1 Sn15 142.4(3) . 13_575
Sn15 Na1 Sn15 73.4(3) 6_465 13_575
Sn15 Na1 Sn15 85.6(4) 4_464 13_575
Sn17 Na1 Sn15 128.9(11) 15_665 11_576
Sn17 Na1 Sn15 43.8(5) . 11_576
Sn13 Na1 Sn15 142.4(3) 15_665 11_576
Sn13 Na1 Sn15 76.58(9) . 11_576
Sn15 Na1 Sn15 85.6(4) 6_465 11_576
Sn15 Na1 Sn15 73.4(3) 4_464 11_576
Sn15 Na1 Sn15 129.6(8) 13_575 11_576
Sn17 Na1 Sn10 87.2(6) 15_665 12_666
Sn17 Na1 Sn10 87.2(6) . 12_666
Sn13 Na1 Sn10 106.90(9) 15_665 12_666
Sn13 Na1 Sn10 106.90(9) . 12_666
Sn15 Na1 Sn10 43.58(15) 6_465 12_666
Sn15 Na1 Sn10 110.4(5) 4_464 12_666
Sn15 Na1 Sn10 110.4(5) 13_575 12_666
Sn15 Na1 Sn10 43.58(15) 11_576 12_666
Sn17 Na1 Sn10 87.2(6) 15_665 3_554
Sn17 Na1 Sn10 87.2(6) . 3_554
Sn13 Na1 Sn10 106.90(9) 15_665 3_554
Sn13 Na1 Sn10 106.90(9) . 3_554
Sn15 Na1 Sn10 110.4(5) 6_465 3_554
Sn15 Na1 Sn10 43.58(15) 4_464 3_554
Sn15 Na1 Sn10 43.58(15) 13_575 3_554
Sn15 Na1 Sn10 110.4(5) 11_576 3_554
Sn10 Na1 Sn10 127.5(7) 12_666 3_554
Sn17 Na1 Cs2 94.2(9) 15_665 12_666
Sn17 Na1 Cs2 94.2(9) . 12_666
Sn13 Na1 Cs2 64.4(4) 15_665 12_666
Sn13 Na1 Cs2 64.4(4) . 12_666
Sn15 Na1 Cs2 80.21(14) 6_465 12_666
Sn15 Na1 Cs2 136.9(3) 4_464 12_666
Sn15 Na1 Cs2 136.9(3) 13_575 12_666
Sn15 Na1 Cs2 80.21(14) 11_576 12_666
Sn10 Na1 Cs2 67.38(7) 12_666 12_666
Sn10 Na1 Cs2 165.1(6) 3_554 12_666
Sn17 Na1 Cs2 94.2(9) 15_665 3_554
Sn17 Na1 Cs2 94.2(9) . 3_554
Sn13 Na1 Cs2 64.4(4) 15_665 3_554
Sn13 Na1 Cs2 64.4(4) . 3_554
Sn15 Na1 Cs2 136.9(3) 6_465 3_554
Sn15 Na1 Cs2 80.21(14) 4_464 3_554
Sn15 Na1 Cs2 80.21(14) 13_575 3_554
Sn15 Na1 Cs2 136.9(3) 11_576 3_554
Sn10 Na1 Cs2 165.1(6) 12_666 3_554
Sn10 Na1 Cs2 67.38(7) 3_554 3_554
Cs2 Na1 Cs2 97.7(6) 12_666 3_554
Sn17 Na1 Cs1 83.6(13) 15_665 9_665
Sn17 Na1 Cs1 83.6(13) . 9_665
Sn13 Na1 Cs1 131.1(4) 15_665 9_665
Sn13 Na1 Cs1 131.1(4) . 9_665
Sn15 Na1 Cs1 64.8(4) 6_465 9_665
Sn15 Na1 Cs1 64.8(4) 4_464 9_665
Sn15 Na1 Cs1 64.8(4) 13_575 9_665
Sn15 Na1 Cs1 64.8(4) 11_576 9_665
Sn10 Na1 Cs1 63.8(3) 12_666 9_665
Sn10 Na1 Cs1 63.8(3) 3_554 9_665
Cs2 Na1 Cs1 131.1(3) 12_666 9_665
Cs2 Na1 Cs1 131.1(3) 3_554 9_665
Sn17 Na1 Sn5 112.7(14) 15_665 9_665
Sn17 Na1 Sn5 80.0(13) . 9_665
Sn13 Na1 Sn5 65.3(4) 15_665 9_665
Sn13 Na1 Sn5 32.6(3) . 9_665
Sn15 Na1 Sn5 126.8(5) 6_465 9_665
Sn15 Na1 Sn5 102.6(3) 4_464 9_665
Sn15 Na1 Sn5 126.8(5) 13_575 9_665
Sn15 Na1 Sn5 102.6(3) 11_576 9_665
Sn10 Na1 Sn5 115.1(3) 12_666 9_665
Sn10 Na1 Sn5 115.1(3) 3_554 9_665
Cs2 Na1 Sn5 50.9(3) 12_666 9_665
Cs2 Na1 Sn5 50.9(3) 3_554 9_665
Cs1 Na1 Sn5 163.66(9) 9_665 9_665
Sn17 Na1 Sn5 80.0(13) 15_665 7
Sn17 Na1 Sn5 112.7(14) . 7
Sn13 Na1 Sn5 32.6(3) 15_665 7
Sn13 Na1 Sn5 65.3(4) . 7
Sn15 Na1 Sn5 102.6(3) 6_465 7
Sn15 Na1 Sn5 126.8(5) 4_464 7
Sn15 Na1 Sn5 102.6(3) 13_575 7
Sn15 Na1 Sn5 126.8(5) 11_576 7
Sn10 Na1 Sn5 115.1(3) 12_666 7
Sn10 Na1 Sn5 115.1(3) 3_554 7
Cs2 Na1 Sn5 50.9(3) 12_666 7
Cs2 Na1 Sn5 50.9(3) 3_554 7
Cs1 Na1 Sn5 163.66(9) 9_665 7
Sn5 Na1 Sn5 32.68(18) 9_665 7
Sn17 Na1 Sn7 135.48(9) 15_665 4_464
Sn17 Na1 Sn7 45.36(18) . 4_464
Sn13 Na1 Sn7 120.4(4) 15_665 4_464
Sn13 Na1 Sn7 55.41(4) . 4_464
Sn15 Na1 Sn7 157.3(7) 6_465 4_464
Sn15 Na1 Sn7 28.07(13) 4_464 4_464
Sn15 Na1 Sn7 94.89(12) 13_575 4_464
Sn15 Na1 Sn7 87.41(10) 11_576 4_464
Sn10 Na1 Sn7 130.5(3) 12_666 4_464
Sn10 Na1 Sn7 52.60(3) 3_554 4_464
Cs2 Na1 Sn7 119.8(4) 12_666 4_464
Cs2 Na1 Sn7 56.05(8) 3_554 4_464
Cs1 Na1 Sn7 92.7(3) 9_665 4_464
Sn5 Na1 Sn7 75.8(2) 9_665 4_464
Sn5 Na1 Sn7 98.9(4) 7 4_464
Sn17 Na1 Sn7 45.36(18) 15_665 6_465
Sn17 Na1 Sn7 135.48(9) . 6_465
Sn13 Na1 Sn7 55.41(4) 15_665 6_465
Sn13 Na1 Sn7 120.4(4) . 6_465
Sn15 Na1 Sn7 28.07(13) 6_465 6_465
Sn15 Na1 Sn7 157.3(7) 4_464 6_465
Sn15 Na1 Sn7 87.41(10) 13_575 6_465
Sn15 Na1 Sn7 94.89(12) 11_576 6_465
Sn10 Na1 Sn7 52.60(3) 12_666 6_465
Sn10 Na1 Sn7 130.5(3) 3_554 6_465
Cs2 Na1 Sn7 56.05(8) 12_666 6_465
Cs2 Na1 Sn7 119.8(4) 3_554 6_465
Cs1 Na1 Sn7 92.7(3) 9_665 6_465
Sn5 Na1 Sn7 98.9(4) 9_665 6_465
Sn5 Na1 Sn7 75.8(2) 7 6_465
Sn7 Na1 Sn7 174.6(6) 4_464 6_465
Sn17 Na1 Sn7 45.36(18) 15_665 13_575
Sn17 Na1 Sn7 135.48(9) . 13_575
Sn13 Na1 Sn7 55.41(4) 15_665 13_575
Sn13 Na1 Sn7 120.4(4) . 13_575
Sn15 Na1 Sn7 87.41(10) 6_465 13_575
Sn15 Na1 Sn7 94.89(12) 4_464 13_575
Sn15 Na1 Sn7 28.07(13) 13_575 13_575
Sn15 Na1 Sn7 157.3(7) 11_576 13_575
Sn10 Na1 Sn7 130.5(3) 12_666 13_575
Sn10 Na1 Sn7 52.60(2) 3_554 13_575
Cs2 Na1 Sn7 119.8(4) 12_666 13_575
Cs2 Na1 Sn7 56.05(8) 3_554 13_575
Cs1 Na1 Sn7 92.7(3) 9_665 13_575
Sn5 Na1 Sn7 98.9(4) 9_665 13_575
Sn5 Na1 Sn7 75.8(2) 7 13_575
Sn7 Na1 Sn7 90.83(4) 4_464 13_575
Sn7 Na1 Sn7 88.92(3) 6_465 13_575
Sn17 Na1 Sn7 135.48(9) 15_665 11_576
Sn17 Na1 Sn7 45.36(18) . 11_576
Sn13 Na1 Sn7 120.4(4) 15_665 11_576
Sn13 Na1 Sn7 55.41(4) . 11_576
Sn15 Na1 Sn7 94.89(12) 6_465 11_576
Sn15 Na1 Sn7 87.41(10) 4_464 11_576
Sn15 Na1 Sn7 157.3(7) 13_575 11_576
Sn15 Na1 Sn7 28.07(13) 11_576 11_576
Sn10 Na1 Sn7 52.60(3) 12_666 11_576
Sn10 Na1 Sn7 130.5(3) 3_554 11_576
Cs2 Na1 Sn7 56.05(8) 12_666 11_576
Cs2 Na1 Sn7 119.8(4) 3_554 11_576
Cs1 Na1 Sn7 92.7(3) 9_665 11_576
Sn5 Na1 Sn7 75.8(2) 9_665 11_576
Sn5 Na1 Sn7 98.9(4) 7 11_576
Sn7 Na1 Sn7 88.92(3) 4_464 11_576
Sn7 Na1 Sn7 90.83(4) 6_465 11_576
Sn7 Na1 Sn7 174.6(6) 13_575 11_576
Sn17 Na1 Sn1 42.4(9) 15_665 16
Sn17 Na1 Sn1 147.2(11) . 16
Sn13 Na1 Sn1 25.93(2) 15_665 16
Sn13 Na1 Sn1 107.3(6) . 16
Sn15 Na1 Sn1 54.29(16) 6_465 16
Sn15 Na1 Sn1 166.73(11) 4_464 16
Sn15 Na1 Sn1 83.92(10) 13_575 16
Sn15 Na1 Sn1 119.70(7) 11_576 16
Sn10 Na1 Sn1 81.01(6) 12_666 16
Sn10 Na1 Sn1 124.11(4) 3_554 16
Cs2 Na1 Sn1 52.99(17) 12_666 16
Cs2 Na1 Sn1 90.0(4) 3_554 16
Cs1 Na1 Sn1 117.2(3) 9_665 16
Sn5 Na1 Sn1 77.6(3) 9_665 16
Sn5 Na1 Sn1 48.51(18) 7 16
Sn7 Na1 Sn1 145.5(5) 4_464 16
Sn7 Na1 Sn1 29.87(5) 6_465 16
Sn7 Na1 Sn1 72.10(11) 13_575 16
Sn7 Na1 Sn1 105.3(2) 11_576 16
Sn16 Na2 Sn14 173(5) . .
Sn16 Na2 Na2 36(2) . 10
Sn14 Na2 Na2 137(2) . 10
Sn16 Na2 Sn14 54(2) . 10
Sn14 Na2 Sn14 119(3) . 10
Na2 Na2 Sn14 17.4(9) 10 10
Sn16 Na2 Sn12 129.7(19) . 6_455
Sn14 Na2 Sn12 54.7(13) . 6_455
Na2 Na2 Sn12 141.2(6) 10 6_455
Sn14 Na2 Sn12 137.6(9) 10 6_455
Sn16 Na2 Sn12 129.7(19) . 12_656
Sn14 Na2 Sn12 54.7(13) . 12_656
Na2 Na2 Sn12 141.2(6) 10 12_656
Sn14 Na2 Sn12 137.6(9) 10 12_656
Sn12 Na2 Sn12 77.6(12) 6_455 12_656
Sn16 Na2 Sn8 52.3(10) . .
Sn14 Na2 Sn8 130.3(11) . .
Na2 Na2 Sn8 72.2(9) 10 .
Sn14 Na2 Sn8 83.8(11) 10 .
Sn12 Na2 Sn8 134.6(17) 6_455 .
Sn12 Na2 Sn8 78.2(6) 12_656 .
Sn16 Na2 Sn8 52.3(10) . 7
Sn14 Na2 Sn8 130.3(11) . 7
Na2 Na2 Sn8 72.2(9) 10 7
Sn14 Na2 Sn8 83.8(11) 10 7
Sn12 Na2 Sn8 78.2(6) 6_455 7
Sn12 Na2 Sn8 134.6(17) 12_656 7
Sn8 Na2 Sn8 92.8(13) . 7
Sn16 Na2 Sn14 142(3) . 2
Sn14 Na2 Sn14 30.6(15) . 2
Na2 Na2 Sn14 105.9(8) 10 2
Sn14 Na2 Sn14 88.6(12) 10 2
Sn12 Na2 Sn14 76.7(10) 6_455 2
Sn12 Na2 Sn14 76.7(10) 12_656 2
Sn8 Na2 Sn14 132.7(7) . 2
Sn8 Na2 Sn14 132.7(7) 7 2
Sn16 Na2 Cs2 81(2) . .
Sn14 Na2 Cs2 106(3) . .
Na2 Na2 Cs2 117.6(8) 10 .
Sn14 Na2 Cs2 135.0(16) 10 .
Sn12 Na2 Cs2 69.8(9) 6_455 .
Sn12 Na2 Cs2 69.8(9) 12_656 .
Sn8 Na2 Cs2 66.0(9) . .
Sn8 Na2 Cs2 66.0(9) 7 .
Sn14 Na2 Cs2 136.5(15) 2 .
Sn16 Na2 Cs1 96.9(16) . 9_655
Sn14 Na2 Cs1 78.9(14) . 9_655
Na2 Na2 Cs1 75.8(7) 10 9_655
Sn14 Na2 Cs1 66.8(7) 10 9_655
Sn12 Na2 Cs1 71.1(4) 6_455 9_655
Sn12 Na2 Cs1 133.4(15) 12_656 9_655
Sn8 Na2 Cs1 147.3(16) . 9_655
Sn8 Na2 Cs1 70.9(3) 7 9_655
Sn14 Na2 Cs1 63.3(7) 2 9_655
Cs2 Na2 Cs1 126.1(6) . 9_655
Sn16 Na2 Cs1 96.9(16) . 1_455
Sn14 Na2 Cs1 78.9(14) . 1_455
Na2 Na2 Cs1 75.8(7) 10 1_455
Sn14 Na2 Cs1 66.8(7) 10 1_455
Sn12 Na2 Cs1 133.4(15) 6_455 1_455
Sn12 Na2 Cs1 71.1(4) 12_656 1_455
Sn8 Na2 Cs1 70.9(3) . 1_455
Sn8 Na2 Cs1 147.3(16) 7 1_455
Sn14 Na2 Cs1 63.3(7) 2 1_455
Cs2 Na2 Cs1 126.1(6) . 1_455
Cs1 Na2 Cs1 107.6(12) 9_655 1_455
Sn16 Na2 Sn6 92.0(12) . 6_455
Sn14 Na2 Sn6 91.0(12) . 6_455
Na2 Na2 Sn6 106.0(7) 10 6_455
Sn14 Na2 Sn6 111.0(7) 10 6_455
Sn12 Na2 Sn6 38.9(2) 6_455 6_455
Sn12 Na2 Sn6 111.0(13) 12_656 6_455
Sn8 Na2 Sn6 123.0(14) . 6_455
Sn8 Na2 Sn6 39.8(2) 7 6_455
Sn14 Na2 Sn6 103.3(8) 2 6_455
Cs2 Na2 Sn6 65.8(6) . 6_455
Cs1 Na2 Sn6 60.46(8) 9_655 6_455
Cs1 Na2 Sn6 166.1(13) 1_455 6_455
Sn16 Na2 Sn6 92.0(12) . 12_656
Sn14 Na2 Sn6 91.0(12) . 12_656
Na2 Na2 Sn6 106.0(7) 10 12_656
Sn14 Na2 Sn6 111.0(7) 10 12_656
Sn12 Na2 Sn6 111.0(13) 6_455 12_656
Sn12 Na2 Sn6 38.9(2) 12_656 12_656
Sn8 Na2 Sn6 39.8(2) . 12_656
Sn8 Na2 Sn6 123.0(14) 7 12_656
Sn14 Na2 Sn6 103.3(8) 2 12_656
Cs2 Na2 Sn6 65.8(6) . 12_656
Cs1 Na2 Sn6 166.1(13) 9_655 12_656
Cs1 Na2 Sn6 60.46(8) 1_455 12_656
Sn6 Na2 Sn6 130.1(13) 6_455 12_656
Sn16 Na2 Na2 126(2) . 2
Sn14 Na2 Na2 47(2) . 2
Na2 Na2 Na2 90.002(2) 10 2
Sn14 Na2 Na2 72.6(9) 10 2
Sn12 Na2 Na2 89.0(9) 6_455 2
Sn12 Na2 Na2 89.0(9) 12_656 2
Sn8 Na2 Na2 128.2(7) . 2
Sn8 Na2 Na2 128.2(7) 7 2
Sn14 Na2 Na2 15.9(8) 2 2
Cs2 Na2 Na2 152.4(8) . 2
Cs1 Na2 Na2 57.5(6) 9_655 2
Cs1 Na2 Na2 57.5(6) 1_455 2
Sn6 Na2 Na2 108.6(7) 6_455 2
Sn6 Na2 Na2 108.6(7) 12_656 2
Sn16 Na2 Sn14 85(2) . 9
Sn14 Na2 Sn14 87(2) . 9
Na2 Na2 Sn14 49.2(7) 10 9
Sn14 Na2 Sn14 31.8(5) 10 9
Sn12 Na2 Sn14 119.8(11) 6_455 9
Sn12 Na2 Sn14 119.8(11) 12_656 9
Sn8 Na2 Sn14 105.5(11) . 9
Sn8 Na2 Sn14 105.5(11) 7 9
Sn14 Na2 Sn14 56.7(7) 2 9
Cs2 Na2 Sn14 166.8(14) . 9
Cs1 Na2 Sn14 55.5(6) 9_655 9
Cs1 Na2 Sn14 55.5(6) 1_455 9
Sn6 Na2 Sn14 115.0(6) 6_455 9
Sn6 Na2 Sn14 115.0(6) 12_656 9
Na2 Na2 Sn14 40.8(7) 2 9
Sn16 Na2 Na2 102(3) . 9
Sn14 Na2 Na2 71(2) . 9
Na2 Na2 Na2 65.5(12) 10 9
Sn14 Na2 Na2 48.2(9) 10 9
Sn12 Na2 Na2 107.9(14) 6_455 9
Sn12 Na2 Na2 107.9(14) 12_656 9
Sn8 Na2 Na2 115.8(13) . 9
Sn8 Na2 Na2 115.8(13) 7 9
Sn14 Na2 Na2 40.4(8) 2 9
Cs2 Na2 Na2 177(2) . 9
Cs1 Na2 Na2 53.8(6) 9_655 9
Cs1 Na2 Na2 53.8(6) 1_455 9
Sn6 Na2 Na2 113.9(7) 6_455 9
Sn6 Na2 Na2 113.9(7) 12_656 9
Na2 Na2 Na2 24.5(12) 2 9
Sn14 Na2 Na2 16.3(6) 9 9
Sn16 Na2 Sn12 43.0(16) . 3_544
Sn14 Na2 Sn12 131(2) . 3_544
Na2 Na2 Sn12 24.0(3) 10 3_544
Sn14 Na2 Sn12 29.0(4) 10 3_544
Sn12 Na2 Sn12 165.2(8) 6_455 3_544
Sn12 Na2 Sn12 117.2(3) 12_656 3_544
Sn8 Na2 Sn12 55.4(7) . 3_544
Sn8 Na2 Sn12 91.3(11) 7 3_544
Sn14 Na2 Sn12 103.9(11) 2 3_544
Cs2 Na2 Sn12 115.6(11) . 3_544
Cs1 Na2 Sn12 95.7(10) 9_655 3_544
Cs1 Na2 Sn12 56.1(5) 1_455 3_544
Sn6 Na2 Sn12 128.7(10) 6_455 3_544
Sn6 Na2 Sn12 83.5(5) 12_656 3_544
Na2 Na2 Sn12 89.4(6) 2 3_544
Sn14 Na2 Sn12 52.8(5) 9 3_544
Na2 Na2 Sn12 67.2(11) 9 3_544
Sn16 Na2 Sn12 43.0(16) . 13_565
Sn14 Na2 Sn12 131(2) . 13_565
Na2 Na2 Sn12 24.0(2) 10 13_565
Sn14 Na2 Sn12 29.0(4) 10 13_565
Sn12 Na2 Sn12 117.2(3) 6_455 13_565
Sn12 Na2 Sn12 165.2(8) 12_656 13_565
Sn8 Na2 Sn12 91.3(11) . 13_565
Sn8 Na2 Sn12 55.4(7) 7 13_565
Sn14 Na2 Sn12 103.9(11) 2 13_565
Cs2 Na2 Sn12 115.6(11) . 13_565
Cs1 Na2 Sn12 56.1(5) 9_655 13_565
Cs1 Na2 Sn12 95.7(10) 1_455 13_565
Sn6 Na2 Sn12 83.5(5) 6_455 13_565
Sn6 Na2 Sn12 128.7(10) 12_656 13_565
Na2 Na2 Sn12 89.4(6) 2 13_565
Sn14 Na2 Sn12 52.8(5) 9 13_565
Na2 Na2 Sn12 67.2(11) 9 13_565
Sn12 Na2 Sn12 48.0(5) 3_544 13_565
Sn16 Na2 Cs2 5.9(18) . 10
Sn14 Na2 Cs2 179(3) . 10
Na2 Na2 Cs2 42.1(6) 10 10
Sn14 Na2 Cs2 59.5(8) 10 10
Sn12 Na2 Cs2 126.1(10) 6_455 10
Sn12 Na2 Cs2 126.1(10) 12_656 10
Sn8 Na2 Cs2 50.1(7) . 10
Sn8 Na2 Cs2 50.1(7) 7 10
Sn14 Na2 Cs2 148.0(14) 2 10
Cs2 Na2 Cs2 75.5(8) . 10
Cs1 Na2 Cs2 100.3(8) 9_655 10
Cs1 Na2 Cs2 100.3(8) 1_455 10
Sn6 Na2 Cs2 89.5(7) 6_455 10
Sn6 Na2 Cs2 89.5(7) 12_656 10
Na2 Na2 Cs2 132.1(6) 2 10
Sn14 Na2 Cs2 91.3(9) 9 10
Na2 Na2 Cs2 107.6(15) 9 10
Sn12 Na2 Cs2 47.9(5) 3_544 10
Sn12 Na2 Cs2 47.9(5) 13_565 10
Sn14 Cs1 Sn14 71.01(9) 9_655 1_655
Sn14 Cs1 Sn14 36.29(8) 9_655 10_655
Sn14 Cs1 Sn14 58.71(9) 1_655 10_655
Sn14 Cs1 Sn14 58.71(9) 9_655 2_655
Sn14 Cs1 Sn14 36.29(8) 1_655 2_655
Sn14 Cs1 Sn14 71.01(9) 10_655 2_655
Sn14 Cs1 Na2 19.2(7) 9_655 9_655
Sn14 Cs1 Na2 68.3(6) 1_655 9_655
Sn14 Cs1 Na2 52.4(7) 10_655 9_655
Sn14 Cs1 Na2 45.2(7) 2_655 9_655
Sn14 Cs1 Na2 68.3(6) 9_655 1_655
Sn14 Cs1 Na2 19.2(7) 1_655 1_655
Sn14 Cs1 Na2 45.2(7) 10_655 1_655
Sn14 Cs1 Na2 52.4(7) 2_655 1_655
Na2 Cs1 Na2 72.4(12) 9_655 1_655
Sn14 Cs1 Na2 52.4(7) 9_655 10_655
Sn14 Cs1 Na2 45.2(7) 1_655 10_655
Sn14 Cs1 Na2 19.2(7) 10_655 10_655
Sn14 Cs1 Na2 68.3(6) 2_655 10_655
Na2 Cs1 Na2 65.0(12) 9_655 10_655
Na2 Cs1 Na2 28.3(14) 1_655 10_655
Sn14 Cs1 Na2 45.2(7) 9_655 2_655
Sn14 Cs1 Na2 52.4(7) 1_655 2_655
Sn14 Cs1 Na2 68.3(6) 10_655 2_655
Sn14 Cs1 Na2 19.2(7) 2_655 2_655
Na2 Cs1 Na2 28.3(14) 9_655 2_655
Na2 Cs1 Na2 65.0(12) 1_655 2_655
Na2 Cs1 Na2 72.4(12) 10_655 2_655
Sn14 Cs1 Sn15 100.39(4) 9_655 14_755
Sn14 Cs1 Sn15 165.87(6) 1_655 14_755
Sn14 Cs1 Sn15 120.75(4) 10_655 14_755
Sn14 Cs1 Sn15 129.70(4) 2_655 14_755
Na2 Cs1 Sn15 99.8(6) 9_655 14_755
Na2 Cs1 Sn15 165.9(7) 1_655 14_755
Na2 Cs1 Sn15 137.8(7) 10_655 14_755
Na2 Cs1 Sn15 113.5(7) 2_655 14_755
Sn14 Cs1 Sn15 165.87(6) 9_655 12_756
Sn14 Cs1 Sn15 100.39(4) 1_655 12_756
Sn14 Cs1 Sn15 129.70(4) 10_655 12_756
Sn14 Cs1 Sn15 120.75(4) 2_655 12_756
Na2 Cs1 Sn15 165.9(7) 9_655 12_756
Na2 Cs1 Sn15 99.8(6) 1_655 12_756
Na2 Cs1 Sn15 113.5(7) 10_655 12_756
Na2 Cs1 Sn15 137.8(7) 2_655 12_756
Sn15 Cs1 Sn15 90.12(8) 14_755 12_756
Sn14 Cs1 Sn15 129.70(4) 9_655 5_645
Sn14 Cs1 Sn15 120.75(4) 1_655 5_645
Sn14 Cs1 Sn15 165.87(6) 10_655 5_645
Sn14 Cs1 Sn15 100.39(4) 2_655 5_645
Na2 Cs1 Sn15 113.5(7) 9_655 5_645
Na2 Cs1 Sn15 137.8(7) 1_655 5_645
Na2 Cs1 Sn15 165.9(7) 10_655 5_645
Na2 Cs1 Sn15 99.8(6) 2_655 5_645
Sn15 Cs1 Sn15 55.76(5) 14_755 5_645
Sn15 Cs1 Sn15 64.20(5) 12_756 5_645
Sn14 Cs1 Sn15 120.75(4) 9_655 3_644
Sn14 Cs1 Sn15 129.70(4) 1_655 3_644
Sn14 Cs1 Sn15 100.39(4) 10_655 3_644
Sn14 Cs1 Sn15 165.87(6) 2_655 3_644
Na2 Cs1 Sn15 137.8(7) 9_655 3_644
Na2 Cs1 Sn15 113.5(7) 1_655 3_644
Na2 Cs1 Sn15 99.8(6) 10_655 3_644
Na2 Cs1 Sn15 165.9(7) 2_655 3_644
Sn15 Cs1 Sn15 64.20(5) 14_755 3_644
Sn15 Cs1 Sn15 55.76(5) 12_756 3_644
Sn15 Cs1 Sn15 90.12(8) 5_645 3_644
Sn14 Cs1 Sn6 65.82(4) 9_655 14_755
Sn14 Cs1 Sn6 128.65(8) 1_655 14_755
Sn14 Cs1 Sn6 96.72(6) 10_655 14_755
Sn14 Cs1 Sn6 95.62(6) 2_655 14_755
Na2 Cs1 Sn6 61.7(6) 9_655 14_755
Na2 Cs1 Sn6 133.4(6) 1_655 14_755
Na2 Cs1 Sn6 115.7(7) 10_655 14_755
Na2 Cs1 Sn6 77.2(7) 2_655 14_755
Sn15 Cs1 Sn6 38.32(3) 14_755 14_755
Sn15 Cs1 Sn6 126.73(8) 12_756 14_755
Sn15 Cs1 Sn6 72.52(4) 5_645 14_755
Sn15 Cs1 Sn6 96.54(5) 3_644 14_755
Sn14 Cs1 Sn6 128.65(8) 9_655 12_756
Sn14 Cs1 Sn6 65.82(4) 1_655 12_756
Sn14 Cs1 Sn6 95.62(6) 10_655 12_756
Sn14 Cs1 Sn6 96.72(6) 2_655 12_756
Na2 Cs1 Sn6 133.4(6) 9_655 12_756
Na2 Cs1 Sn6 61.7(6) 1_655 12_756
Na2 Cs1 Sn6 77.2(7) 10_655 12_756
Na2 Cs1 Sn6 115.7(7) 2_655 12_756
Sn15 Cs1 Sn6 126.73(8) 14_755 12_756
Sn15 Cs1 Sn6 38.32(3) 12_756 12_756
Sn15 Cs1 Sn6 96.54(5) 5_645 12_756
Sn15 Cs1 Sn6 72.52(4) 3_644 12_756
Sn6 Cs1 Sn6 164.83(10) 14_755 12_756
Sn14 Cs1 Sn6 95.62(6) 9_655 5_645
Sn14 Cs1 Sn6 96.72(6) 1_655 5_645
Sn14 Cs1 Sn6 128.65(8) 10_655 5_645
Sn14 Cs1 Sn6 65.82(4) 2_655 5_645
Na2 Cs1 Sn6 77.2(7) 9_655 5_645
Na2 Cs1 Sn6 115.7(7) 1_655 5_645
Na2 Cs1 Sn6 133.4(6) 10_655 5_645
Na2 Cs1 Sn6 61.7(6) 2_655 5_645
Sn15 Cs1 Sn6 72.52(4) 14_755 5_645
Sn15 Cs1 Sn6 96.54(5) 12_756 5_645
Sn15 Cs1 Sn6 38.32(3) 5_645 5_645
Sn15 Cs1 Sn6 126.73(8) 3_644 5_645
Sn6 Cs1 Sn6 62.36(3) 14_755 5_645
Sn6 Cs1 Sn6 115.41(3) 12_756 5_645
Sn14 Cs1 Sn6 96.72(6) 9_655 3_644
Sn14 Cs1 Sn6 95.62(6) 1_655 3_644
Sn14 Cs1 Sn6 65.82(4) 10_655 3_644
Sn14 Cs1 Sn6 128.65(8) 2_655 3_644
Na2 Cs1 Sn6 115.7(7) 9_655 3_644
Na2 Cs1 Sn6 77.2(7) 1_655 3_644
Na2 Cs1 Sn6 61.7(6) 10_655 3_644
Na2 Cs1 Sn6 133.4(6) 2_655 3_644
Sn15 Cs1 Sn6 96.54(5) 14_755 3_644
Sn15 Cs1 Sn6 72.52(4) 12_756 3_644
Sn15 Cs1 Sn6 126.73(8) 5_645 3_644
Sn15 Cs1 Sn6 38.32(3) 3_644 3_644
Sn6 Cs1 Sn6 115.41(3) 14_755 3_644
Sn6 Cs1 Sn6 62.36(3) 12_756 3_644
Sn6 Cs1 Sn6 164.83(10) 5_645 3_644
Sn14 Cs1 Na1 144.49(4) 9_655 9_665
Sn14 Cs1 Na1 144.49(4) 1_655 9_665
Sn14 Cs1 Na1 144.49(4) 10_655 9_665
Sn14 Cs1 Na1 144.49(4) 2_655 9_665
Na2 Cs1 Na1 143.8(6) 9_655 9_665
Na2 Cs1 Na1 143.8(6) 1_655 9_665
Na2 Cs1 Na1 143.8(6) 10_655 9_665
Na2 Cs1 Na1 143.8(6) 2_655 9_665
Sn15 Cs1 Na1 45.06(4) 14_755 9_665
Sn15 Cs1 Na1 45.06(4) 12_756 9_665
Sn15 Cs1 Na1 45.06(4) 5_645 9_665
Sn15 Cs1 Na1 45.06(4) 3_644 9_665
Sn6 Cs1 Na1 82.42(5) 14_755 9_665
Sn6 Cs1 Na1 82.42(5) 12_756 9_665
Sn6 Cs1 Na1 82.42(5) 5_645 9_665
Sn6 Cs1 Na1 82.42(5) 3_644 9_665
Sn14 Cs1 Sn12 36.90(4) 9_655 14_755
Sn14 Cs1 Sn12 107.90(8) 1_655 14_755
Sn14 Cs1 Sn12 60.73(5) 10_655 14_755
Sn14 Cs1 Sn12 89.81(7) 2_655 14_755
Na2 Cs1 Sn12 44.7(7) 9_655 14_755
Na2 Cs1 Sn12 102.9(6) 1_655 14_755
Na2 Cs1 Sn12 79.9(7) 10_655 14_755
Na2 Cs1 Sn12 71.7(7) 2_655 14_755
Sn15 Cs1 Sn12 64.45(2) 14_755 14_755
Sn15 Cs1 Sn12 149.15(7) 12_756 14_755
Sn15 Cs1 Sn12 109.16(3) 5_645 14_755
Sn15 Cs1 Sn12 95.68(3) 3_644 14_755
Sn6 Cs1 Sn12 36.652(19) 14_755 14_755
Sn6 Cs1 Sn12 151.90(4) 12_756 14_755
Sn6 Cs1 Sn12 92.22(2) 5_645 14_755
Sn6 Cs1 Sn12 92.36(2) 3_644 14_755
Na1 Cs1 Sn12 107.60(5) 9_665 14_755
Sn14 Cs1 Sn12 107.90(8) 9_655 12_756
Sn14 Cs1 Sn12 36.90(4) 1_655 12_756
Sn14 Cs1 Sn12 89.81(7) 10_655 12_756
Sn14 Cs1 Sn12 60.73(5) 2_655 12_756
Na2 Cs1 Sn12 102.9(6) 9_655 12_756
Na2 Cs1 Sn12 44.7(7) 1_655 12_756
Na2 Cs1 Sn12 71.7(7) 10_655 12_756
Na2 Cs1 Sn12 79.9(7) 2_655 12_756
Sn15 Cs1 Sn12 149.15(7) 14_755 12_756
Sn15 Cs1 Sn12 64.45(3) 12_756 12_756
Sn15 Cs1 Sn12 95.68(3) 5_645 12_756
Sn15 Cs1 Sn12 109.16(3) 3_644 12_756
Sn6 Cs1 Sn12 151.90(4) 14_755 12_756
Sn6 Cs1 Sn12 36.652(19) 12_756 12_756
Sn6 Cs1 Sn12 92.36(2) 5_645 12_756
Sn6 Cs1 Sn12 92.22(2) 3_644 12_756
Na1 Cs1 Sn12 107.60(5) 9_665 12_756
Sn12 Cs1 Sn12 144.80(9) 14_755 12_756
Sn14 Cs1 Sn12 89.81(7) 9_655 5_645
Sn14 Cs1 Sn12 60.73(5) 1_655 5_645
Sn14 Cs1 Sn12 107.90(8) 10_655 5_645
Sn14 Cs1 Sn12 36.90(4) 2_655 5_645
Na2 Cs1 Sn12 71.7(7) 9_655 5_645
Na2 Cs1 Sn12 79.9(7) 1_655 5_645
Na2 Cs1 Sn12 102.9(6) 10_655 5_645
Na2 Cs1 Sn12 44.7(7) 2_655 5_645
Sn15 Cs1 Sn12 109.16(3) 14_755 5_645
Sn15 Cs1 Sn12 95.68(3) 12_756 5_645
Sn15 Cs1 Sn12 64.45(2) 5_645 5_645
Sn15 Cs1 Sn12 149.15(7) 3_644 5_645
Sn6 Cs1 Sn12 92.22(2) 14_755 5_645
Sn6 Cs1 Sn12 92.36(2) 12_756 5_645
Sn6 Cs1 Sn12 36.652(19) 5_645 5_645
Sn6 Cs1 Sn12 151.90(4) 3_644 5_645
Na1 Cs1 Sn12 107.60(5) 9_665 5_645
Sn12 Cs1 Sn12 108.62(5) 14_755 5_645
Sn12 Cs1 Sn12 59.85(3) 12_756 5_645
Sn14 Cs1 Sn12 60.73(5) 9_655 3_644
Sn14 Cs1 Sn12 89.81(7) 1_655 3_644
Sn14 Cs1 Sn12 36.90(4) 10_655 3_644
Sn14 Cs1 Sn12 107.90(8) 2_655 3_644
Na2 Cs1 Sn12 79.9(7) 9_655 3_644
Na2 Cs1 Sn12 71.7(7) 1_655 3_644
Na2 Cs1 Sn12 44.7(7) 10_655 3_644
Na2 Cs1 Sn12 102.9(6) 2_655 3_644
Sn15 Cs1 Sn12 95.68(3) 14_755 3_644
Sn15 Cs1 Sn12 109.16(3) 12_756 3_644
Sn15 Cs1 Sn12 149.15(7) 5_645 3_644
Sn15 Cs1 Sn12 64.45(3) 3_644 3_644
Sn6 Cs1 Sn12 92.36(2) 14_755 3_644
Sn6 Cs1 Sn12 92.22(2) 12_756 3_644
Sn6 Cs1 Sn12 151.90(4) 5_645 3_644
Sn6 Cs1 Sn12 36.652(19) 3_644 3_644
Na1 Cs1 Sn12 107.60(5) 9_665 3_644
Sn12 Cs1 Sn12 59.85(3) 14_755 3_644
Sn12 Cs1 Sn12 108.62(5) 12_756 3_644
Sn12 Cs1 Sn12 144.80(9) 5_645 3_644
Sn14 Cs1 Sn17 134.59(7) 9_655 7
Sn14 Cs1 Sn17 150.18(5) 1_655 7
Sn14 Cs1 Sn17 150.18(5) 10_655 7
Sn14 Cs1 Sn17 134.59(7) 2_655 7
Na2 Cs1 Sn17 129.4(6) 9_655 7
Na2 Cs1 Sn17 157.1(6) 1_655 7
Na2 Cs1 Sn17 157.1(6) 10_655 7
Na2 Cs1 Sn17 129.4(6) 2_655 7
Sn15 Cs1 Sn17 34.70(6) 14_755 7
Sn15 Cs1 Sn17 57.33(8) 12_756 7
Sn15 Cs1 Sn17 34.70(6) 5_645 7
Sn15 Cs1 Sn17 57.33(8) 3_644 7
Sn6 Cs1 Sn17 69.40(8) 14_755 7
Sn6 Cs1 Sn17 95.59(9) 12_756 7
Sn6 Cs1 Sn17 69.40(8) 5_645 7
Sn6 Cs1 Sn17 95.59(9) 3_644 7
Na1 Cs1 Sn17 15.41(8) 9_665 7
Sn12 Cs1 Sn17 99.15(6) 14_755 7
Sn12 Cs1 Sn17 115.09(6) 12_756 7
Sn12 Cs1 Sn17 99.15(6) 5_645 7
Sn12 Cs1 Sn17 115.09(6) 3_644 7
Sn14 Cs1 Sn17 150.18(5) 9_655 9_665
Sn14 Cs1 Sn17 134.59(7) 1_655 9_665
Sn14 Cs1 Sn17 134.59(7) 10_655 9_665
Sn14 Cs1 Sn17 150.18(5) 2_655 9_665
Na2 Cs1 Sn17 157.1(6) 9_655 9_665
Na2 Cs1 Sn17 129.4(6) 1_655 9_665
Na2 Cs1 Sn17 129.4(6) 10_655 9_665
Na2 Cs1 Sn17 157.1(6) 2_655 9_665
Sn15 Cs1 Sn17 57.33(8) 14_755 9_665
Sn15 Cs1 Sn17 34.70(6) 12_756 9_665
Sn15 Cs1 Sn17 57.33(8) 5_645 9_665
Sn15 Cs1 Sn17 34.70(6) 3_644 9_665
Sn6 Cs1 Sn17 95.59(9) 14_755 9_665
Sn6 Cs1 Sn17 69.40(8) 12_756 9_665
Sn6 Cs1 Sn17 95.59(9) 5_645 9_665
Sn6 Cs1 Sn17 69.40(8) 3_644 9_665
Na1 Cs1 Sn17 15.41(8) 9_665 9_665
Sn12 Cs1 Sn17 115.09(6) 14_755 9_665
Sn12 Cs1 Sn17 99.15(6) 12_756 9_665
Sn12 Cs1 Sn17 115.09(6) 5_645 9_665
Sn12 Cs1 Sn17 99.15(6) 3_644 9_665
Sn17 Cs1 Sn17 30.82(17) 7 9_665
Sn14 Cs1 Sn10 95.19(4) 9_655 4_554
Sn14 Cs1 Sn10 151.45(6) 1_655 4_554
Sn14 Cs1 Sn10 95.19(4) 10_655 4_554
Sn14 Cs1 Sn10 151.45(6) 2_655 4_554
Na2 Cs1 Sn10 106.5(7) 9_655 4_554
Na2 Cs1 Sn10 132.6(7) 1_655 4_554
Na2 Cs1 Sn10 106.5(7) 10_655 4_554
Na2 Cs1 Sn10 132.6(7) 2_655 4_554
Sn15 Cs1 Sn10 37.24(3) 14_755 4_554
Sn15 Cs1 Sn10 87.45(6) 12_756 4_554
Sn15 Cs1 Sn10 87.45(6) 5_645 4_554
Sn15 Cs1 Sn10 37.24(3) 3_644 4_554
Sn6 Cs1 Sn10 60.36(3) 14_755 4_554
Sn6 Cs1 Sn10 109.73(5) 12_756 4_554
Sn6 Cs1 Sn10 109.73(5) 5_645 4_554
Sn6 Cs1 Sn10 60.36(3) 3_644 4_554
Na1 Cs1 Sn10 53.49(4) 9_665 4_554
Sn12 Cs1 Sn10 61.78(2) 14_755 4_554
Sn12 Cs1 Sn10 146.38(5) 12_756 4_554
Sn12 Cs1 Sn10 146.38(5) 5_645 4_554
Sn12 Cs1 Sn10 61.78(2) 3_644 4_554
Sn17 Cs1 Sn10 55.00(5) 7 4_554
Sn17 Cs1 Sn10 55.00(4) 9_665 4_554
Sn14 Cs1 Sn10 151.45(6) 9_655 11_666
Sn14 Cs1 Sn10 95.19(4) 1_655 11_666
Sn14 Cs1 Sn10 151.45(6) 10_655 11_666
Sn14 Cs1 Sn10 95.19(4) 2_655 11_666
Na2 Cs1 Sn10 132.6(7) 9_655 11_666
Na2 Cs1 Sn10 106.5(7) 1_655 11_666
Na2 Cs1 Sn10 132.6(7) 10_655 11_666
Na2 Cs1 Sn10 106.5(7) 2_655 11_666
Sn15 Cs1 Sn10 87.45(6) 14_755 11_666
Sn15 Cs1 Sn10 37.24(3) 12_756 11_666
Sn15 Cs1 Sn10 37.24(3) 5_645 11_666
Sn15 Cs1 Sn10 87.45(6) 3_644 11_666
Sn6 Cs1 Sn10 109.73(5) 14_755 11_666
Sn6 Cs1 Sn10 60.36(3) 12_756 11_666
Sn6 Cs1 Sn10 60.36(3) 5_645 11_666
Sn6 Cs1 Sn10 109.73(5) 3_644 11_666
Na1 Cs1 Sn10 53.49(4) 9_665 11_666
Sn12 Cs1 Sn10 146.38(5) 14_755 11_666
Sn12 Cs1 Sn10 61.78(2) 12_756 11_666
Sn12 Cs1 Sn10 61.78(2) 5_645 11_666
Sn12 Cs1 Sn10 146.38(5) 3_644 11_666
Sn17 Cs1 Sn10 55.00(4) 7 11_666
Sn17 Cs1 Sn10 55.00(5) 9_665 11_666
Sn10 Cs1 Sn10 106.97(8) 4_554 11_666
Sn14 Cs1 Sn8 97.34(7) 9_655 1_655
Sn14 Cs1 Sn8 61.29(5) 1_655 1_655
Sn14 Cs1 Sn8 61.29(5) 10_655 1_655
Sn14 Cs1 Sn8 97.34(7) 2_655 1_655
Na2 Cs1 Sn8 110.5(6) 9_655 1_655
Na2 Cs1 Sn8 45.6(6) 1_655 1_655
Na2 Cs1 Sn8 45.6(6) 10_655 1_655
Na2 Cs1 Sn8 110.5(6) 2_655 1_655
Sn15 Cs1 Sn8 132.20(6) 14_755 1_655
Sn15 Cs1 Sn8 68.54(3) 12_756 1_655
Sn15 Cs1 Sn8 132.20(6) 5_645 1_655
Sn15 Cs1 Sn8 68.54(3) 3_644 1_655
Sn6 Cs1 Sn8 148.63(2) 14_755 1_655
Sn6 Cs1 Sn8 37.185(17) 12_756 1_655
Sn6 Cs1 Sn8 148.63(2) 5_645 1_655
Sn6 Cs1 Sn8 37.185(17) 3_644 1_655
Na1 Cs1 Sn8 102.50(5) 9_665 1_655
Sn12 Cs1 Sn8 114.93(4) 14_755 1_655
Sn12 Cs1 Sn8 56.460(19) 12_756 1_655
Sn12 Cs1 Sn8 114.93(4) 5_645 1_655
Sn12 Cs1 Sn8 56.460(19) 3_644 1_655
Sn17 Cs1 Sn8 117.91(10) 7 1_655
Sn17 Cs1 Sn8 87.10(9) 9_665 1_655
Sn10 Cs1 Sn8 97.40(2) 4_554 1_655
Sn10 Cs1 Sn8 97.40(2) 11_666 1_655
Sn14 Cs1 Sn8 61.29(5) 9_655 15_655
Sn14 Cs1 Sn8 97.34(7) 1_655 15_655
Sn14 Cs1 Sn8 97.34(7) 10_655 15_655
Sn14 Cs1 Sn8 61.29(5) 2_655 15_655
Na2 Cs1 Sn8 45.6(6) 9_655 15_655
Na2 Cs1 Sn8 110.5(6) 1_655 15_655
Na2 Cs1 Sn8 110.5(6) 10_655 15_655
Na2 Cs1 Sn8 45.6(6) 2_655 15_655
Sn15 Cs1 Sn8 68.54(3) 14_755 15_655
Sn15 Cs1 Sn8 132.20(6) 12_756 15_655
Sn15 Cs1 Sn8 68.54(3) 5_645 15_655
Sn15 Cs1 Sn8 132.20(6) 3_644 15_655
Sn6 Cs1 Sn8 37.185(17) 14_755 15_655
Sn6 Cs1 Sn8 148.63(2) 12_756 15_655
Sn6 Cs1 Sn8 37.185(17) 5_645 15_655
Sn6 Cs1 Sn8 148.63(2) 3_644 15_655
Na1 Cs1 Sn8 102.50(5) 9_665 15_655
Sn12 Cs1 Sn8 56.460(19) 14_755 15_655
Sn12 Cs1 Sn8 114.93(4) 12_756 15_655
Sn12 Cs1 Sn8 56.460(19) 5_645 15_655
Sn12 Cs1 Sn8 114.93(4) 3_644 15_655
Sn17 Cs1 Sn8 87.10(9) 7 15_655
Sn17 Cs1 Sn8 117.91(10) 9_665 15_655
Sn10 Cs1 Sn8 97.40(2) 4_554 15_655
Sn10 Cs1 Sn8 97.40(2) 11_666 15_655
Sn8 Cs1 Sn8 154.99(10) 1_655 15_655
Sn14 Cs1 Sn4 119.85(8) 9_655 11_666
Sn14 Cs1 Sn4 61.15(5) 1_655 11_666
Sn14 Cs1 Sn4 119.85(8) 10_655 11_666
Sn14 Cs1 Sn4 61.15(5) 2_655 11_666
Na2 Cs1 Sn4 104.6(7) 9_655 11_666
Na2 Cs1 Sn4 76.3(7) 1_655 11_666
Na2 Cs1 Sn4 104.6(7) 10_655 11_666
Na2 Cs1 Sn4 76.3(7) 2_655 11_666
Sn15 Cs1 Sn4 117.45(6) 14_755 11_666
Sn15 Cs1 Sn4 61.70(3) 12_756 11_666
Sn15 Cs1 Sn4 61.70(3) 5_645 11_666
Sn15 Cs1 Sn4 117.45(6) 3_644 11_666
Sn6 Cs1 Sn4 121.094(18) 14_755 11_666
Sn6 Cs1 Sn4 58.741(14) 12_756 11_666
Sn6 Cs1 Sn4 58.741(14) 5_645 11_666
Sn6 Cs1 Sn4 121.094(18) 3_644 11_666
Na1 Cs1 Sn4 89.46(5) 9_665 11_666
Sn12 Cs1 Sn4 144.59(5) 14_755 11_666
Sn12 Cs1 Sn4 35.968(17) 12_756 11_666
Sn12 Cs1 Sn4 35.968(17) 5_645 11_666
Sn12 Cs1 Sn4 144.59(5) 3_644 11_666
Sn17 Cs1 Sn4 89.48(5) 7 11_666
Sn17 Cs1 Sn4 89.48(5) 9_665 11_666
Sn10 Cs1 Sn4 142.95(9) 4_554 11_666
Sn10 Cs1 Sn4 35.98(3) 11_666 11_666
Sn8 Cs1 Sn4 90.116(11) 1_655 11_666
Sn8 Cs1 Sn4 90.116(11) 15_655 11_666
Sn14 Cs1 Sn4 61.15(5) 9_655 4_554
Sn14 Cs1 Sn4 119.85(8) 1_655 4_554
Sn14 Cs1 Sn4 61.15(5) 10_655 4_554
Sn14 Cs1 Sn4 119.85(8) 2_655 4_554
Na2 Cs1 Sn4 76.3(7) 9_655 4_554
Na2 Cs1 Sn4 104.6(7) 1_655 4_554
Na2 Cs1 Sn4 76.3(7) 10_655 4_554
Na2 Cs1 Sn4 104.6(7) 2_655 4_554
Sn15 Cs1 Sn4 61.70(3) 14_755 4_554
Sn15 Cs1 Sn4 117.45(6) 12_756 4_554
Sn15 Cs1 Sn4 117.45(6) 5_645 4_554
Sn15 Cs1 Sn4 61.70(3) 3_644 4_554
Sn6 Cs1 Sn4 58.741(14) 14_755 4_554
Sn6 Cs1 Sn4 121.094(18) 12_756 4_554
Sn6 Cs1 Sn4 121.094(18) 5_645 4_554
Sn6 Cs1 Sn4 58.741(14) 3_644 4_554
Na1 Cs1 Sn4 89.46(5) 9_665 4_554
Sn12 Cs1 Sn4 35.968(17) 14_755 4_554
Sn12 Cs1 Sn4 144.59(5) 12_756 4_554
Sn12 Cs1 Sn4 144.59(5) 5_645 4_554
Sn12 Cs1 Sn4 35.968(17) 3_644 4_554
Sn17 Cs1 Sn4 89.48(5) 7 4_554
Sn17 Cs1 Sn4 89.48(5) 9_665 4_554
Sn10 Cs1 Sn4 35.98(3) 4_554 4_554
Sn10 Cs1 Sn4 142.95(9) 11_666 4_554
Sn8 Cs1 Sn4 90.116(11) 1_655 4_554
Sn8 Cs1 Sn4 90.116(11) 15_655 4_554
Sn4 Cs1 Sn4 178.93(11) 11_666 4_554
Sn14 Cs1 Sn16 66.29(7) 9_655 1_655
Sn14 Cs1 Sn16 35.35(5) 1_655 1_655
Sn14 Cs1 Sn16 35.35(5) 10_655 1_655
Sn14 Cs1 Sn16 66.29(7) 2_655 1_655
Na2 Cs1 Sn16 75.7(6) 9_655 1_655
Na2 Cs1 Sn16 16.2(7) 1_655 1_655
Na2 Cs1 Sn16 16.2(7) 10_655 1_655
Na2 Cs1 Sn16 75.7(6) 2_655 1_655
Sn15 Cs1 Sn16 151.77(2) 14_755 1_655
Sn15 Cs1 Sn16 100.11(4) 12_756 1_655
Sn15 Cs1 Sn16 151.77(2) 5_645 1_655
Sn15 Cs1 Sn16 100.11(4) 3_644 1_655
Sn6 Cs1 Sn16 131.28(7) 14_755 1_655
Sn6 Cs1 Sn16 62.46(4) 12_756 1_655
Sn6 Cs1 Sn16 131.28(7) 5_645 1_655
Sn6 Cs1 Sn16 62.46(4) 3_644 1_655
Na1 Cs1 Sn16 138.42(5) 9_665 1_655
Sn12 Cs1 Sn16 96.02(6) 14_755 1_655
Sn12 Cs1 Sn16 56.13(3) 12_756 1_655
Sn12 Cs1 Sn16 96.02(6) 5_645 1_655
Sn12 Cs1 Sn16 56.13(3) 3_644 1_655
Sn17 Cs1 Sn16 153.82(10) 7 1_655
Sn17 Cs1 Sn16 123.01(9) 9_665 1_655
Sn10 Cs1 Sn16 116.43(2) 4_554 1_655
Sn10 Cs1 Sn16 116.43(2) 11_666 1_655
Sn8 Cs1 Sn16 35.91(4) 1_655 1_655
Sn8 Cs1 Sn16 119.08(9) 15_655 1_655
Sn4 Cs1 Sn16 90.40(4) 11_666 1_655
Sn4 Cs1 Sn16 90.40(4) 4_554 1_655
Sn13 Cs2 Sn13 78.09(6) 5_545 11_566
Sn13 Cs2 Sn5 41.73(3) 5_545 13_566
Sn13 Cs2 Sn5 72.48(4) 11_566 13_566
Sn13 Cs2 Sn5 72.48(4) 5_545 3_545
Sn13 Cs2 Sn5 41.73(3) 11_566 3_545
Sn5 Cs2 Sn5 41.39(4) 13_566 3_545
Sn13 Cs2 Na2 117.5(5) 5_545 .
Sn13 Cs2 Na2 117.5(5) 11_566 .
Sn5 Cs2 Na2 83.1(7) 13_566 .
Sn5 Cs2 Na2 83.1(7) 3_545 .
Sn13 Cs2 Sn16 129.50(6) 5_545 .
Sn13 Cs2 Sn16 129.50(6) 11_566 .
Sn5 Cs2 Sn16 100.37(7) 13_566 .
Sn5 Cs2 Sn16 100.37(7) 3_545 .
Na2 Cs2 Sn16 18.4(8) . .
Sn13 Cs2 Sn3 97.24(3) 5_545 7
Sn13 Cs2 Sn3 152.88(8) 11_566 7
Sn5 Cs2 Sn3 121.32(3) 13_566 7
Sn5 Cs2 Sn3 161.53(5) 3_545 7
Na2 Cs2 Sn3 88.5(6) . 7
Sn16 Cs2 Sn3 73.96(5) . 7
Sn13 Cs2 Sn3 152.88(8) 5_545 .
Sn13 Cs2 Sn3 97.24(3) 11_566 .
Sn5 Cs2 Sn3 161.53(5) 13_566 .
Sn5 Cs2 Sn3 121.32(3) 3_545 .
Na2 Cs2 Sn3 88.5(6) . .
Sn16 Cs2 Sn3 73.96(5) . .
Sn3 Cs2 Sn3 74.66(5) 7 .
Sn13 Cs2 Sn2 117.69(6) 5_545 .
Sn13 Cs2 Sn2 117.69(6) 11_566 .
Sn5 Cs2 Sn2 157.37(4) 13_566 .
Sn5 Cs2 Sn2 157.37(4) 3_545 .
Na2 Cs2 Sn2 106.7(8) . .
Sn16 Cs2 Sn2 88.27(6) . .
Sn3 Cs2 Sn2 41.10(3) 7 .
Sn3 Cs2 Sn2 41.10(3) . .
Sn13 Cs2 Na1 48.90(16) 5_545 11_566
Sn13 Cs2 Na1 48.90(16) 11_566 11_566
Sn5 Cs2 Na1 77.0(3) 13_566 11_566
Sn5 Cs2 Na1 77.0(3) 3_545 11_566
Na2 Cs2 Na1 158.7(8) . 11_566
Sn16 Cs2 Na1 177.2(3) . 11_566
Sn3 Cs2 Na1 108.2(2) 7 11_566
Sn3 Cs2 Na1 108.2(2) . 11_566
Sn2 Cs2 Na1 94.6(3) . 11_566
Sn13 Cs2 Sn8 165.95(8) 5_545 .
Sn13 Cs2 Sn8 102.05(3) 11_566 .
Sn5 Cs2 Sn8 124.60(7) 13_566 .
Sn5 Cs2 Sn8 98.10(4) 3_545 .
Na2 Cs2 Sn8 49.7(5) . .
Sn16 Cs2 Sn8 40.47(3) . .
Sn3 Cs2 Sn8 88.83(5) 7 .
Sn3 Cs2 Sn8 41.13(3) . .
Sn2 Cs2 Sn8 74.95(4) . .
Na1 Cs2 Sn8 140.50(10) 11_566 .
Sn13 Cs2 Sn8 102.05(3) 5_545 7
Sn13 Cs2 Sn8 165.95(8) 11_566 7
Sn5 Cs2 Sn8 98.10(4) 13_566 7
Sn5 Cs2 Sn8 124.60(7) 3_545 7
Na2 Cs2 Sn8 49.7(5) . 7
Sn16 Cs2 Sn8 40.47(3) . 7
Sn3 Cs2 Sn8 41.13(3) 7 7
Sn3 Cs2 Sn8 88.83(5) . 7
Sn2 Cs2 Sn8 74.95(4) . 7
Na1 Cs2 Sn8 140.50(10) 11_566 7
Sn8 Cs2 Sn8 74.35(6) . 7
Sn13 Cs2 Sn12 70.18(4) 5_545 6_455
Sn13 Cs2 Sn12 106.28(5) 11_566 6_455
Sn5 Cs2 Sn12 40.23(3) 13_566 6_455
Sn5 Cs2 Sn12 65.42(4) 3_545 6_455
Na2 Cs2 Sn12 47.4(6) . 6_455
Sn16 Cs2 Sn12 62.08(5) . 6_455
Sn3 Cs2 Sn12 96.88(4) 7 6_455
Sn3 Cs2 Sn12 135.73(7) . 6_455
Sn2 Cs2 Sn12 136.03(5) . 6_455
Na1 Cs2 Sn12 115.6(2) 11_566 6_455
Sn8 Cs2 Sn12 96.58(6) . 6_455
Sn8 Cs2 Sn12 61.35(4) 7 6_455
Sn13 Cs2 Sn12 106.28(5) 5_545 12_656
Sn13 Cs2 Sn12 70.18(4) 11_566 12_656
Sn5 Cs2 Sn12 65.42(4) 13_566 12_656
Sn5 Cs2 Sn12 40.23(3) 3_545 12_656
Na2 Cs2 Sn12 47.4(6) . 12_656
Sn16 Cs2 Sn12 62.08(5) . 12_656
Sn3 Cs2 Sn12 135.73(7) 7 12_656
Sn3 Cs2 Sn12 96.88(4) . 12_656
Sn2 Cs2 Sn12 136.03(5) . 12_656
Na1 Cs2 Sn12 115.6(2) 11_566 12_656
Sn8 Cs2 Sn12 61.35(4) . 12_656
Sn8 Cs2 Sn12 96.58(6) 7 12_656
Sn12 Cs2 Sn12 58.89(4) 6_455 12_656
Sn13 Cs2 Sn17 37.28(8) 5_545 5_545
Sn13 Cs2 Sn17 63.35(9) 11_566 5_545
Sn5 Cs2 Sn17 72.97(8) 13_566 5_545
Sn5 Cs2 Sn17 84.37(8) 3_545 5_545
Na2 Cs2 Sn17 154.7(6) . 5_545
Sn16 Cs2 Sn17 163.94(8) . 5_545
Sn3 Cs2 Sn17 96.70(8) 7 5_545
Sn3 Cs2 Sn17 116.80(10) . 5_545
Sn2 Cs2 Sn17 93.06(8) . 5_545
Na1 Cs2 Sn17 16.06(9) 11_566 5_545
Sn8 Cs2 Sn17 154.61(10) . 5_545
Sn8 Cs2 Sn17 124.78(9) 7 5_545
Sn12 Cs2 Sn17 107.25(8) 6_455 5_545
Sn12 Cs2 Sn17 124.58(8) 12_656 5_545
Sn13 Cs2 Sn17 63.35(9) 5_545 11_566
Sn13 Cs2 Sn17 37.28(8) 11_566 11_566
Sn5 Cs2 Sn17 84.37(8) 13_566 11_566
Sn5 Cs2 Sn17 72.97(8) 3_545 11_566
Na2 Cs2 Sn17 154.7(6) . 11_566
Sn16 Cs2 Sn17 163.94(8) . 11_566
Sn3 Cs2 Sn17 116.80(10) 7 11_566
Sn3 Cs2 Sn17 96.70(8) . 11_566
Sn2 Cs2 Sn17 93.06(8) . 11_566
Na1 Cs2 Sn17 16.06(9) 11_566 11_566
Sn8 Cs2 Sn17 124.78(8) . 11_566
Sn8 Cs2 Sn17 154.61(10) 7 11_566
Sn12 Cs2 Sn17 124.58(8) 6_455 11_566
Sn12 Cs2 Sn17 107.25(8) 12_656 11_566
Sn17 Cs2 Sn17 32.00(17) 5_545 11_566
Sn13 Cs2 Sn1 38.99(3) 5_545 6_455
Sn13 Cs2 Sn1 117.08(6) 11_566 6_455
Sn5 Cs2 Sn1 61.45(3) 13_566 6_455
Sn5 Cs2 Sn1 102.33(4) 3_545 6_455
Na2 Cs2 Sn1 97.64(13) . 6_455
Sn16 Cs2 Sn1 100.17(4) . 6_455
Sn3 Cs2 Sn1 62.43(2) 7 6_455
Sn3 Cs2 Sn1 136.34(5) . 6_455
Sn2 Cs2 Sn1 96.58(3) . 6_455
Na1 Cs2 Sn1 79.53(5) 11_566 6_455
Sn8 Cs2 Sn1 138.70(6) . 6_455
Sn8 Cs2 Sn1 64.48(2) 7 6_455
Sn12 Cs2 Sn1 61.41(2) 6_455 6_455
Sn12 Cs2 Sn1 118.90(5) 12_656 6_455
Sn17 Cs2 Sn1 63.77(9) 5_545 6_455
Sn17 Cs2 Sn1 95.58(9) 11_566 6_455
Sn13 Cs2 Sn1 117.08(6) 5_545 12_656
Sn13 Cs2 Sn1 38.99(3) 11_566 12_656
Sn5 Cs2 Sn1 102.33(4) 13_566 12_656
Sn5 Cs2 Sn1 61.45(3) 3_545 12_656
Na2 Cs2 Sn1 97.64(13) . 12_656
Sn16 Cs2 Sn1 100.17(4) . 12_656
Sn3 Cs2 Sn1 136.34(5) 7 12_656
Sn3 Cs2 Sn1 62.42(2) . 12_656
Sn2 Cs2 Sn1 96.58(3) . 12_656
Na1 Cs2 Sn1 79.53(5) 11_566 12_656
Sn8 Cs2 Sn1 64.48(2) . 12_656
Sn8 Cs2 Sn1 138.70(6) 7 12_656
Sn12 Cs2 Sn1 118.90(5) 6_455 12_656
Sn12 Cs2 Sn1 61.41(2) 12_656 12_656
Sn17 Cs2 Sn1 95.58(9) 5_545 12_656
Sn17 Cs2 Sn1 63.77(9) 11_566 12_656
Sn1 Cs2 Sn1 156.03(6) 6_455 12_656
Sn13 Cs2 Sn10 88.51(5) 5_545 .
Sn13 Cs2 Sn10 88.51(5) 11_566 .
Sn5 Cs2 Sn10 128.72(6) 13_566 .
Sn5 Cs2 Sn10 128.72(6) 3_545 .
Na2 Cs2 Sn10 145.4(8) . .
Sn16 Cs2 Sn10 126.95(6) . .
Sn3 Cs2 Sn10 64.55(4) 7 .
Sn3 Cs2 Sn10 64.54(4) . .
Sn2 Cs2 Sn10 38.67(3) . .
Na1 Cs2 Sn10 55.9(3) 11_566 .
Sn8 Cs2 Sn10 105.54(4) . .
Sn8 Cs2 Sn10 105.54(4) 7 .
Sn12 Cs2 Sn10 150.25(3) 6_455 .
Sn12 Cs2 Sn10 150.25(3) 12_656 .
Sn17 Cs2 Sn10 56.08(7) 5_545 .
Sn17 Cs2 Sn10 56.08(7) 11_566 .
Sn1 Cs2 Sn10 88.93(4) 6_455 .
Sn1 Cs2 Sn10 88.93(4) 12_656 .
Sn13 Cs2 Sn7 61.29(3) 5_545 15_665
Sn13 Cs2 Sn7 124.61(7) 11_566 15_665
Sn5 Cs2 Sn7 95.84(3) 13_566 15_665
Sn5 Cs2 Sn7 133.62(5) 3_545 15_665
Na2 Cs2 Sn7 114.2(3) . 15_665
Sn16 Cs2 Sn7 105.69(4) . 15_665
Sn3 Cs2 Sn7 37.73(2) 7 15_665
Sn3 Cs2 Sn7 102.61(5) . 15_665
Sn2 Cs2 Sn7 61.59(3) . 15_665
Na1 Cs2 Sn7 75.75(15) 11_566 15_665
Sn8 Cs2 Sn7 126.43(5) . 15_665
Sn8 Cs2 Sn7 65.69(3) 7 15_665
Sn12 Cs2 Sn7 94.19(2) 6_455 15_665
Sn12 Cs2 Sn7 153.03(5) 12_656 15_665
Sn17 Cs2 Sn7 61.49(8) 5_545 15_665
Sn17 Cs2 Sn7 88.93(9) 11_566 15_665
Sn1 Cs2 Sn7 36.023(18) 6_455 15_665
Sn1 Cs2 Sn7 145.00(7) 12_656 15_665
Sn10 Cs2 Sn7 56.67(3) . 15_665
Sn13 Cs2 Sn7 124.61(7) 5_545 2_665
Sn13 Cs2 Sn7 61.29(3) 11_566 2_665
Sn5 Cs2 Sn7 133.62(5) 13_566 2_665
Sn5 Cs2 Sn7 95.84(3) 3_545 2_665
Na2 Cs2 Sn7 114.2(3) . 2_665
Sn16 Cs2 Sn7 105.69(4) . 2_665
Sn3 Cs2 Sn7 102.61(5) 7 2_665
Sn3 Cs2 Sn7 37.73(2) . 2_665
Sn2 Cs2 Sn7 61.59(3) . 2_665
Na1 Cs2 Sn7 75.75(15) 11_566 2_665
Sn8 Cs2 Sn7 65.69(3) . 2_665
Sn8 Cs2 Sn7 126.43(5) 7 2_665
Sn12 Cs2 Sn7 153.03(5) 6_455 2_665
Sn12 Cs2 Sn7 94.19(2) 12_656 2_665
Sn17 Cs2 Sn7 88.93(9) 5_545 2_665
Sn17 Cs2 Sn7 61.49(8) 11_566 2_665
Sn1 Cs2 Sn7 145.00(7) 6_455 2_665
Sn1 Cs2 Sn7 36.023(18) 12_656 2_665
Sn10 Cs2 Sn7 56.67(3) . 2_665
Sn7 Cs2 Sn7 112.63(6) 15_665 2_665
Sn13 Cs2 Sn6 67.22(3) 5_545 6_455
Sn13 Cs2 Sn6 135.45(5) 11_566 6_455
Sn5 Cs2 Sn6 63.07(3) 13_566 6_455
Sn5 Cs2 Sn6 99.45(5) 3_545 6_455
Na2 Cs2 Sn6 61.40(9) . 6_455
Sn16 Cs2 Sn6 64.89(4) . 6_455
Sn3 Cs2 Sn6 62.14(3) 7 6_455
Sn3 Cs2 Sn6 126.26(5) . 6_455
Sn2 Cs2 Sn6 103.15(3) . 6_455
Na1 Cs2 Sn6 114.33(9) 11_566 6_455
Sn8 Cs2 Sn6 105.16(6) . 6_455
Sn8 Cs2 Sn6 37.49(2) 7 6_455
Sn12 Cs2 Sn6 36.44(2) 6_455 6_455
Sn12 Cs2 Sn6 93.09(5) 12_656 6_455
Sn17 Cs2 Sn6 99.29(9) 5_545 6_455
Sn17 Cs2 Sn6 129.98(9) 11_566 6_455
Sn1 Cs2 Sn6 36.361(19) 6_455 6_455
Sn1 Cs2 Sn6 154.50(6) 12_656 6_455
Sn10 Cs2 Sn6 116.57(3) . 6_455
Sn7 Cs2 Sn6 60.317(18) 15_665 6_455
Sn7 Cs2 Sn6 163.26(5) 2_665 6_455
Sn13 Cs2 Sn6 135.45(5) 5_545 12_656
Sn13 Cs2 Sn6 67.22(3) 11_566 12_656
Sn5 Cs2 Sn6 99.45(5) 13_566 12_656
Sn5 Cs2 Sn6 63.07(3) 3_545 12_656
Na2 Cs2 Sn6 61.40(9) . 12_656
Sn16 Cs2 Sn6 64.89(4) . 12_656
Sn3 Cs2 Sn6 126.25(5) 7 12_656
Sn3 Cs2 Sn6 62.14(3) . 12_656
Sn2 Cs2 Sn6 103.15(3) . 12_656
Na1 Cs2 Sn6 114.33(9) 11_566 12_656
Sn8 Cs2 Sn6 37.50(2) . 12_656
Sn8 Cs2 Sn6 105.16(6) 7 12_656
Sn12 Cs2 Sn6 93.09(5) 6_455 12_656
Sn12 Cs2 Sn6 36.44(2) 12_656 12_656
Sn17 Cs2 Sn6 129.98(9) 5_545 12_656
Sn17 Cs2 Sn6 99.29(9) 11_566 12_656
Sn1 Cs2 Sn6 154.50(6) 6_455 12_656
Sn1 Cs2 Sn6 36.361(19) 12_656 12_656
Sn10 Cs2 Sn6 116.57(3) . 12_656
Sn7 Cs2 Sn6 163.26(5) 15_665 12_656
Sn7 Cs2 Sn6 60.317(18) 2_665 12_656
Sn6 Cs2 Sn6 121.61(6) 6_455 12_656
Sn13 Cs2 Sn14 104.92(6) 5_545 .
Sn13 Cs2 Sn14 104.92(6) 11_566 .
Sn5 Cs2 Sn14 67.15(5) 13_566 .
Sn5 Cs2 Sn14 67.15(5) 3_545 .
Na2 Cs2 Sn14 17.2(8) . .
Sn16 Cs2 Sn14 35.62(6) . .
Sn3 Cs2 Sn14 102.10(6) 7 .
Sn3 Cs2 Sn14 102.10(6) . .
Sn2 Cs2 Sn14 123.89(7) . .
Na1 Cs2 Sn14 141.5(3) 11_566 .
Sn8 Cs2 Sn14 61.28(5) . .
Sn8 Cs2 Sn14 61.28(5) 7 .
Sn12 Cs2 Sn14 36.07(3) 6_455 .
Sn12 Cs2 Sn14 36.07(3) 12_656 .
Sn17 Cs2 Sn14 140.07(9) 5_545 .
Sn17 Cs2 Sn14 140.07(9) 11_566 .
Sn1 Cs2 Sn14 94.58(4) 6_455 .
Sn1 Cs2 Sn14 94.58(4) 12_656 .
Sn10 Cs2 Sn14 162.57(7) . .
Sn7 Cs2 Sn14 120.12(4) 15_665 .
Sn7 Cs2 Sn14 120.12(4) 2_665 .
Sn6 Cs2 Sn14 60.98(3) 6_455 .
Sn6 Cs2 Sn14 60.98(3) 12_656 .
Sn13 Cs2 Sn15 55.24(4) 5_545 15_665
Sn13 Cs2 Sn15 91.51(6) 11_566 15_665
Sn5 Cs2 Sn15 96.94(4) 13_566 15_665
Sn5 Cs2 Sn15 117.09(6) 3_545 15_665
Na2 Cs2 Sn15 149.1(3) . 15_665
Sn16 Cs2 Sn15 138.64(5) . 15_665
Sn3 Cs2 Sn15 64.95(4) 7 15_665
Sn3 Cs2 Sn15 98.67(5) . 15_665
Sn2 Cs2 Sn15 64.01(4) . 15_665
Na1 Cs2 Sn15 43.4(2) 11_566 15_665
Sn8 Cs2 Sn15 138.41(6) . 15_665
Sn8 Cs2 Sn15 100.12(4) 7 15_665
Sn12 Cs2 Sn15 117.20(3) 6_455 15_665
Sn12 Cs2 Sn15 157.32(6) 12_656 15_665
Sn17 Cs2 Sn15 32.81(7) 5_545 15_665
Sn17 Cs2 Sn15 54.59(9) 11_566 15_665
Sn1 Cs2 Sn15 56.96(3) 6_455 15_665
Sn1 Cs2 Sn15 112.40(6) 12_656 15_665
Sn10 Cs2 Sn15 34.96(3) . 15_665
Sn7 Cs2 Sn15 34.90(3) 15_665 15_665
Sn7 Cs2 Sn15 88.16(5) 2_665 15_665
Sn6 Cs2 Sn15 90.92(2) 6_455 15_665
Sn6 Cs2 Sn15 147.43(5) 12_656 15_665
Sn14 Cs2 Sn15 151.47(2) . 15_665
Sn13 Cs2 Sn15 91.51(6) 5_545 2_665
Sn13 Cs2 Sn15 55.24(4) 11_566 2_665
Sn5 Cs2 Sn15 117.09(6) 13_566 2_665
Sn5 Cs2 Sn15 96.94(4) 3_545 2_665
Na2 Cs2 Sn15 149.1(3) . 2_665
Sn16 Cs2 Sn15 138.64(5) . 2_665
Sn3 Cs2 Sn15 98.67(5) 7 2_665
Sn3 Cs2 Sn15 64.95(4) . 2_665
Sn2 Cs2 Sn15 64.01(4) . 2_665
Na1 Cs2 Sn15 43.4(2) 11_566 2_665
Sn8 Cs2 Sn15 100.12(4) . 2_665
Sn8 Cs2 Sn15 138.41(6) 7 2_665
Sn12 Cs2 Sn15 157.32(6) 6_455 2_665
Sn12 Cs2 Sn15 117.20(3) 12_656 2_665
Sn17 Cs2 Sn15 54.59(9) 5_545 2_665
Sn17 Cs2 Sn15 32.81(7) 11_566 2_665
Sn1 Cs2 Sn15 112.40(6) 6_455 2_665
Sn1 Cs2 Sn15 56.96(3) 12_656 2_665
Sn10 Cs2 Sn15 34.96(3) . 2_665
Sn7 Cs2 Sn15 88.16(5) 15_665 2_665
Sn7 Cs2 Sn15 34.90(3) 2_665 2_665
Sn6 Cs2 Sn15 147.43(5) 6_455 2_665
Sn6 Cs2 Sn15 90.92(2) 12_656 2_665
Sn14 Cs2 Sn15 151.47(2) . 2_665
Sn15 Cs2 Sn15 56.52(4) 15_665 2_665
Sn13 Cs2 Na2 130.6(3) 5_545 10
Sn13 Cs2 Na2 130.6(3) 11_566 10
Sn5 Cs2 Na2 102.1(5) 13_566 10
Sn5 Cs2 Na2 102.1(5) 3_545 10
Na2 Cs2 Na2 20.3(11) . 10
Sn16 Cs2 Na2 1.9(6) . 10
Sn3 Cs2 Na2 72.5(5) 7 10
Sn3 Cs2 Na2 72.5(5) . 10
Sn2 Cs2 Na2 86.4(6) . 10
Na1 Cs2 Na2 179.0(7) 11_566 10
Sn8 Cs2 Na2 39.81(19) . 10
Sn8 Cs2 Na2 39.8(2) 7 10
Sn12 Cs2 Na2 63.6(5) 6_455 10
Sn12 Cs2 Na2 63.6(5) 12_656 10
Sn17 Cs2 Na2 164.00(9) 5_545 10
Sn17 Cs2 Na2 164.00(9) 11_566 10
Sn1 Cs2 Na2 100.37(7) 6_455 10
Sn1 Cs2 Na2 100.37(7) 12_656 10
Sn10 Cs2 Na2 125.1(6) . 10
Sn7 Cs2 Na2 104.7(3) 15_665 10
Sn7 Cs2 Na2 104.7(3) 2_665 10
Sn6 Cs2 Na2 65.40(17) 6_455 10
Sn6 Cs2 Na2 65.40(17) 12_656 10
Sn14 Cs2 Na2 37.5(6) . 10
Sn15 Cs2 Na2 137.3(4) 15_665 10
Sn15 Cs2 Na2 137.3(4) 2_665 10
Sn13 Cs2 Cs2 140.10(3) 5_545 10
Sn13 Cs2 Cs2 140.10(3) 11_566 10
Sn5 Cs2 Cs2 140.08(4) 13_566 10
Sn5 Cs2 Cs2 140.08(4) 3_545 10
Na2 Cs2 Cs2 62.4(8) . 10
Sn16 Cs2 Cs2 43.98(5) . 10
Sn3 Cs2 Cs2 44.23(3) 7 10
Sn3 Cs2 Cs2 44.23(3) . 10
Sn2 Cs2 Cs2 44.29(4) . 10
Na1 Cs2 Cs2 138.9(3) 11_566 10
Sn8 Cs2 Cs2 44.61(3) . 10
Sn8 Cs2 Cs2 44.61(3) 7 10
Sn12 Cs2 Cs2 99.95(3) 6_455 10
Sn12 Cs2 Cs2 99.95(3) 12_656 10
Sn17 Cs2 Cs2 135.11(7) 5_545 10
Sn17 Cs2 Cs2 135.11(7) 11_566 10
Sn1 Cs2 Cs2 101.71(3) 6_455 10
Sn1 Cs2 Cs2 101.71(3) 12_656 10
Sn10 Cs2 Cs2 82.97(3) . 10
Sn7 Cs2 Cs2 81.86(3) 15_665 10
Sn7 Cs2 Cs2 81.86(3) 2_665 10
Sn6 Cs2 Cs2 82.04(3) 6_455 10
Sn6 Cs2 Cs2 82.04(3) 12_656 10
Sn14 Cs2 Cs2 79.60(5) . 10
Sn15 Cs2 Cs2 102.71(3) 15_665 10
Sn15 Cs2 Cs2 102.71(3) 2_665 10
Na2 Cs2 Cs2 42.1(6) 10 10
Sn13 Cs2 Cs2 39.90(3) 5_545 10_556
Sn13 Cs2 Cs2 39.90(3) 11_566 10_556
Sn5 Cs2 Cs2 39.92(4) 13_566 10_556
Sn5 Cs2 Cs2 39.92(4) 3_545 10_556
Na2 Cs2 Cs2 117.6(8) . 10_556
Sn16 Cs2 Cs2 136.02(5) . 10_556
Sn3 Cs2 Cs2 135.77(3) 7 10_556
Sn3 Cs2 Cs2 135.77(3) . 10_556
Sn2 Cs2 Cs2 135.70(4) . 10_556
Na1 Cs2 Cs2 41.1(3) 11_566 10_556
Sn8 Cs2 Cs2 135.39(3) . 10_556
Sn8 Cs2 Cs2 135.39(3) 7 10_556
Sn12 Cs2 Cs2 80.05(3) 6_455 10_556
Sn12 Cs2 Cs2 80.05(3) 12_656 10_556
Sn17 Cs2 Cs2 44.88(7) 5_545 10_556
Sn17 Cs2 Cs2 44.88(7) 11_566 10_556
Sn1 Cs2 Cs2 78.29(3) 6_455 10_556
Sn1 Cs2 Cs2 78.29(3) 12_656 10_556
Sn10 Cs2 Cs2 97.03(3) . 10_556
Sn7 Cs2 Cs2 98.14(3) 15_665 10_556
Sn7 Cs2 Cs2 98.14(3) 2_665 10_556
Sn6 Cs2 Cs2 97.96(3) 6_455 10_556
Sn6 Cs2 Cs2 97.96(3) 12_656 10_556
Sn14 Cs2 Cs2 100.40(5) . 10_556
Sn15 Cs2 Cs2 77.29(3) 15_665 10_556
Sn15 Cs2 Cs2 77.29(3) 2_665 10_556
Na2 Cs2 Cs2 137.9(6) 10 10_556
Cs2 Cs2 Cs2 180.0 10 10_556
Sn13 Cs2 Cs5 75.59(4) 5_545 .
Sn13 Cs2 Cs5 75.59(4) 11_566 .
Sn5 Cs2 Cs5 33.87(3) 13_566 .
Sn5 Cs2 Cs5 33.87(3) 3_545 .
Na2 Cs2 Cs5 55.2(8) . .
Sn16 Cs2 Cs5 73.67(5) . .
Sn3 Cs2 Cs5 129.63(5) 7 .
Sn3 Cs2 Cs5 129.63(5) . .
Sn2 Cs2 Cs5 161.94(6) . .
Na1 Cs2 Cs5 103.5(3) 11_566 .
Sn8 Cs2 Cs5 90.77(5) . .
Sn8 Cs2 Cs5 90.77(5) 7 .
Sn12 Cs2 Cs5 33.26(2) 6_455 .
Sn12 Cs2 Cs5 33.26(2) 12_656 .
Sn17 Cs2 Cs5 104.28(7) 5_545 .
Sn17 Cs2 Cs5 104.28(7) 11_566 .
Sn1 Cs2 Cs5 86.83(3) 6_455 .
Sn1 Cs2 Cs5 86.83(3) 12_656 .
Sn10 Cs2 Cs5 159.38(5) . .
Sn7 Cs2 Cs5 122.73(3) 15_665 .
Sn7 Cs2 Cs5 122.73(3) 2_665 .
Sn6 Cs2 Cs5 69.51(3) 6_455 .
Sn6 Cs2 Cs5 69.51(3) 12_656 .
Sn14 Cs2 Cs5 38.05(4) . .
Sn15 Cs2 Cs5 130.80(4) 15_665 .
Sn15 Cs2 Cs5 130.80(4) 2_665 .
Na2 Cs2 Cs5 75.6(6) 10 .
Cs2 Cs2 Cs5 117.65(2) 10 .
Cs2 Cs2 Cs5 62.35(2) 10_556 .
Sn15 Cs3 Sn15 61.69(5) 13_575 6_465
Sn15 Cs3 Sn6 42.38(3) 13_575 13_575
Sn15 Cs3 Sn6 81.25(4) 6_465 13_575
Sn15 Cs3 Sn6 81.25(4) 13_575 6_465
Sn15 Cs3 Sn6 42.38(3) 6_465 6_465
Sn6 Cs3 Sn6 69.79(4) 13_575 6_465
Sn15 Cs3 Sn11 166.81(5) 13_575 8_675
Sn15 Cs3 Sn11 127.88(3) 6_465 8_675
Sn6 Cs3 Sn11 125.86(6) 13_575 8_675
Sn6 Cs3 Sn11 100.64(4) 6_465 8_675
Sn15 Cs3 Sn11 127.88(3) 13_575 15_675
Sn15 Cs3 Sn11 166.81(5) 6_465 15_675
Sn6 Cs3 Sn11 100.64(4) 13_575 15_675
Sn6 Cs3 Sn11 125.86(6) 6_465 15_675
Sn11 Cs3 Sn11 41.06(3) 8_675 15_675
Sn15 Cs3 Sn11 120.02(6) 13_575 7
Sn15 Cs3 Sn11 98.35(4) 6_465 7
Sn6 Cs3 Sn11 159.91(5) 13_575 7
Sn6 Cs3 Sn11 122.88(2) 6_465 7
Sn11 Cs3 Sn11 70.05(3) 8_675 7
Sn11 Cs3 Sn11 84.36(4) 15_675 7
Sn15 Cs3 Sn11 98.35(4) 13_575 16
Sn15 Cs3 Sn11 120.02(6) 6_465 16
Sn6 Cs3 Sn11 122.88(2) 13_575 16
Sn6 Cs3 Sn11 159.91(5) 6_465 16
Sn11 Cs3 Sn11 84.36(4) 8_675 16
Sn11 Cs3 Sn11 70.05(3) 15_675 16
Sn11 Cs3 Sn11 40.53(3) 7 16
Sn15 Cs3 Sn9 153.52(6) 13_575 5
Sn15 Cs3 Sn9 100.09(3) 6_465 5
Sn6 Cs3 Sn9 160.71(6) 13_575 5
Sn6 Cs3 Sn9 98.091(19) 6_465 5
Sn11 Cs3 Sn9 39.535(18) 8_675 5
Sn11 Cs3 Sn9 73.80(3) 15_675 5
Sn11 Cs3 Sn9 39.323(18) 7 5
Sn11 Cs3 Sn9 73.30(3) 16 5
Sn15 Cs3 Sn9 100.09(3) 13_575 13_675
Sn15 Cs3 Sn9 153.52(6) 6_465 13_675
Sn6 Cs3 Sn9 98.091(19) 13_575 13_675
Sn6 Cs3 Sn9 160.71(6) 6_465 13_675
Sn11 Cs3 Sn9 73.80(3) 8_675 13_675
Sn11 Cs3 Sn9 39.535(18) 15_675 13_675
Sn11 Cs3 Sn9 73.30(3) 7 13_675
Sn11 Cs3 Sn9 39.323(18) 16 13_675
Sn9 Cs3 Sn9 89.16(3) 5 13_675
Sn15 Cs3 Sn8 73.51(4) 13_575 7_565
Sn15 Cs3 Sn8 73.51(4) 6_465 7_565
Sn6 Cs3 Sn8 39.55(2) 13_575 7_565
Sn6 Cs3 Sn8 39.55(2) 6_465 7_565
Sn11 Cs3 Sn8 99.51(5) 8_675 7_565
Sn11 Cs3 Sn8 99.51(5) 15_675 7_565
Sn11 Cs3 Sn8 159.30(2) 7 7_565
Sn11 Cs3 Sn8 159.30(2) 16 7_565
Sn9 Cs3 Sn8 122.09(4) 5 7_565
Sn9 Cs3 Sn8 122.09(4) 13_675 7_565
Sn15 Cs3 Sn7 38.90(3) 13_575 13_575
Sn15 Cs3 Sn7 94.70(4) 6_465 13_575
Sn6 Cs3 Sn7 62.66(2) 13_575 13_575
Sn6 Cs3 Sn7 120.02(4) 6_465 13_575
Sn11 Cs3 Sn7 136.31(4) 8_675 13_575
Sn11 Cs3 Sn7 97.75(2) 15_675 13_575
Sn11 Cs3 Sn7 97.50(4) 7 13_575
Sn11 Cs3 Sn7 63.23(3) 16 13_575
Sn9 Cs3 Sn7 135.75(5) 5 13_575
Sn9 Cs3 Sn7 62.539(18) 13_675 13_575
Sn8 Cs3 Sn7 102.06(3) 7_565 13_575
Sn15 Cs3 Sn7 94.70(4) 13_575 6_465
Sn15 Cs3 Sn7 38.90(3) 6_465 6_465
Sn6 Cs3 Sn7 120.02(4) 13_575 6_465
Sn6 Cs3 Sn7 62.66(2) 6_465 6_465
Sn11 Cs3 Sn7 97.75(2) 8_675 6_465
Sn11 Cs3 Sn7 136.31(4) 15_675 6_465
Sn11 Cs3 Sn7 63.23(3) 7 6_465
Sn11 Cs3 Sn7 97.50(4) 16 6_465
Sn9 Cs3 Sn7 62.539(18) 5 6_465
Sn9 Cs3 Sn7 135.75(5) 13_675 6_465
Sn8 Cs3 Sn7 102.06(3) 7_565 6_465
Sn7 Cs3 Sn7 114.01(5) 13_575 6_465
Sn15 Cs3 Sn1 119.61(4) 13_575 6_465
Sn15 Cs3 Sn1 67.78(3) 6_465 6_465
Sn6 Cs3 Sn1 100.97(4) 13_575 6_465
Sn6 Cs3 Sn1 38.48(2) 6_465 6_465
Sn11 Cs3 Sn1 64.01(3) 8_675 6_465
Sn11 Cs3 Sn1 99.10(4) 15_675 6_465
Sn11 Cs3 Sn1 97.38(2) 7 6_465
Sn11 Cs3 Sn1 135.85(4) 16 6_465
Sn9 Cs3 Sn1 62.654(17) 5 6_465
Sn9 Cs3 Sn1 137.28(5) 13_675 6_465
Sn8 Cs3 Sn1 61.97(3) 7_565 6_465
Sn7 Cs3 Sn1 158.48(5) 13_575 6_465
Sn7 Cs3 Sn1 60.238(18) 6_465 6_465
Sn15 Cs3 Sn1 67.78(3) 13_575 13_575
Sn15 Cs3 Sn1 119.61(4) 6_465 13_575
Sn6 Cs3 Sn1 38.48(2) 13_575 13_575
Sn6 Cs3 Sn1 100.97(4) 6_465 13_575
Sn11 Cs3 Sn1 99.10(4) 8_675 13_575
Sn11 Cs3 Sn1 64.01(3) 15_675 13_575
Sn11 Cs3 Sn1 135.85(4) 7 13_575
Sn11 Cs3 Sn1 97.38(2) 16 13_575
Sn9 Cs3 Sn1 137.28(5) 5 13_575
Sn9 Cs3 Sn1 62.654(17) 13_675 13_575
Sn8 Cs3 Sn1 61.97(3) 7_565 13_575
Sn7 Cs3 Sn1 60.238(18) 13_575 13_575
Sn7 Cs3 Sn1 158.48(5) 6_465 13_575
Sn1 Cs3 Sn1 116.54(5) 6_465 13_575
Sn15 Cs3 Sn3 105.78(4) 13_575 7_565
Sn15 Cs3 Sn3 105.78(4) 6_465 7_565
Sn6 Cs3 Sn3 64.01(3) 13_575 7_565
Sn6 Cs3 Sn3 64.01(3) 6_465 7_565
Sn11 Cs3 Sn3 64.28(4) 8_675 7_565
Sn11 Cs3 Sn3 64.28(4) 15_675 7_565
Sn11 Cs3 Sn3 134.12(5) 7 7_565
Sn11 Cs3 Sn3 134.12(5) 16 7_565
Sn9 Cs3 Sn3 97.43(4) 5 7_565
Sn9 Cs3 Sn3 97.43(4) 13_675 7_565
Sn8 Cs3 Sn3 37.77(3) 7_565 7_565
Sn7 Cs3 Sn3 118.24(3) 13_575 7_565
Sn7 Cs3 Sn3 118.24(3) 6_465 7_565
Sn1 Cs3 Sn3 58.93(3) 6_465 7_565
Sn1 Cs3 Sn3 58.93(3) 13_575 7_565
Sn15 Cs3 Sn7 137.38(5) 13_575 15_675
Sn15 Cs3 Sn7 102.76(3) 6_465 15_675
Sn6 Cs3 Sn7 98.99(5) 13_575 15_675
Sn6 Cs3 Sn7 65.27(3) 6_465 15_675
Sn11 Cs3 Sn7 37.84(2) 8_675 15_675
Sn11 Cs3 Sn7 64.06(3) 15_675 15_675
Sn11 Cs3 Sn7 100.66(3) 7 15_675
Sn11 Cs3 Sn7 122.20(4) 16 15_675
Sn9 Cs3 Sn7 61.83(2) 5 15_675
Sn9 Cs3 Sn7 103.48(4) 13_675 15_675
Sn8 Cs3 Sn7 63.90(3) 7_565 15_675
Sn7 Cs3 Sn7 152.57(4) 13_575 15_675
Sn7 Cs3 Sn7 92.581(16) 6_465 15_675
Sn1 Cs3 Sn7 35.93(2) 6_465 15_675
Sn1 Cs3 Sn7 92.56(4) 13_575 15_675
Sn3 Cs3 Sn7 36.51(2) 7_565 15_675
Sn15 Cs3 Sn7 102.76(3) 13_575 8_675
Sn15 Cs3 Sn7 137.38(5) 6_465 8_675
Sn6 Cs3 Sn7 65.27(3) 13_575 8_675
Sn6 Cs3 Sn7 98.99(5) 6_465 8_675
Sn11 Cs3 Sn7 64.06(3) 8_675 8_675
Sn11 Cs3 Sn7 37.84(2) 15_675 8_675
Sn11 Cs3 Sn7 122.20(4) 7 8_675
Sn11 Cs3 Sn7 100.66(3) 16 8_675
Sn9 Cs3 Sn7 103.48(4) 5 8_675
Sn9 Cs3 Sn7 61.83(2) 13_675 8_675
Sn8 Cs3 Sn7 63.90(3) 7_565 8_675
Sn7 Cs3 Sn7 92.581(16) 13_575 8_675
Sn7 Cs3 Sn7 152.57(4) 6_465 8_675
Sn1 Cs3 Sn7 92.56(4) 6_465 8_675
Sn1 Cs3 Sn7 35.93(2) 13_575 8_675
Sn3 Cs3 Sn7 36.51(2) 7_565 8_675
Sn7 Cs3 Sn7 60.30(4) 15_675 8_675
Sn15 Cs3 Sn1 62.48(3) 13_575 7
Sn15 Cs3 Sn1 91.65(5) 6_465 7
Sn6 Cs3 Sn1 97.44(3) 13_575 7
Sn6 Cs3 Sn1 132.63(5) 6_465 7
Sn11 Cs3 Sn1 121.75(4) 8_675 7
Sn11 Cs3 Sn1 100.98(3) 15_675 7
Sn11 Cs3 Sn1 62.47(3) 7 7
Sn11 Cs3 Sn1 37.46(2) 16 7
Sn9 Cs3 Sn1 101.74(4) 5 7
Sn9 Cs3 Sn1 62.06(2) 13_675 7
Sn8 Cs3 Sn1 135.26(4) 7_565 7
Sn7 Cs3 Sn1 35.96(2) 13_575 7
Sn7 Cs3 Sn1 89.63(4) 6_465 7
Sn1 Cs3 Sn1 149.63(4) 6_465 7
Sn1 Cs3 Sn1 92.785(17) 13_575 7
Sn3 Cs3 Sn1 151.353(18) 7_565 7
Sn7 Cs3 Sn1 159.57(5) 15_675 7
Sn7 Cs3 Sn1 117.15(2) 8_675 7
Sn15 Cs3 Sn1 91.65(5) 13_575 16
Sn15 Cs3 Sn1 62.48(3) 6_465 16
Sn6 Cs3 Sn1 132.63(5) 13_575 16
Sn6 Cs3 Sn1 97.44(3) 6_465 16
Sn11 Cs3 Sn1 100.98(3) 8_675 16
Sn11 Cs3 Sn1 121.75(4) 15_675 16
Sn11 Cs3 Sn1 37.46(2) 7 16
Sn11 Cs3 Sn1 62.47(3) 16 16
Sn9 Cs3 Sn1 62.06(2) 5 16
Sn9 Cs3 Sn1 101.74(4) 13_675 16
Sn8 Cs3 Sn1 135.26(4) 7_565 16
Sn7 Cs3 Sn1 89.63(4) 13_575 16
Sn7 Cs3 Sn1 35.96(2) 6_465 16
Sn1 Cs3 Sn1 92.785(17) 6_465 16
Sn1 Cs3 Sn1 149.63(4) 13_575 16
Sn3 Cs3 Sn1 151.353(18) 7_565 16
Sn7 Cs3 Sn1 117.15(2) 15_675 16
Sn7 Cs3 Sn1 159.57(5) 8_675 16
Sn1 Cs3 Sn1 57.19(4) 7 16
Sn15 Cs3 Sn17 34.84(4) 13_575 15_665
Sn15 Cs3 Sn17 34.84(4) 6_465 15_665
Sn6 Cs3 Sn17 71.97(7) 13_575 15_665
Sn6 Cs3 Sn17 71.97(7) 6_465 15_665
Sn11 Cs3 Sn17 158.06(4) 8_675 15_665
Sn11 Cs3 Sn17 158.06(4) 15_675 15_665
Sn11 Cs3 Sn17 96.15(8) 7 15_665
Sn11 Cs3 Sn17 96.15(8) 16 15_665
Sn9 Cs3 Sn17 119.66(6) 5 15_665
Sn9 Cs3 Sn17 119.66(6) 13_675 15_665
Sn8 Cs3 Sn17 87.76(9) 7_565 15_665
Sn7 Cs3 Sn17 60.37(3) 13_575 15_665
Sn7 Cs3 Sn17 60.37(3) 6_465 15_665
Sn1 Cs3 Sn17 102.57(5) 6_465 15_665
Sn1 Cs3 Sn17 102.57(5) 13_575 15_665
Sn3 Cs3 Sn17 125.53(9) 7_565 15_665
Sn7 Cs3 Sn17 136.61(6) 15_675 15_665
Sn7 Cs3 Sn17 136.61(6) 8_675 15_665
Sn1 Cs3 Sn17 60.79(7) 7 15_665
Sn1 Cs3 Sn17 60.79(7) 16 15_665
Sn15 Cs3 Sn11 127.99(4) 13_575 13_576
Sn15 Cs3 Sn11 66.52(3) 6_465 13_576
Sn6 Cs3 Sn11 132.93(4) 13_575 13_576
Sn6 Cs3 Sn11 63.24(2) 6_465 13_576
Sn11 Cs3 Sn11 63.13(2) 8_675 13_576
Sn11 Cs3 Sn11 103.98(4) 15_675 13_576
Sn11 Cs3 Sn11 62.78(2) 7 13_576
Sn11 Cs3 Sn11 103.15(4) 16 13_576
Sn9 Cs3 Sn11 36.875(12) 5 13_576
Sn9 Cs3 Sn11 126.03(4) 13_675 13_576
Sn8 Cs3 Sn11 96.65(3) 7_565 13_576
Sn7 Cs3 Sn11 148.45(5) 13_575 13_576
Sn7 Cs3 Sn11 36.234(18) 6_465 13_576
Sn1 Cs3 Sn11 36.032(18) 6_465 13_576
Sn1 Cs3 Sn11 150.86(5) 13_575 13_576
Sn3 Cs3 Sn11 91.97(3) 7_565 13_576
Sn7 Cs3 Sn11 58.98(2) 15_675 13_576
Sn7 Cs3 Sn11 118.56(4) 8_675 13_576
Sn1 Cs3 Sn11 116.06(4) 7 13_576
Sn1 Cs3 Sn11 59.51(2) 16 13_576
Sn17 Cs3 Sn11 95.62(3) 15_665 13_576
Sn15 Cs3 Sn11 66.52(3) 13_575 6_464
Sn15 Cs3 Sn11 127.99(4) 6_465 6_464
Sn6 Cs3 Sn11 63.24(2) 13_575 6_464
Sn6 Cs3 Sn11 132.93(4) 6_465 6_464
Sn11 Cs3 Sn11 103.98(4) 8_675 6_464
Sn11 Cs3 Sn11 63.13(2) 15_675 6_464
Sn11 Cs3 Sn11 103.15(4) 7 6_464
Sn11 Cs3 Sn11 62.78(2) 16 6_464
Sn9 Cs3 Sn11 126.03(4) 5 6_464
Sn9 Cs3 Sn11 36.875(12) 13_675 6_464
Sn8 Cs3 Sn11 96.65(3) 7_565 6_464
Sn7 Cs3 Sn11 36.234(18) 13_575 6_464
Sn7 Cs3 Sn11 148.45(5) 6_465 6_464
Sn1 Cs3 Sn11 150.86(5) 6_465 6_464
Sn1 Cs3 Sn11 36.032(18) 13_575 6_464
Sn3 Cs3 Sn11 91.97(3) 7_565 6_464
Sn7 Cs3 Sn11 118.56(4) 15_675 6_464
Sn7 Cs3 Sn11 58.98(2) 8_675 6_464
Sn1 Cs3 Sn11 59.51(2) 7 6_464
Sn1 Cs3 Sn11 116.06(4) 16 6_464
Sn17 Cs3 Sn11 95.62(3) 15_665 6_464
Sn11 Cs3 Sn11 162.89(5) 13_576 6_464
Sn15 Cs3 Sn13 57.07(4) 13_575 15_665
Sn15 Cs3 Sn13 57.07(4) 6_465 15_665
Sn6 Cs3 Sn13 99.39(4) 13_575 15_665
Sn6 Cs3 Sn13 99.39(4) 6_465 15_665
Sn11 Cs3 Sn13 134.47(5) 8_675 15_665
Sn11 Cs3 Sn13 134.47(5) 15_675 15_665
Sn11 Cs3 Sn13 64.71(4) 7 15_665
Sn11 Cs3 Sn13 64.71(4) 16 15_665
Sn9 Cs3 Sn13 97.35(4) 5 15_665
Sn9 Cs3 Sn13 97.35(4) 13_675 15_665
Sn8 Cs3 Sn13 121.41(5) 7_565 15_665
Sn7 Cs3 Sn13 57.45(3) 13_575 15_665
Sn7 Cs3 Sn13 57.45(3) 6_465 15_665
Sn1 Cs3 Sn13 116.52(3) 6_465 15_665
Sn1 Cs3 Sn13 116.52(3) 13_575 15_665
Sn3 Cs3 Sn13 159.18(5) 7_565 15_665
Sn7 Cs3 Sn13 149.839(18) 15_675 15_665
Sn7 Cs3 Sn13 149.839(18) 8_675 15_665
Sn1 Cs3 Sn13 35.84(2) 7 15_665
Sn1 Cs3 Sn13 35.84(2) 16 15_665
Sn17 Cs3 Sn13 33.65(8) 15_665 15_665
Sn11 Cs3 Sn13 91.11(3) 13_576 15_665
Sn11 Cs3 Sn13 91.11(3) 6_464 15_665
Sn15 Cs3 Na1 34.14(11) 13_575 .
Sn15 Cs3 Na1 34.14(11) 6_465 .
Sn6 Cs3 Na1 70.6(2) 13_575 .
Sn6 Cs3 Na1 70.6(2) 6_465 .
Sn11 Cs3 Na1 158.58(8) 8_675 .
Sn11 Cs3 Na1 158.58(8) 15_675 .
Sn11 Cs3 Na1 97.7(3) 7 .
Sn11 Cs3 Na1 97.7(3) 16 .
Sn9 Cs3 Na1 120.63(16) 5 .
Sn9 Cs3 Na1 120.63(16) 13_675 .
Sn8 Cs3 Na1 86.1(3) 7_565 .
Sn7 Cs3 Na1 60.82(8) 13_575 .
Sn7 Cs3 Na1 60.82(8) 6_465 .
Sn1 Cs3 Na1 101.75(14) 6_465 .
Sn1 Cs3 Na1 101.75(14) 13_575 .
Sn3 Cs3 Na1 123.9(3) 7_565 .
Sn7 Cs3 Na1 135.47(19) 15_675 .
Sn7 Cs3 Na1 135.47(19) 8_675 .
Sn1 Cs3 Na1 62.2(2) 7 .
Sn1 Cs3 Na1 62.2(2) 16 .
Sn17 Cs3 Na1 1.7(3) 15_665 .
Sn11 Cs3 Na1 95.80(4) 13_576 .
Sn11 Cs3 Na1 95.80(4) 6_464 .
Sn13 Cs3 Na1 35.3(3) 15_665 .
Sn15 Cs3 Cs3 138.71(5) 13_575 9_675
Sn15 Cs3 Cs3 138.71(5) 6_465 9_675
Sn6 Cs3 Cs3 139.59(4) 13_575 9_675
Sn6 Cs3 Cs3 139.59(4) 6_465 9_675
Sn11 Cs3 Cs3 42.50(3) 8_675 9_675
Sn11 Cs3 Cs3 42.50(3) 15_675 9_675
Sn11 Cs3 Cs3 41.86(3) 7 9_675
Sn11 Cs3 Cs3 41.86(3) 16 9_675
Sn9 Cs3 Cs3 44.581(16) 5 9_675
Sn9 Cs3 Cs3 44.581(16) 13_675 9_675
Sn8 Cs3 Cs3 138.24(7) 7_565 9_675
Sn7 Cs3 Cs3 100.32(3) 13_575 9_675
Sn7 Cs3 Cs3 100.32(3) 6_465 9_675
Sn1 Cs3 Cs3 101.14(3) 6_465 9_675
Sn1 Cs3 Cs3 101.14(3) 13_575 9_675
Sn3 Cs3 Cs3 100.47(5) 7_565 9_675
Sn7 Cs3 Cs3 80.34(4) 15_675 9_675
Sn7 Cs3 Cs3 80.34(4) 8_675 9_675
Sn1 Cs3 Cs3 79.28(4) 7 9_675
Sn1 Cs3 Cs3 79.28(4) 16 9_675
Sn17 Cs3 Cs3 134.00(10) 15_665 9_675
Sn11 Cs3 Cs3 81.45(2) 13_576 9_675
Sn11 Cs3 Cs3 81.45(2) 6_464 9_675
Sn13 Cs3 Cs3 100.35(5) 15_665 9_675
Na1 Cs3 Cs3 135.7(3) . 9_675
Sn15 Cs3 Cs1 39.98(3) 13_575 9_665
Sn15 Cs3 Cs1 39.98(3) 6_465 9_665
Sn6 Cs3 Cs1 41.45(3) 13_575 9_665
Sn6 Cs3 Cs1 41.45(3) 6_465 9_665
Sn11 Cs3 Cs1 139.30(5) 8_675 9_665
Sn11 Cs3 Cs1 139.30(5) 15_675 9_665
Sn11 Cs3 Cs1 136.32(5) 7 9_665
Sn11 Cs3 Cs1 136.32(5) 16 9_665
Sn9 Cs3 Cs1 135.379(16) 5 9_665
Sn9 Cs3 Cs1 135.379(16) 13_675 9_665
Sn8 Cs3 Cs1 43.89(4) 7_565 9_665
Sn7 Cs3 Cs1 78.58(3) 13_575 9_665
Sn7 Cs3 Cs1 78.58(3) 6_465 9_665
Sn1 Cs3 Cs1 79.92(3) 6_465 9_665
Sn1 Cs3 Cs1 79.92(3) 13_575 9_665
Sn3 Cs3 Cs1 81.66(4) 7_565 9_665
Sn7 Cs3 Cs1 101.48(4) 15_675 9_665
Sn7 Cs3 Cs1 101.48(4) 8_675 9_665
Sn1 Cs3 Cs1 98.87(4) 7 9_665
Sn1 Cs3 Cs1 98.87(4) 16 9_665
Sn17 Cs3 Cs1 43.87(8) 15_665 9_665
Sn11 Cs3 Cs1 98.52(2) 13_576 9_665
Sn11 Cs3 Cs1 98.52(2) 6_464 9_665
Sn13 Cs3 Cs1 77.53(4) 15_665 9_665
Na1 Cs3 Cs1 42.2(3) . 9_665
Cs3 Cs3 Cs1 177.88(7) 9_675 9_665
Sn15 Cs3 Cs4 134.42(4) 13_575 15_675
Sn15 Cs3 Cs4 134.42(4) 6_465 15_675
Sn6 Cs3 Cs4 93.15(4) 13_575 15_675
Sn6 Cs3 Cs4 93.15(4) 6_465 15_675
Sn11 Cs3 Cs4 32.87(2) 8_675 15_675
Sn11 Cs3 Cs4 32.87(2) 15_675 15_675
Sn11 Cs3 Cs4 101.03(3) 7 15_675
Sn11 Cs3 Cs4 101.03(3) 16 15_675
Sn9 Cs3 Cs4 72.02(3) 5 15_675
Sn9 Cs3 Cs4 72.02(3) 13_675 15_675
Sn8 Cs3 Cs4 73.92(4) 7_565 15_675
Sn7 Cs3 Cs4 122.76(3) 13_575 15_675
Sn7 Cs3 Cs4 122.76(3) 6_465 15_675
Sn1 Cs3 Cs4 69.08(3) 6_465 15_675
Sn1 Cs3 Cs4 69.08(3) 13_575 15_675
Sn3 Cs3 Cs4 36.14(3) 7_565 15_675
Sn7 Cs3 Cs4 33.155(19) 15_675 15_675
Sn7 Cs3 Cs4 33.155(19) 8_675 15_675
Sn1 Cs3 Cs4 133.84(3) 7 15_675
Sn1 Cs3 Cs4 133.84(3) 16 15_675
Sn17 Cs3 Cs4 161.68(9) 15_665 15_675
Sn11 Cs3 Cs4 86.69(3) 13_576 15_675
Sn11 Cs3 Cs4 86.69(3) 6_464 15_675
Sn13 Cs3 Cs4 164.67(4) 15_665 15_675
Na1 Cs3 Cs4 160.0(3) . 15_675
Cs3 Cs3 Cs4 64.32(4) 9_675 15_675
Cs1 Cs3 Cs4 117.80(4) 9_665 15_675
Sn15 Cs3 Cs4 36.61(2) 13_575 13_575
Sn15 Cs3 Cs4 96.61(4) 6_465 13_575
Sn6 Cs3 Cs4 32.356(18) 13_575 13_575
Sn6 Cs3 Cs4 100.32(3) 6_465 13_575
Sn11 Cs3 Cs4 130.90(3) 8_675 13_575
Sn11 Cs3 Cs4 91.56(2) 15_675 13_575
Sn11 Cs3 Cs4 129.02(3) 7 13_575
Sn11 Cs3 Cs4 90.56(2) 16 13_575
Sn9 Cs3 Cs4 161.02(3) 5 13_575
Sn9 Cs3 Cs4 71.895(11) 13_675 13_575
Sn8 Cs3 Cs4 71.45(2) 7_565 13_575
Sn7 Cs3 Cs4 32.703(18) 13_575 13_575
Sn7 Cs3 Cs4 131.28(4) 6_465 13_575
Sn1 Cs3 Cs4 133.28(4) 6_465 13_575
Sn1 Cs3 Cs4 33.200(18) 13_575 13_575
Sn3 Cs3 Cs4 86.57(2) 7_565 13_575
Sn7 Cs3 Cs4 122.85(4) 15_675 13_575
Sn7 Cs3 Cs4 69.114(19) 8_675 13_575
Sn1 Cs3 Cs4 68.662(19) 7 13_575
Sn1 Cs3 Cs4 119.53(4) 16 13_575
Sn17 Cs3 Cs4 71.03(3) 15_665 13_575
Sn11 Cs3 Cs4 162.00(4) 13_576 13_575
Sn11 Cs3 Cs4 35.024(17) 6_464 13_575
Sn13 Cs3 Cs4 84.19(2) 15_665 13_575
Na1 Cs3 Cs4 70.50(9) . 13_575
Cs3 Cs3 Cs4 116.466(16) 9_675 13_575
Cs1 Cs3 Cs4 63.503(16) 9_665 13_575
Cs4 Cs3 Cs4 102.27(2) 15_675 13_575
Sn15 Cs3 Cs4 96.61(4) 13_575 13_576
Sn15 Cs3 Cs4 36.61(2) 6_465 13_576
Sn6 Cs3 Cs4 100.32(3) 13_575 13_576
Sn6 Cs3 Cs4 32.356(18) 6_465 13_576
Sn11 Cs3 Cs4 91.56(2) 8_675 13_576
Sn11 Cs3 Cs4 130.90(3) 15_675 13_576
Sn11 Cs3 Cs4 90.56(2) 7 13_576
Sn11 Cs3 Cs4 129.02(3) 16 13_576
Sn9 Cs3 Cs4 71.895(11) 5 13_576
Sn9 Cs3 Cs4 161.02(3) 13_675 13_576
Sn8 Cs3 Cs4 71.45(2) 7_565 13_576
Sn7 Cs3 Cs4 131.28(4) 13_575 13_576
Sn7 Cs3 Cs4 32.703(18) 6_465 13_576
Sn1 Cs3 Cs4 33.200(18) 6_465 13_576
Sn1 Cs3 Cs4 133.28(4) 13_575 13_576
Sn3 Cs3 Cs4 86.57(2) 7_565 13_576
Sn7 Cs3 Cs4 69.114(19) 15_675 13_576
Sn7 Cs3 Cs4 122.85(4) 8_675 13_576
Sn1 Cs3 Cs4 119.53(4) 7 13_576
Sn1 Cs3 Cs4 68.662(19) 16 13_576
Sn17 Cs3 Cs4 71.03(3) 15_665 13_576
Sn11 Cs3 Cs4 35.024(17) 13_576 13_576
Sn11 Cs3 Cs4 162.00(4) 6_464 13_576
Sn13 Cs3 Cs4 84.19(2) 15_665 13_576
Na1 Cs3 Cs4 70.50(9) . 13_576
Cs3 Cs3 Cs4 116.466(16) 9_675 13_576
Cs1 Cs3 Cs4 63.503(16) 9_665 13_576
Cs4 Cs3 Cs4 102.27(2) 15_675 13_576
Cs4 Cs3 Cs4 127.00(3) 13_575 13_576
Sn4 Cs4 Sn4 44.17(4) 9_665 2_665
Sn4 Cs4 Sn7 106.74(3) 9_665 10
Sn4 Cs4 Sn7 137.41(4) 2_665 10
Sn4 Cs4 Sn7 137.41(4) 9_665 .
Sn4 Cs4 Sn7 106.74(3) 2_665 .
Sn7 Cs4 Sn7 73.15(4) 10 .
Sn4 Cs4 Sn1 108.62(3) 9_665 10
Sn4 Cs4 Sn1 138.32(4) 2_665 10
Sn7 Cs4 Sn1 71.69(3) 10 10
Sn7 Cs4 Sn1 111.31(4) . 10
Sn4 Cs4 Sn1 138.32(4) 9_665 .
Sn4 Cs4 Sn1 108.62(3) 2_665 .
Sn7 Cs4 Sn1 111.31(4) 10 .
Sn7 Cs4 Sn1 71.69(3) . .
Sn1 Cs4 Sn1 69.29(4) 10 .
Sn4 Cs4 Sn5 72.26(3) 9_665 .
Sn4 Cs4 Sn5 72.26(3) 2_665 .
Sn7 Cs4 Sn5 137.05(3) 10 .
Sn7 Cs4 Sn5 137.05(3) . .
Sn1 Cs4 Sn5 68.52(3) 10 .
Sn1 Cs4 Sn5 68.51(3) . .
Sn4 Cs4 Sn11 179.08(3) 9_665 10
Sn4 Cs4 Sn11 136.64(2) 2_665 10
Sn7 Cs4 Sn11 72.34(3) 10 10
Sn7 Cs4 Sn11 42.62(2) . 10
Sn1 Cs4 Sn11 71.02(3) 10 10
Sn1 Cs4 Sn11 42.46(2) . 10
Sn5 Cs4 Sn11 108.28(4) . 10
Sn4 Cs4 Sn11 136.64(2) 9_665 .
Sn4 Cs4 Sn11 179.08(3) 2_665 .
Sn7 Cs4 Sn11 42.63(2) 10 .
Sn7 Cs4 Sn11 72.34(3) . .
Sn1 Cs4 Sn11 42.46(2) 10 .
Sn1 Cs4 Sn11 71.02(3) . .
Sn5 Cs4 Sn11 108.28(4) . .
Sn11 Cs4 Sn11 42.55(3) 10 .
Sn4 Cs4 Sn6 110.80(4) 9_665 .
Sn4 Cs4 Sn6 69.43(3) 2_665 .
Sn7 Cs4 Sn6 139.33(4) 10 .
Sn7 Cs4 Sn6 68.84(2) . .
Sn1 Cs4 Sn6 109.33(4) 10 .
Sn1 Cs4 Sn6 42.53(2) . .
Sn5 Cs4 Sn6 71.14(2) . .
Sn11 Cs4 Sn6 70.12(2) 10 .
Sn11 Cs4 Sn6 109.98(3) . .
Sn4 Cs4 Sn6 69.43(3) 9_665 10
Sn4 Cs4 Sn6 110.79(4) 2_665 10
Sn7 Cs4 Sn6 68.84(2) 10 10
Sn7 Cs4 Sn6 139.33(4) . 10
Sn1 Cs4 Sn6 42.54(2) 10 10
Sn1 Cs4 Sn6 109.33(4) . 10
Sn5 Cs4 Sn6 71.13(2) . 10
Sn11 Cs4 Sn6 109.98(3) 10 10
Sn11 Cs4 Sn6 70.12(2) . 10
Sn6 Cs4 Sn6 139.87(5) . 10
Sn4 Cs4 Sn10 73.23(3) 9_665 2_665
Sn4 Cs4 Sn10 42.52(3) 2_665 2_665
Sn7 Cs4 Sn10 108.81(4) 10 2_665
Sn7 Cs4 Sn10 67.15(3) . 2_665
Sn1 Cs4 Sn10 177.93(3) 10 2_665
Sn1 Cs4 Sn10 108.74(2) . 2_665
Sn5 Cs4 Sn10 111.54(4) . 2_665
Sn11 Cs4 Sn10 107.14(3) 10 2_665
Sn11 Cs4 Sn10 136.68(4) . 2_665
Sn6 Cs4 Sn10 68.92(3) . 2_665
Sn6 Cs4 Sn10 139.53(4) 10 2_665
Sn4 Cs4 Sn10 42.52(3) 9_665 9_665
Sn4 Cs4 Sn10 73.23(3) 2_665 9_665
Sn7 Cs4 Sn10 67.15(3) 10 9_665
Sn7 Cs4 Sn10 108.81(4) . 9_665
Sn1 Cs4 Sn10 108.74(2) 10 9_665
Sn1 Cs4 Sn10 177.93(3) . 9_665
Sn5 Cs4 Sn10 111.54(4) . 9_665
Sn11 Cs4 Sn10 136.68(4) 10 9_665
Sn11 Cs4 Sn10 107.14(3) . 9_665
Sn6 Cs4 Sn10 139.53(4) . 9_665
Sn6 Cs4 Sn10 68.92(3) 10 9_665
Sn10 Cs4 Sn10 73.22(4) 2_665 9_665
Sn4 Cs4 Sn2 71.12(3) 9_665 9_665
Sn4 Cs4 Sn2 71.12(3) 2_665 9_665
Sn7 Cs4 Sn2 69.34(3) 10 9_665
Sn7 Cs4 Sn2 69.34(3) . 9_665
Sn1 Cs4 Sn2 138.76(3) 10 9_665
Sn1 Cs4 Sn2 138.76(3) . 9_665
Sn5 Cs4 Sn2 140.37(4) . 9_665
Sn11 Cs4 Sn2 108.55(4) 10 9_665
Sn11 Cs4 Sn2 108.55(4) . 9_665
Sn6 Cs4 Sn2 108.79(2) . 9_665
Sn6 Cs4 Sn2 108.79(2) 10 9_665
Sn10 Cs4 Sn2 42.43(3) 2_665 9_665
Sn10 Cs4 Sn2 42.43(3) 9_665 9_665
Sn4 Cs4 Sn12 42.28(3) 9_665 10
Sn4 Cs4 Sn12 72.70(3) 2_665 10
Sn7 Cs4 Sn12 107.38(2) 10 10
Sn7 Cs4 Sn12 179.41(3) . 10
Sn1 Cs4 Sn12 69.17(3) 10 10
Sn1 Cs4 Sn12 108.26(4) . 10
Sn5 Cs4 Sn12 42.68(2) . 10
Sn11 Cs4 Sn12 137.70(4) 10 10
Sn11 Cs4 Sn12 108.21(3) . 10
Sn6 Cs4 Sn12 110.71(4) . 10
Sn6 Cs4 Sn12 41.26(2) 10 10
Sn10 Cs4 Sn12 112.36(4) 2_665 10
Sn10 Cs4 Sn12 71.26(3) 9_665 10
Sn2 Cs4 Sn12 110.57(3) 9_665 10
Sn4 Cs4 Sn12 72.70(3) 9_665 .
Sn4 Cs4 Sn12 42.28(3) 2_665 .
Sn7 Cs4 Sn12 179.41(3) 10 .
Sn7 Cs4 Sn12 107.38(2) . .
Sn1 Cs4 Sn12 108.26(4) 10 .
Sn1 Cs4 Sn12 69.17(3) . .
Sn5 Cs4 Sn12 42.68(2) . .
Sn11 Cs4 Sn12 108.21(3) 10 .
Sn11 Cs4 Sn12 137.70(4) . .
Sn6 Cs4 Sn12 41.26(2) . .
Sn6 Cs4 Sn12 110.71(4) 10 .
Sn10 Cs4 Sn12 71.26(3) 2_665 .
Sn10 Cs4 Sn12 112.37(4) 9_665 .
Sn2 Cs4 Sn12 110.57(3) 9_665 .
Sn12 Cs4 Sn12 72.09(4) 10 .
Sn4 Cs4 Sn3 109.64(4) 9_665 9_665
Sn4 Cs4 Sn3 109.64(4) 2_665 9_665
Sn7 Cs4 Sn3 41.98(2) 10 9_665
Sn7 Cs4 Sn3 41.98(2) . 9_665
Sn1 Cs4 Sn3 109.83(3) 10 9_665
Sn1 Cs4 Sn3 109.83(3) . 9_665
Sn5 Cs4 Sn3 177.92(5) . 9_665
Sn11 Cs4 Sn3 69.80(3) 10 9_665
Sn11 Cs4 Sn3 69.80(3) . 9_665
Sn6 Cs4 Sn3 108.60(2) . 9_665
Sn6 Cs4 Sn3 108.60(2) 10 9_665
Sn10 Cs4 Sn3 70.06(3) 2_665 9_665
Sn10 Cs4 Sn3 70.06(3) 9_665 9_665
Sn2 Cs4 Sn3 41.71(3) 9_665 9_665
Sn12 Cs4 Sn3 138.32(3) 10 9_665
Sn12 Cs4 Sn3 138.32(3) . 9_665
Sn4 Cs4 Sn15 110.30(4) 9_665 .
Sn4 Cs4 Sn15 69.06(3) 2_665 .
Sn7 Cs4 Sn15 110.93(4) 10 .
Sn7 Cs4 Sn15 40.62(2) . .
Sn1 Cs4 Sn15 137.88(4) 10 .
Sn1 Cs4 Sn15 71.14(2) . .
Sn5 Cs4 Sn15 109.20(2) . .
Sn11 Cs4 Sn15 70.29(2) 10 .
Sn11 Cs4 Sn15 110.03(3) . .
Sn6 Cs4 Sn15 40.57(2) . .
Sn6 Cs4 Sn15 179.51(4) 10 .
Sn10 Cs4 Sn15 40.06(2) 2_665 .
Sn10 Cs4 Sn15 110.60(4) 9_665 .
Sn2 Cs4 Sn15 70.72(2) 9_665 .
Sn12 Cs4 Sn15 138.79(4) 10 .
Sn12 Cs4 Sn15 69.52(2) . .
Sn3 Cs4 Sn15 71.07(2) 9_665 .
Sn4 Cs4 Sn15 69.06(3) 9_665 10
Sn4 Cs4 Sn15 110.30(4) 2_665 10
Sn7 Cs4 Sn15 40.62(2) 10 10
Sn7 Cs4 Sn15 110.93(4) . 10
Sn1 Cs4 Sn15 71.14(2) 10 10
Sn1 Cs4 Sn15 137.87(4) . 10
Sn5 Cs4 Sn15 109.20(2) . 10
Sn11 Cs4 Sn15 110.03(3) 10 10
Sn11 Cs4 Sn15 70.29(2) . 10
Sn6 Cs4 Sn15 179.51(4) . 10
Sn6 Cs4 Sn15 40.57(2) 10 10
Sn10 Cs4 Sn15 110.60(4) 2_665 10
Sn10 Cs4 Sn15 40.06(2) 9_665 10
Sn2 Cs4 Sn15 70.72(2) 9_665 10
Sn12 Cs4 Sn15 69.52(2) 10 10
Sn12 Cs4 Sn15 138.79(4) . 10
Sn3 Cs4 Sn15 71.08(2) 9_665 10
Sn15 Cs4 Sn15 138.99(5) . 10
Sn4 Cs4 Sn13 109.96(4) 9_665 9_665
Sn4 Cs4 Sn13 109.96(4) 2_665 9_665
Sn7 Cs4 Sn13 109.76(3) 10 9_665
Sn7 Cs4 Sn13 109.76(3) . 9_665
Sn1 Cs4 Sn13 40.65(2) 10 9_665
Sn1 Cs4 Sn13 40.65(2) . 9_665
Sn5 Cs4 Sn13 40.81(3) . 9_665
Sn11 Cs4 Sn13 70.37(3) 10 9_665
Sn11 Cs4 Sn13 70.37(3) . 9_665
Sn6 Cs4 Sn13 71.36(2) . 9_665
Sn6 Cs4 Sn13 71.36(2) 10 9_665
Sn10 Cs4 Sn13 138.11(3) 2_665 9_665
Sn10 Cs4 Sn13 138.11(3) 9_665 9_665
Sn2 Cs4 Sn13 178.83(5) 9_665 9_665
Sn12 Cs4 Sn13 70.35(3) 10 9_665
Sn12 Cs4 Sn13 70.35(3) . 9_665
Sn3 Cs4 Sn13 137.11(4) 9_665 9_665
Sn15 Cs4 Sn13 109.13(2) . 9_665
Sn15 Cs4 Sn13 109.13(2) 10 9_665
Sn4 Cs4 Cs5 36.86(2) 9_665 3_554
Sn4 Cs4 Cs5 36.86(2) 2_665 3_554
Sn7 Cs4 Cs5 140.46(2) 10 3_554
Sn7 Cs4 Cs5 140.46(2) . 3_554
Sn1 Cs4 Cs5 101.54(3) 10 3_554
Sn1 Cs4 Cs5 101.54(3) . 3_554
Sn5 Cs4 Cs5 40.51(2) . 3_554
Sn11 Cs4 Cs5 143.95(3) 10 3_554
Sn11 Cs4 Cs5 143.95(3) . 3_554
Sn6 Cs4 Cs5 80.13(2) . 3_554
Sn6 Cs4 Cs5 80.13(2) 10 3_554
Sn10 Cs4 Cs5 79.37(3) 2_665 3_554
Sn10 Cs4 Cs5 79.37(3) 9_665 3_554
Sn2 Cs4 Cs5 99.86(3) 9_665 3_554
Sn12 Cs4 Cs5 38.955(19) 10 3_554
Sn12 Cs4 Cs5 38.956(19) . 3_554
Sn3 Cs4 Cs5 141.57(3) 9_665 3_554
Sn15 Cs4 Cs5 99.89(2) . 3_554
Sn15 Cs4 Cs5 99.89(2) 10 3_554
Sn13 Cs4 Cs5 81.32(3) 9_665 3_554
Sn4 Cs4 Cs4 36.19(2) 9_665 7
Sn4 Cs4 Cs4 36.19(2) 2_665 7
Sn7 Cs4 Cs4 101.25(2) 10 7
Sn7 Cs4 Cs4 101.25(2) . 7
Sn1 Cs4 Cs4 142.19(2) 10 7
Sn1 Cs4 Cs4 142.19(2) . 7
Sn5 Cs4 Cs4 100.24(3) . 7
Sn11 Cs4 Cs4 143.87(2) 10 7
Sn11 Cs4 Cs4 143.87(2) . 7
Sn6 Cs4 Cs4 99.81(2) . 7
Sn6 Cs4 Cs4 99.81(2) 10 7
Sn10 Cs4 Cs4 39.85(2) 2_665 7
Sn10 Cs4 Cs4 39.85(2) 9_665 7
Sn2 Cs4 Cs4 40.13(3) 9_665 7
Sn12 Cs4 Cs4 78.42(2) 10 7
Sn12 Cs4 Cs4 78.42(2) . 7
Sn3 Cs4 Cs4 81.84(3) 9_665 7
Sn15 Cs4 Cs4 79.80(2) . 7
Sn15 Cs4 Cs4 79.80(2) 10 7
Sn13 Cs4 Cs4 141.05(3) 9_665 7
Cs5 Cs4 Cs4 59.730(12) 3_554 7
Sn4 Cs4 Cs2 79.29(3) 9_665 4_554
Sn4 Cs4 Cs2 99.23(3) 2_665 4_554
Sn7 Cs4 Cs2 104.49(2) 10 4_554
Sn7 Cs4 Cs2 143.04(4) . 4_554
Sn1 Cs4 Cs2 39.12(2) 10 4_554
Sn1 Cs4 Cs2 75.39(3) . 4_554
Sn5 Cs4 Cs2 32.574(19) . 4_554
Sn11 Cs4 Cs2 100.77(3) 10 4_554
Sn11 Cs4 Cs2 81.52(3) . 4_554
Sn6 Cs4 Cs2 97.36(3) . 4_554
Sn6 Cs4 Cs2 42.52(3) 10 4_554
Sn10 Cs4 Cs2 141.55(4) 2_665 4_554
Sn10 Cs4 Cs2 103.52(3) 9_665 4_554
Sn2 Cs4 Cs2 145.78(3) 9_665 4_554
Sn12 Cs4 Cs2 37.20(3) 10 4_554
Sn12 Cs4 Cs2 75.25(3) . 4_554
Sn3 Cs4 Cs2 146.31(2) 9_665 4_554
Sn15 Cs4 Cs2 137.92(3) . 4_554
Sn15 Cs4 Cs2 83.07(3) 10 4_554
Sn13 Cs4 Cs2 34.91(3) 9_665 4_554
Cs5 Cs4 Cs2 62.64(2) 3_554 4_554
Cs4 Cs4 Cs2 115.10(2) 7 4_554
Sn4 Cs4 Cs2 99.23(3) 9_665 11_666
Sn4 Cs4 Cs2 79.29(3) 2_665 11_666
Sn7 Cs4 Cs2 143.04(4) 10 11_666
Sn7 Cs4 Cs2 104.49(2) . 11_666
Sn1 Cs4 Cs2 75.39(3) 10 11_666
Sn1 Cs4 Cs2 39.12(2) . 11_666
Sn5 Cs4 Cs2 32.574(19) . 11_666
Sn11 Cs4 Cs2 81.52(3) 10 11_666
Sn11 Cs4 Cs2 100.77(3) . 11_666
Sn6 Cs4 Cs2 42.52(3) . 11_666
Sn6 Cs4 Cs2 97.36(3) 10 11_666
Sn10 Cs4 Cs2 103.52(3) 2_665 11_666
Sn10 Cs4 Cs2 141.55(4) 9_665 11_666
Sn2 Cs4 Cs2 145.78(3) 9_665 11_666
Sn12 Cs4 Cs2 75.25(3) 10 11_666
Sn12 Cs4 Cs2 37.20(3) . 11_666
Sn3 Cs4 Cs2 146.31(2) 9_665 11_666
Sn15 Cs4 Cs2 83.07(3) . 11_666
Sn15 Cs4 Cs2 137.92(3) 10 11_666
Sn13 Cs4 Cs2 34.91(3) 9_665 11_666
Cs5 Cs4 Cs2 62.64(2) 3_554 11_666
Cs4 Cs4 Cs2 115.10(2) 7 11_666
Cs2 Cs4 Cs2 54.85(4) 4_554 11_666
Sn4 Cs4 Cs3 145.00(3) 9_665 15_765
Sn4 Cs4 Cs3 145.00(3) 2_665 15_765
Sn7 Cs4 Cs3 40.45(2) 10 15_765
Sn7 Cs4 Cs3 40.45(2) . 15_765
Sn1 Cs4 Cs3 76.48(3) 10 15_765
Sn1 Cs4 Cs3 76.48(3) . 15_765
Sn5 Cs4 Cs3 137.06(4) . 15_765
Sn11 Cs4 Cs3 34.17(2) 10 15_765
Sn11 Cs4 Cs3 34.17(2) . 15_765
Sn6 Cs4 Cs3 99.12(2) . 15_765
Sn6 Cs4 Cs3 99.12(2) 10 15_765
Sn10 Cs4 Cs3 102.56(3) 2_665 15_765
Sn10 Cs4 Cs3 102.56(3) 9_665 15_765
Sn2 Cs4 Cs3 82.58(3) 9_665 15_765
Sn12 Cs4 Cs3 140.13(2) 10 15_765
Sn12 Cs4 Cs3 140.13(2) . 15_765
Sn3 Cs4 Cs3 40.86(3) 9_665 15_765
Sn15 Cs4 Cs3 80.87(2) . 15_765
Sn15 Cs4 Cs3 80.87(2) 10 15_765
Sn13 Cs4 Cs3 96.25(3) 9_665 15_765
Cs5 Cs4 Cs3 177.57(3) 3_554 15_765
Cs4 Cs4 Cs3 122.703(19) 7 15_765
Cs2 Cs4 Cs3 115.27(3) 4_554 15_765
Cs2 Cs4 Cs3 115.27(3) 11_666 15_765
Sn4 Cs4 Cs3 138.58(3) 9_665 13_676
Sn4 Cs4 Cs3 94.41(2) 2_665 13_676
Sn7 Cs4 Cs3 106.82(3) 10 13_676
Sn7 Cs4 Cs3 38.99(2) . 13_676
Sn1 Cs4 Cs3 104.44(3) 10 13_676
Sn1 Cs4 Cs3 39.82(2) . 13_676
Sn5 Cs4 Cs3 98.19(2) . 13_676
Sn11 Cs4 Cs3 42.230(19) 10 13_676
Sn11 Cs4 Cs3 84.78(2) . 13_676
Sn6 Cs4 Cs3 32.54(2) . 13_676
Sn6 Cs4 Cs3 146.95(4) 10 13_676
Sn10 Cs4 Cs3 73.49(2) 2_665 13_676
Sn10 Cs4 Cs3 141.56(4) 9_665 13_676
Sn2 Cs4 Cs3 99.21(2) 9_665 13_676
Sn12 Cs4 Cs3 140.69(3) 10 13_676
Sn12 Cs4 Cs3 73.77(2) . 13_676
Sn3 Cs4 Cs3 80.93(2) 9_665 13_676
Sn15 Cs4 Cs3 33.47(2) . 13_676
Sn15 Cs4 Cs3 147.39(4) 10 13_676
Sn13 Cs4 Cs3 80.30(2) 9_665 13_676
Cs5 Cs4 Cs3 112.518(18) 3_554 13_676
Cs4 Cs4 Cs3 113.003(18) 7 13_676
Cs2 Cs4 Cs3 114.48(3) 4_554 13_676
Cs2 Cs4 Cs3 65.79(2) 11_666 13_676
Cs3 Cs4 Cs3 66.90(2) 15_765 13_676
Sn4 Cs4 Cs3 94.41(2) 9_665 13_675
Sn4 Cs4 Cs3 138.58(3) 2_665 13_675
Sn7 Cs4 Cs3 38.99(2) 10 13_675
Sn7 Cs4 Cs3 106.82(3) . 13_675
Sn1 Cs4 Cs3 39.82(2) 10 13_675
Sn1 Cs4 Cs3 104.44(3) . 13_675
Sn5 Cs4 Cs3 98.19(2) . 13_675
Sn11 Cs4 Cs3 84.78(2) 10 13_675
Sn11 Cs4 Cs3 42.230(19) . 13_675
Sn6 Cs4 Cs3 146.95(4) . 13_675
Sn6 Cs4 Cs3 32.54(2) 10 13_675
Sn10 Cs4 Cs3 141.56(4) 2_665 13_675
Sn10 Cs4 Cs3 73.49(2) 9_665 13_675
Sn2 Cs4 Cs3 99.21(2) 9_665 13_675
Sn12 Cs4 Cs3 73.77(2) 10 13_675
Sn12 Cs4 Cs3 140.69(3) . 13_675
Sn3 Cs4 Cs3 80.93(2) 9_665 13_675
Sn15 Cs4 Cs3 147.39(4) . 13_675
Sn15 Cs4 Cs3 33.47(2) 10 13_675
Sn13 Cs4 Cs3 80.30(2) 9_665 13_675
Cs5 Cs4 Cs3 112.518(18) 3_554 13_675
Cs4 Cs4 Cs3 113.003(18) 7 13_675
Cs2 Cs4 Cs3 65.79(2) 4_554 13_675
Cs2 Cs4 Cs3 114.48(3) 11_666 13_675
Cs3 Cs4 Cs3 66.90(2) 15_765 13_675
Cs3 Cs4 Cs3 127.00(3) 13_676 13_675
Sn4 Cs4 Cs3 146.63(3) 9_665 7
Sn4 Cs4 Cs3 146.63(3) 2_665 7
Sn7 Cs4 Cs3 75.77(3) 10 7
Sn7 Cs4 Cs3 75.77(3) . 7
Sn1 Cs4 Cs3 39.35(2) 10 7
Sn1 Cs4 Cs3 39.35(2) . 7
Sn5 Cs4 Cs3 83.52(3) . 7
Sn11 Cs4 Cs3 33.23(2) 10 7
Sn11 Cs4 Cs3 33.23(2) . 7
Sn6 Cs4 Cs3 81.35(2) . 7
Sn6 Cs4 Cs3 81.35(2) 10 7
Sn10 Cs4 Cs3 138.65(2) 2_665 7
Sn10 Cs4 Cs3 138.65(2) 9_665 7
Sn2 Cs4 Cs3 136.11(4) 9_665 7
Sn12 Cs4 Cs3 104.58(3) 10 7
Sn12 Cs4 Cs3 104.58(3) . 7
Sn3 Cs4 Cs3 94.40(3) 9_665 7
Sn15 Cs4 Cs3 99.02(2) . 7
Sn15 Cs4 Cs3 99.02(2) 10 7
Sn13 Cs4 Cs3 42.71(3) 9_665 7
Cs5 Cs4 Cs3 124.03(3) 3_554 7
Cs4 Cs4 Cs3 176.237(18) 7 7
Cs2 Cs4 Cs3 68.16(3) 4_554 7
Cs2 Cs4 Cs3 68.16(3) 11_666 7
Cs3 Cs4 Cs3 53.53(3) 15_765 7
Cs3 Cs4 Cs3 66.17(2) 13_676 7
Cs3 Cs4 Cs3 66.17(2) 13_675 7
Sn4 Cs4 Cs2 99.27(3) 9_665 2_665
Sn4 Cs4 Cs2 80.87(3) 2_665 2_665
Sn7 Cs4 Cs2 74.06(3) 10 2_665
Sn7 Cs4 Cs2 38.61(2) . 2_665
Sn1 Cs4 Cs2 140.65(4) 10 2_665
Sn1 Cs4 Cs2 106.85(3) . 2_665
Sn5 Cs4 Cs2 148.78(3) . 2_665
Sn11 Cs4 Cs2 80.65(2) 10 2_665
Sn11 Cs4 Cs2 98.40(3) . 2_665
Sn6 Cs4 Cs2 84.90(3) . 2_665
Sn6 Cs4 Cs2 135.23(3) 10 2_665
Sn10 Cs4 Cs2 38.81(3) 2_665 2_665
Sn10 Cs4 Cs2 74.22(3) 9_665 2_665
Sn2 Cs4 Cs2 32.043(19) 9_665 2_665
Sn12 Cs4 Cs2 141.17(3) 10 2_665
Sn12 Cs4 Cs2 106.18(3) . 2_665
Sn3 Cs4 Cs2 32.45(2) 9_665 2_665
Sn15 Cs4 Cs2 44.33(3) . 2_665
Sn15 Cs4 Cs2 94.66(3) 10 2_665
Sn13 Cs4 Cs2 147.24(2) 9_665 2_665
Cs5 Cs4 Cs2 117.24(2) 3_554 2_665
Cs4 Cs4 Cs2 63.661(13) 7 2_665
Cs2 Cs4 Cs2 177.63(4) 4_554 2_665
Cs2 Cs4 Cs2 127.404(5) 11_666 2_665
Cs3 Cs4 Cs2 64.91(2) 15_765 2_665
Cs3 Cs4 Cs2 67.85(2) 13_676 2_665
Cs3 Cs4 Cs2 112.59(3) 13_675 2_665
Cs3 Cs4 Cs2 113.01(2) 7 2_665
Sn4 Cs4 Cs2 80.87(3) 9_665 9_665
Sn4 Cs4 Cs2 99.27(3) 2_665 9_665
Sn7 Cs4 Cs2 38.61(2) 10 9_665
Sn7 Cs4 Cs2 74.06(3) . 9_665
Sn1 Cs4 Cs2 106.85(3) 10 9_665
Sn1 Cs4 Cs2 140.65(4) . 9_665
Sn5 Cs4 Cs2 148.78(3) . 9_665
Sn11 Cs4 Cs2 98.40(3) 10 9_665
Sn11 Cs4 Cs2 80.65(2) . 9_665
Sn6 Cs4 Cs2 135.23(3) . 9_665
Sn6 Cs4 Cs2 84.90(3) 10 9_665
Sn10 Cs4 Cs2 74.22(3) 2_665 9_665
Sn10 Cs4 Cs2 38.81(3) 9_665 9_665
Sn2 Cs4 Cs2 32.043(19) 9_665 9_665
Sn12 Cs4 Cs2 106.18(3) 10 9_665
Sn12 Cs4 Cs2 141.17(3) . 9_665
Sn3 Cs4 Cs2 32.45(2) 9_665 9_665
Sn15 Cs4 Cs2 94.66(3) . 9_665
Sn15 Cs4 Cs2 44.33(3) 10 9_665
Sn13 Cs4 Cs2 147.24(2) 9_665 9_665
Cs5 Cs4 Cs2 117.24(2) 3_554 9_665
Cs4 Cs4 Cs2 63.661(13) 7 9_665
Cs2 Cs4 Cs2 127.404(5) 4_554 9_665
Cs2 Cs4 Cs2 177.63(4) 11_666 9_665
Cs3 Cs4 Cs2 64.91(2) 15_765 9_665
Cs3 Cs4 Cs2 112.59(3) 13_676 9_665
Cs3 Cs4 Cs2 67.85(2) 13_675 9_665
Cs3 Cs4 Cs2 113.01(2) 7 9_665
Cs2 Cs4 Cs2 50.33(4) 2_665 9_665
Sn4 Cs5 Sn4 180.00(2) 12_656 4_455
Sn4 Cs5 Sn4 135.86(4) 12_656 11_566
Sn4 Cs5 Sn4 44.14(4) 4_455 11_566
Sn4 Cs5 Sn4 44.14(4) 12_656 3_545
Sn4 Cs5 Sn4 135.86(4) 4_455 3_545
Sn4 Cs5 Sn4 180.0 11_566 3_545
Sn4 Cs5 Sn12 74.07(2) 12_656 13_566
Sn4 Cs5 Sn12 105.93(2) 4_455 13_566
Sn4 Cs5 Sn12 136.938(19) 11_566 13_566
Sn4 Cs5 Sn12 43.062(19) 3_545 13_566
Sn4 Cs5 Sn12 105.93(2) 12_656 5_545
Sn4 Cs5 Sn12 74.07(2) 4_455 5_545
Sn4 Cs5 Sn12 43.062(19) 11_566 5_545
Sn4 Cs5 Sn12 136.938(19) 3_545 5_545
Sn12 Cs5 Sn12 180.0 13_566 5_545
Sn4 Cs5 Sn12 43.062(19) 12_656 11_566
Sn4 Cs5 Sn12 136.938(19) 4_455 11_566
Sn4 Cs5 Sn12 105.93(2) 11_566 11_566
Sn4 Cs5 Sn12 74.07(2) 3_545 11_566
Sn12 Cs5 Sn12 114.32(3) 13_566 11_566
Sn12 Cs5 Sn12 65.68(3) 5_545 11_566
Sn4 Cs5 Sn12 136.938(19) 12_656 3_545
Sn4 Cs5 Sn12 43.062(19) 4_455 3_545
Sn4 Cs5 Sn12 74.07(2) 11_566 3_545
Sn4 Cs5 Sn12 105.93(2) 3_545 3_545
Sn12 Cs5 Sn12 65.68(3) 13_566 3_545
Sn12 Cs5 Sn12 114.32(3) 5_545 3_545
Sn12 Cs5 Sn12 180.00(3) 11_566 3_545
Sn4 Cs5 Sn12 136.938(19) 12_656 14_656
Sn4 Cs5 Sn12 43.062(19) 4_455 14_656
Sn4 Cs5 Sn12 74.07(2) 11_566 14_656
Sn4 Cs5 Sn12 105.93(2) 3_545 14_656
Sn12 Cs5 Sn12 105.27(3) 13_566 14_656
Sn12 Cs5 Sn12 74.73(3) 5_545 14_656
Sn12 Cs5 Sn12 108.96(3) 11_566 14_656
Sn12 Cs5 Sn12 71.04(3) 3_545 14_656
Sn4 Cs5 Sn12 43.062(19) 12_656 6_455
Sn4 Cs5 Sn12 136.938(19) 4_455 6_455
Sn4 Cs5 Sn12 105.93(2) 11_566 6_455
Sn4 Cs5 Sn12 74.07(2) 3_545 6_455
Sn12 Cs5 Sn12 74.73(3) 13_566 6_455
Sn12 Cs5 Sn12 105.27(3) 5_545 6_455
Sn12 Cs5 Sn12 71.04(3) 11_566 6_455
Sn12 Cs5 Sn12 108.96(3) 3_545 6_455
Sn12 Cs5 Sn12 180.0 14_656 6_455
Sn4 Cs5 Sn12 105.93(2) 12_656 12_656
Sn4 Cs5 Sn12 74.07(2) 4_455 12_656
Sn4 Cs5 Sn12 43.062(19) 11_566 12_656
Sn4 Cs5 Sn12 136.938(19) 3_545 12_656
Sn12 Cs5 Sn12 108.96(3) 13_566 12_656
Sn12 Cs5 Sn12 71.04(3) 5_545 12_656
Sn12 Cs5 Sn12 105.27(3) 11_566 12_656
Sn12 Cs5 Sn12 74.73(3) 3_545 12_656
Sn12 Cs5 Sn12 114.32(3) 14_656 12_656
Sn12 Cs5 Sn12 65.68(3) 6_455 12_656
Sn4 Cs5 Sn12 74.07(2) 12_656 4_455
Sn4 Cs5 Sn12 105.93(2) 4_455 4_455
Sn4 Cs5 Sn12 136.938(19) 11_566 4_455
Sn4 Cs5 Sn12 43.062(19) 3_545 4_455
Sn12 Cs5 Sn12 71.04(3) 13_566 4_455
Sn12 Cs5 Sn12 108.96(3) 5_545 4_455
Sn12 Cs5 Sn12 74.73(3) 11_566 4_455
Sn12 Cs5 Sn12 105.27(3) 3_545 4_455
Sn12 Cs5 Sn12 65.68(3) 14_656 4_455
Sn12 Cs5 Sn12 114.32(3) 6_455 4_455
Sn12 Cs5 Sn12 180.000(19) 12_656 4_455
Sn4 Cs5 Sn5 70.751(18) 12_656 11_566
Sn4 Cs5 Sn5 109.249(18) 4_455 11_566
Sn4 Cs5 Sn5 109.249(18) 11_566 11_566
Sn4 Cs5 Sn5 70.751(18) 3_545 11_566
Sn12 Cs5 Sn5 110.49(2) 13_566 11_566
Sn12 Cs5 Sn5 69.51(2) 5_545 11_566
Sn12 Cs5 Sn5 42.617(18) 11_566 11_566
Sn12 Cs5 Sn5 137.383(18) 3_545 11_566
Sn12 Cs5 Sn5 69.51(2) 14_656 11_566
Sn12 Cs5 Sn5 110.49(2) 6_455 11_566
Sn12 Cs5 Sn5 137.383(18) 12_656 11_566
Sn12 Cs5 Sn5 42.617(18) 4_455 11_566
Sn4 Cs5 Sn5 109.249(18) 12_656 5_545
Sn4 Cs5 Sn5 70.751(18) 4_455 5_545
Sn4 Cs5 Sn5 70.751(18) 11_566 5_545
Sn4 Cs5 Sn5 109.249(18) 3_545 5_545
Sn12 Cs5 Sn5 137.383(18) 13_566 5_545
Sn12 Cs5 Sn5 42.617(18) 5_545 5_545
Sn12 Cs5 Sn5 69.51(2) 11_566 5_545
Sn12 Cs5 Sn5 110.49(2) 3_545 5_545
Sn12 Cs5 Sn5 42.617(18) 14_656 5_545
Sn12 Cs5 Sn5 137.383(18) 6_455 5_545
Sn12 Cs5 Sn5 110.49(2) 12_656 5_545
Sn12 Cs5 Sn5 69.51(2) 4_455 5_545
Sn5 Cs5 Sn5 41.68(4) 11_566 5_545
Sn4 Cs5 Sn5 109.249(18) 12_656 3_545
Sn4 Cs5 Sn5 70.751(18) 4_455 3_545
Sn4 Cs5 Sn5 70.751(18) 11_566 3_545
Sn4 Cs5 Sn5 109.249(18) 3_545 3_545
Sn12 Cs5 Sn5 69.51(2) 13_566 3_545
Sn12 Cs5 Sn5 110.49(2) 5_545 3_545
Sn12 Cs5 Sn5 137.383(18) 11_566 3_545
Sn12 Cs5 Sn5 42.617(18) 3_545 3_545
Sn12 Cs5 Sn5 110.49(2) 14_656 3_545
Sn12 Cs5 Sn5 69.51(2) 6_455 3_545
Sn12 Cs5 Sn5 42.617(18) 12_656 3_545
Sn12 Cs5 Sn5 137.383(18) 4_455 3_545
Sn5 Cs5 Sn5 180.000(16) 11_566 3_545
Sn5 Cs5 Sn5 138.32(4) 5_545 3_545
Sn4 Cs5 Sn5 70.751(18) 12_656 13_566
Sn4 Cs5 Sn5 109.249(18) 4_455 13_566
Sn4 Cs5 Sn5 109.249(18) 11_566 13_566
Sn4 Cs5 Sn5 70.751(18) 3_545 13_566
Sn12 Cs5 Sn5 42.617(18) 13_566 13_566
Sn12 Cs5 Sn5 137.383(18) 5_545 13_566
Sn12 Cs5 Sn5 110.49(2) 11_566 13_566
Sn12 Cs5 Sn5 69.51(2) 3_545 13_566
Sn12 Cs5 Sn5 137.383(18) 14_656 13_566
Sn12 Cs5 Sn5 42.617(18) 6_455 13_566
Sn12 Cs5 Sn5 69.51(2) 12_656 13_566
Sn12 Cs5 Sn5 110.49(2) 4_455 13_566
Sn5 Cs5 Sn5 138.32(4) 11_566 13_566
Sn5 Cs5 Sn5 180.000(16) 5_545 13_566
Sn5 Cs5 Sn5 41.68(4) 3_545 13_566
Sn4 Cs5 Sn14 69.15(2) 12_656 .
Sn4 Cs5 Sn14 110.85(2) 4_455 .
Sn4 Cs5 Sn14 69.15(2) 11_566 .
Sn4 Cs5 Sn14 110.85(2) 3_545 .
Sn12 Cs5 Sn14 112.91(4) 13_566 .
Sn12 Cs5 Sn14 67.09(4) 5_545 .
Sn12 Cs5 Sn14 67.09(4) 11_566 .
Sn12 Cs5 Sn14 112.91(4) 3_545 .
Sn12 Cs5 Sn14 139.54(3) 14_656 .
Sn12 Cs5 Sn14 40.46(3) 6_455 .
Sn12 Cs5 Sn14 40.46(3) 12_656 .
Sn12 Cs5 Sn14 139.54(3) 4_455 .
Sn5 Cs5 Sn14 107.39(4) 11_566 .
Sn5 Cs5 Sn14 107.39(4) 5_545 .
Sn5 Cs5 Sn14 72.61(4) 3_545 .
Sn5 Cs5 Sn14 72.61(4) 13_566 .
Sn4 Cs5 Sn14 110.85(2) 12_656 10_556
Sn4 Cs5 Sn14 69.15(2) 4_455 10_556
Sn4 Cs5 Sn14 110.85(2) 11_566 10_556
Sn4 Cs5 Sn14 69.15(2) 3_545 10_556
Sn12 Cs5 Sn14 40.46(3) 13_566 10_556
Sn12 Cs5 Sn14 139.54(3) 5_545 10_556
Sn12 Cs5 Sn14 139.54(3) 11_566 10_556
Sn12 Cs5 Sn14 40.46(3) 3_545 10_556
Sn12 Cs5 Sn14 67.09(4) 14_656 10_556
Sn12 Cs5 Sn14 112.91(4) 6_455 10_556
Sn12 Cs5 Sn14 112.91(4) 12_656 10_556
Sn12 Cs5 Sn14 67.09(4) 4_455 10_556
Sn5 Cs5 Sn14 107.39(4) 11_566 10_556
Sn5 Cs5 Sn14 107.39(4) 5_545 10_556
Sn5 Cs5 Sn14 72.61(4) 3_545 10_556
Sn5 Cs5 Sn14 72.61(4) 13_566 10_556
Sn14 Cs5 Sn14 142.71(8) . 10_556
Sn4 Cs5 Sn14 69.15(2) 12_656 2
Sn4 Cs5 Sn14 110.85(2) 4_455 2
Sn4 Cs5 Sn14 69.15(2) 11_566 2
Sn4 Cs5 Sn14 110.85(2) 3_545 2
Sn12 Cs5 Sn14 139.54(3) 13_566 2
Sn12 Cs5 Sn14 40.46(3) 5_545 2
Sn12 Cs5 Sn14 40.46(3) 11_566 2
Sn12 Cs5 Sn14 139.54(3) 3_545 2
Sn12 Cs5 Sn14 112.91(4) 14_656 2
Sn12 Cs5 Sn14 67.09(4) 6_455 2
Sn12 Cs5 Sn14 67.09(4) 12_656 2
Sn12 Cs5 Sn14 112.91(4) 4_455 2
Sn5 Cs5 Sn14 72.61(4) 11_566 2
Sn5 Cs5 Sn14 72.61(4) 5_545 2
Sn5 Cs5 Sn14 107.39(4) 3_545 2
Sn5 Cs5 Sn14 107.39(4) 13_566 2
Sn14 Cs5 Sn14 37.29(8) . 2
Sn14 Cs5 Sn14 180.0 10_556 2
Sn4 Cs5 Sn14 110.85(2) 12_656 9_556
Sn4 Cs5 Sn14 69.15(2) 4_455 9_556
Sn4 Cs5 Sn14 110.85(2) 11_566 9_556
Sn4 Cs5 Sn14 69.15(2) 3_545 9_556
Sn12 Cs5 Sn14 67.09(4) 13_566 9_556
Sn12 Cs5 Sn14 112.91(4) 5_545 9_556
Sn12 Cs5 Sn14 112.91(4) 11_566 9_556
Sn12 Cs5 Sn14 67.09(4) 3_545 9_556
Sn12 Cs5 Sn14 40.46(3) 14_656 9_556
Sn12 Cs5 Sn14 139.54(3) 6_455 9_556
Sn12 Cs5 Sn14 139.54(3) 12_656 9_556
Sn12 Cs5 Sn14 40.46(3) 4_455 9_556
Sn5 Cs5 Sn14 72.61(4) 11_566 9_556
Sn5 Cs5 Sn14 72.61(4) 5_545 9_556
Sn5 Cs5 Sn14 107.39(4) 3_545 9_556
Sn5 Cs5 Sn14 107.39(4) 13_566 9_556
Sn14 Cs5 Sn14 180.0 . 9_556
Sn14 Cs5 Sn14 37.29(8) 10_556 9_556
Sn14 Cs5 Sn14 142.71(8) 2 9_556
Sn4 Cs5 Na2 70.08(10) 12_656 .
Sn4 Cs5 Na2 109.92(10) 4_455 .
Sn4 Cs5 Na2 70.08(10) 11_566 .
Sn4 Cs5 Na2 109.92(10) 3_545 .
Sn12 Cs5 Na2 107.8(5) 13_566 .
Sn12 Cs5 Na2 72.2(5) 5_545 .
Sn12 Cs5 Na2 72.2(5) 11_566 .
Sn12 Cs5 Na2 107.8(5) 3_545 .
Sn12 Cs5 Na2 142.7(3) 14_656 .
Sn12 Cs5 Na2 37.3(3) 6_455 .
Sn12 Cs5 Na2 37.3(3) 12_656 .
Sn12 Cs5 Na2 142.7(3) 4_455 .
Sn5 Cs5 Na2 113.2(5) 11_566 .
Sn5 Cs5 Na2 113.2(5) 5_545 .
Sn5 Cs5 Na2 66.8(5) 3_545 .
Sn5 Cs5 Na2 66.8(5) 13_566 .
Sn14 Cs5 Na2 6.3(6) . .
Sn14 Cs5 Na2 136.4(6) 10_556 .
Sn14 Cs5 Na2 43.6(6) 2 .
Sn14 Cs5 Na2 173.7(6) 9_556 .
Sn4 Cs5 Na2 109.92(10) 12_656 10_556
Sn4 Cs5 Na2 70.08(10) 4_455 10_556
Sn4 Cs5 Na2 109.92(10) 11_566 10_556
Sn4 Cs5 Na2 70.08(10) 3_545 10_556
Sn12 Cs5 Na2 37.3(3) 13_566 10_556
Sn12 Cs5 Na2 142.7(3) 5_545 10_556
Sn12 Cs5 Na2 142.7(3) 11_566 10_556
Sn12 Cs5 Na2 37.3(3) 3_545 10_556
Sn12 Cs5 Na2 72.2(5) 14_656 10_556
Sn12 Cs5 Na2 107.8(5) 6_455 10_556
Sn12 Cs5 Na2 107.8(5) 12_656 10_556
Sn12 Cs5 Na2 72.2(5) 4_455 10_556
Sn5 Cs5 Na2 113.2(5) 11_566 10_556
Sn5 Cs5 Na2 113.2(5) 5_545 10_556
Sn5 Cs5 Na2 66.8(5) 3_545 10_556
Sn5 Cs5 Na2 66.8(5) 13_566 10_556
Sn14 Cs5 Na2 136.4(6) . 10_556
Sn14 Cs5 Na2 6.3(6) 10_556 10_556
Sn14 Cs5 Na2 173.7(6) 2 10_556
Sn14 Cs5 Na2 43.6(6) 9_556 10_556
Na2 Cs5 Na2 130.2(11) . 10_556
Sn4 Cs5 Na2 70.08(10) 12_656 2
Sn4 Cs5 Na2 109.92(10) 4_455 2
Sn4 Cs5 Na2 70.08(10) 11_566 2
Sn4 Cs5 Na2 109.92(10) 3_545 2
Sn12 Cs5 Na2 142.7(3) 13_566 2
Sn12 Cs5 Na2 37.3(3) 5_545 2
Sn12 Cs5 Na2 37.3(3) 11_566 2
Sn12 Cs5 Na2 142.7(3) 3_545 2
Sn12 Cs5 Na2 107.8(5) 14_656 2
Sn12 Cs5 Na2 72.2(5) 6_455 2
Sn12 Cs5 Na2 72.2(5) 12_656 2
Sn12 Cs5 Na2 107.8(5) 4_455 2
Sn5 Cs5 Na2 66.8(5) 11_566 2
Sn5 Cs5 Na2 66.8(5) 5_545 2
Sn5 Cs5 Na2 113.2(5) 3_545 2
Sn5 Cs5 Na2 113.2(5) 13_566 2
Sn14 Cs5 Na2 43.6(6) . 2
Sn14 Cs5 Na2 173.7(6) 10_556 2
Sn14 Cs5 Na2 6.3(6) 2 2
Sn14 Cs5 Na2 136.4(6) 9_556 2
Na2 Cs5 Na2 49.8(11) . 2
Na2 Cs5 Na2 180.0 10_556 2
Sn4 Cs5 Na2 109.92(10) 12_656 9_556
Sn4 Cs5 Na2 70.08(10) 4_455 9_556
Sn4 Cs5 Na2 109.92(10) 11_566 9_556
Sn4 Cs5 Na2 70.08(10) 3_545 9_556
Sn12 Cs5 Na2 72.2(5) 13_566 9_556
Sn12 Cs5 Na2 107.8(5) 5_545 9_556
Sn12 Cs5 Na2 107.8(5) 11_566 9_556
Sn12 Cs5 Na2 72.2(5) 3_545 9_556
Sn12 Cs5 Na2 37.3(3) 14_656 9_556
Sn12 Cs5 Na2 142.7(3) 6_455 9_556
Sn12 Cs5 Na2 142.7(3) 12_656 9_556
Sn12 Cs5 Na2 37.3(3) 4_455 9_556
Sn5 Cs5 Na2 66.8(5) 11_566 9_556
Sn5 Cs5 Na2 66.8(5) 5_545 9_556
Sn5 Cs5 Na2 113.2(5) 3_545 9_556
Sn5 Cs5 Na2 113.2(5) 13_566 9_556
Sn14 Cs5 Na2 173.7(6) . 9_556
Sn14 Cs5 Na2 43.6(6) 10_556 9_556
Sn14 Cs5 Na2 136.4(6) 2 9_556
Sn14 Cs5 Na2 6.3(6) 9_556 9_556
Na2 Cs5 Na2 179.999(2) . 9_556
Na2 Cs5 Na2 49.8(11) 10_556 9_556
Na2 Cs5 Na2 130.2(11) 2 9_556
Sn4 Cs5 Cs4 36.834(15) 12_656 13_566
Sn4 Cs5 Cs4 143.166(15) 4_455 13_566
Sn4 Cs5 Cs4 143.166(15) 11_566 13_566
Sn4 Cs5 Cs4 36.834(15) 3_545 13_566
Sn12 Cs5 Cs4 40.427(17) 13_566 13_566
Sn12 Cs5 Cs4 139.573(17) 5_545 13_566
Sn12 Cs5 Cs4 79.891(18) 11_566 13_566
Sn12 Cs5 Cs4 100.109(18) 3_545 13_566
Sn12 Cs5 Cs4 139.573(17) 14_656 13_566
Sn12 Cs5 Cs4 40.427(17) 6_455 13_566
Sn12 Cs5 Cs4 100.109(18) 12_656 13_566
Sn12 Cs5 Cs4 79.891(18) 4_455 13_566
Sn5 Cs5 Cs4 99.43(2) 11_566 13_566
Sn5 Cs5 Cs4 141.11(2) 5_545 13_566
Sn5 Cs5 Cs4 80.57(2) 3_545 13_566
Sn5 Cs5 Cs4 38.89(2) 13_566 13_566
Sn14 Cs5 Cs4 80.73(2) . 13_566
Sn14 Cs5 Cs4 80.73(2) 10_556 13_566
Sn14 Cs5 Cs4 99.27(2) 2 13_566
Sn14 Cs5 Cs4 99.27(2) 9_556 13_566
Na2 Cs5 Cs4 77.7(3) . 13_566
Na2 Cs5 Cs4 77.7(3) 10_556 13_566
Na2 Cs5 Cs4 102.3(3) 2 13_566
Na2 Cs5 Cs4 102.3(3) 9_556 13_566
Sn4 Cs5 Cs4 143.166(15) 12_656 5_545
Sn4 Cs5 Cs4 36.834(15) 4_455 5_545
Sn4 Cs5 Cs4 36.834(15) 11_566 5_545
Sn4 Cs5 Cs4 143.166(15) 3_545 5_545
Sn12 Cs5 Cs4 139.573(17) 13_566 5_545
Sn12 Cs5 Cs4 40.427(17) 5_545 5_545
Sn12 Cs5 Cs4 100.109(18) 11_566 5_545
Sn12 Cs5 Cs4 79.891(18) 3_545 5_545
Sn12 Cs5 Cs4 40.427(17) 14_656 5_545
Sn12 Cs5 Cs4 139.573(17) 6_455 5_545
Sn12 Cs5 Cs4 79.891(18) 12_656 5_545
Sn12 Cs5 Cs4 100.109(18) 4_455 5_545
Sn5 Cs5 Cs4 80.57(2) 11_566 5_545
Sn5 Cs5 Cs4 38.89(2) 5_545 5_545
Sn5 Cs5 Cs4 99.43(2) 3_545 5_545
Sn5 Cs5 Cs4 141.11(2) 13_566 5_545
Sn14 Cs5 Cs4 99.27(2) . 5_545
Sn14 Cs5 Cs4 99.27(2) 10_556 5_545
Sn14 Cs5 Cs4 80.73(2) 2 5_545
Sn14 Cs5 Cs4 80.73(2) 9_556 5_545
Na2 Cs5 Cs4 102.3(3) . 5_545
Na2 Cs5 Cs4 102.3(3) 10_556 5_545
Na2 Cs5 Cs4 77.7(3) 2 5_545
Na2 Cs5 Cs4 77.7(3) 9_556 5_545
Cs4 Cs5 Cs4 180.0 13_566 5_545
Sn4 Cs5 Cs4 36.834(15) 12_656 11_566
Sn4 Cs5 Cs4 143.166(15) 4_455 11_566
Sn4 Cs5 Cs4 143.166(15) 11_566 11_566
Sn4 Cs5 Cs4 36.834(15) 3_545 11_566
Sn12 Cs5 Cs4 79.891(18) 13_566 11_566
Sn12 Cs5 Cs4 100.109(18) 5_545 11_566
Sn12 Cs5 Cs4 40.427(17) 11_566 11_566
Sn12 Cs5 Cs4 139.573(17) 3_545 11_566
Sn12 Cs5 Cs4 100.109(18) 14_656 11_566
Sn12 Cs5 Cs4 79.891(18) 6_455 11_566
Sn12 Cs5 Cs4 139.573(17) 12_656 11_566
Sn12 Cs5 Cs4 40.427(17) 4_455 11_566
Sn5 Cs5 Cs4 38.89(2) 11_566 11_566
Sn5 Cs5 Cs4 80.57(2) 5_545 11_566
Sn5 Cs5 Cs4 141.11(2) 3_545 11_566
Sn5 Cs5 Cs4 99.43(2) 13_566 11_566
Sn14 Cs5 Cs4 99.27(2) . 11_566
Sn14 Cs5 Cs4 99.27(2) 10_556 11_566
Sn14 Cs5 Cs4 80.73(2) 2 11_566
Sn14 Cs5 Cs4 80.73(2) 9_556 11_566
Na2 Cs5 Cs4 102.3(3) . 11_566
Na2 Cs5 Cs4 102.3(3) 10_556 11_566
Na2 Cs5 Cs4 77.7(3) 2 11_566
Na2 Cs5 Cs4 77.7(3) 9_556 11_566
Cs4 Cs5 Cs4 60.54(2) 13_566 11_566
Cs4 Cs5 Cs4 119.46(2) 5_545 11_566
Sn4 Cs5 Cs4 143.166(15) 12_656 3_545
Sn4 Cs5 Cs4 36.834(15) 4_455 3_545
Sn4 Cs5 Cs4 36.834(15) 11_566 3_545
Sn4 Cs5 Cs4 143.166(15) 3_545 3_545
Sn12 Cs5 Cs4 100.109(18) 13_566 3_545
Sn12 Cs5 Cs4 79.891(18) 5_545 3_545
Sn12 Cs5 Cs4 139.573(17) 11_566 3_545
Sn12 Cs5 Cs4 40.427(17) 3_545 3_545
Sn12 Cs5 Cs4 79.891(18) 14_656 3_545
Sn12 Cs5 Cs4 100.109(18) 6_455 3_545
Sn12 Cs5 Cs4 40.427(17) 12_656 3_545
Sn12 Cs5 Cs4 139.573(17) 4_455 3_545
Sn5 Cs5 Cs4 141.11(2) 11_566 3_545
Sn5 Cs5 Cs4 99.43(2) 5_545 3_545
Sn5 Cs5 Cs4 38.89(2) 3_545 3_545
Sn5 Cs5 Cs4 80.57(2) 13_566 3_545
Sn14 Cs5 Cs4 80.73(2) . 3_545
Sn14 Cs5 Cs4 80.73(2) 10_556 3_545
Sn14 Cs5 Cs4 99.27(2) 2 3_545
Sn14 Cs5 Cs4 99.27(2) 9_556 3_545
Na2 Cs5 Cs4 77.7(3) . 3_545
Na2 Cs5 Cs4 77.7(3) 10_556 3_545
Na2 Cs5 Cs4 102.3(3) 2 3_545
Na2 Cs5 Cs4 102.3(3) 9_556 3_545
Cs4 Cs5 Cs4 119.46(2) 13_566 3_545
Cs4 Cs5 Cs4 60.54(2) 5_545 3_545
Cs4 Cs5 Cs4 180.0 11_566 3_545
Sn4 Cs5 Cs2 79.960(12) 12_656 .
Sn4 Cs5 Cs2 100.040(12) 4_455 .
Sn4 Cs5 Cs2 79.960(12) 11_566 .
Sn4 Cs5 Cs2 100.040(12) 3_545 .
Sn12 Cs5 Cs2 76.52(2) 13_566 .
Sn12 Cs5 Cs2 103.48(2) 5_545 .
Sn12 Cs5 Cs2 103.48(2) 11_566 .
Sn12 Cs5 Cs2 76.52(2) 3_545 .
Sn12 Cs5 Cs2 142.775(18) 14_656 .
Sn12 Cs5 Cs2 37.225(18) 6_455 .
Sn12 Cs5 Cs2 37.225(18) 12_656 .
Sn12 Cs5 Cs2 142.775(18) 4_455 .
Sn5 Cs5 Cs2 145.88(2) 11_566 .
Sn5 Cs5 Cs2 145.88(2) 5_545 .
Sn5 Cs5 Cs2 34.12(2) 3_545 .
Sn5 Cs5 Cs2 34.12(2) 13_566 .
Sn14 Cs5 Cs2 43.71(5) . .
Sn14 Cs5 Cs2 99.00(5) 10_556 .
Sn14 Cs5 Cs2 81.00(5) 2 .
Sn14 Cs5 Cs2 136.29(5) 9_556 .
Na2 Cs5 Cs2 37.4(6) . .
Na2 Cs5 Cs2 92.7(6) 10_556 .
Na2 Cs5 Cs2 87.3(6) 2 .
Na2 Cs5 Cs2 142.6(6) 9_556 .
Cs4 Cs5 Cs2 63.479(12) 13_566 .
Cs4 Cs5 Cs2 116.521(12) 5_545 .
Cs4 Cs5 Cs2 116.521(12) 11_566 .
Cs4 Cs5 Cs2 63.479(12) 3_545 .
Sn4 Cs5 Cs2 100.040(12) 12_656 10_556
Sn4 Cs5 Cs2 79.960(12) 4_455 10_556
Sn4 Cs5 Cs2 100.040(12) 11_566 10_556
Sn4 Cs5 Cs2 79.960(12) 3_545 10_556
Sn12 Cs5 Cs2 37.225(18) 13_566 10_556
Sn12 Cs5 Cs2 142.775(18) 5_545 10_556
Sn12 Cs5 Cs2 142.775(18) 11_566 10_556
Sn12 Cs5 Cs2 37.225(18) 3_545 10_556
Sn12 Cs5 Cs2 103.48(2) 14_656 10_556
Sn12 Cs5 Cs2 76.52(2) 6_455 10_556
Sn12 Cs5 Cs2 76.52(2) 12_656 10_556
Sn12 Cs5 Cs2 103.48(2) 4_455 10_556
Sn5 Cs5 Cs2 145.88(2) 11_566 10_556
Sn5 Cs5 Cs2 145.88(2) 5_545 10_556
Sn5 Cs5 Cs2 34.12(2) 3_545 10_556
Sn5 Cs5 Cs2 34.12(2) 13_566 10_556
Sn14 Cs5 Cs2 99.00(5) . 10_556
Sn14 Cs5 Cs2 43.71(5) 10_556 10_556
Sn14 Cs5 Cs2 136.29(5) 2 10_556
Sn14 Cs5 Cs2 81.00(5) 9_556 10_556
Na2 Cs5 Cs2 92.7(6) . 10_556
Na2 Cs5 Cs2 37.4(6) 10_556 10_556
Na2 Cs5 Cs2 142.6(6) 2 10_556
Na2 Cs5 Cs2 87.3(6) 9_556 10_556
Cs4 Cs5 Cs2 63.479(12) 13_566 10_556
Cs4 Cs5 Cs2 116.521(12) 5_545 10_556
Cs4 Cs5 Cs2 116.521(12) 11_566 10_556
Cs4 Cs5 Cs2 63.479(12) 3_545 10_556
Cs2 Cs5 Cs2 55.29(4) . 10_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Sn1 Sn7 2.8051(13) 12_756
Sn1 Sn11 2.8445(14) 10
Sn1 Sn6 2.8564(15) .
Sn1 Sn13 2.8720(16) 9_665
Sn1 Cs4 3.8717(14) .
Sn1 Cs2 4.4712(11) 11_666
Sn1 Cs3 4.5280(15) 13_676
Sn1 Cs3 4.598(2) 7
Sn1 Na1 5.506(13) 9_665
Sn2 Sn3 2.8856(16) 7
Sn2 Sn3 2.8856(16) .
Sn2 Sn10 2.9012(18) 10
Sn2 Sn10 2.9012(18) .
Sn2 Cs4 4.0167(18) 15_665
Sn2 Cs4 4.0167(18) 9_665
Sn2 Cs2 4.113(2) 10
Sn2 Cs2 4.113(2) .
Sn3 Sn7 2.8506(13) 2_665
Sn3 Sn7 2.8506(13) 9_665
Sn3 Sn8 2.896(2) .
Sn3 Cs4 4.0862(19) 9_665
Sn3 Cs2 4.1081(18) 10
Sn3 Cs2 4.1082(18) .
Sn3 Cs3 4.533(3) 7_455
Sn3 Na2 5.71(5) 10
Sn3 Na2 5.71(5) .
Sn4 Sn12 2.8293(13) 15_665
Sn4 Sn12 2.8293(13) 2_665
Sn4 Sn10 2.837(2) .
Sn4 Sn4 2.862(3) 10
Sn4 Cs4 3.8057(14) 15_665
Sn4 Cs4 3.8057(14) 9_665
Sn4 Cs5 3.8084(14) 3_554
Sn4 Cs1 4.6213(14) 3_545
Sn4 Na2 5.53(4) 12_666
Sn4 Na2 5.53(4) 11_666
Sn5 Sn5 2.865(3) 15_665
Sn5 Sn12 2.8819(13) .
Sn5 Sn12 2.8819(13) 10
Sn5 Sn13 2.887(2) 9_665
Sn5 Cs4 3.8919(18) .
Sn5 Cs5 4.0264(14) 3_554
Sn5 Cs2 4.053(2) 4_554
Sn5 Cs2 4.053(2) 11_666
Sn5 Na1 5.09(3) 9_665
Sn5 Na2 5.39(5) 4_554
Sn5 Na2 5.39(5) 11_666
Sn6 Sn12 2.8244(14) .
Sn6 Sn8 2.8724(14) 11_666
Sn6 Sn15 2.8859(17) .
Sn6 Cs4 3.9967(11) .
Sn6 Cs3 4.0166(18) 13_676
Sn6 Cs1 4.4386(12) 11_676
Sn6 Na2 4.49(2) 11_666
Sn6 Cs2 4.6648(18) 11_666
Sn6 Na2 5.47(4) 4
Sn7 Sn1 2.8051(13) 11_676
Sn7 Sn11 2.8476(14) 10
Sn7 Sn3 2.8507(13) 9_665
Sn7 Sn15 2.8548(17) .
Sn7 Cs4 3.8485(14) .
Sn7 Cs3 4.4814(15) 13_676
Sn7 Cs3 4.566(2) 15_765
Sn7 Cs2 4.5931(17) 2_665
Sn7 Na1 5.3665(17) 3_655
Sn8 Sn16 2.845(2) .
Sn8 Sn6 2.8723(14) 3_544
Sn8 Sn6 2.8723(14) 12_656
Sn8 Na2 3.45(4) 10
Sn8 Na2 3.45(4) .
Sn8 Cs2 4.135(2) .
Sn8 Cs2 4.135(2) 10
Sn8 Cs3 4.404(2) 7_455
Sn8 Cs1 4.5626(17) 1_455
Sn9 Sn11 2.8565(9) 4_465
Sn9 Sn11 2.8565(9) 10_455
Sn9 Sn11 2.8565(9) 3_545
Sn9 Sn11 2.8565(9) 9_665
Sn9 Cs3 4.3110(12) 7_455
Sn9 Cs3 4.3110(12) 5_545
Sn9 Cs3 4.3110(12) 15_665
Sn9 Cs3 4.3110(12) 13_576
Sn10 Sn15 2.8524(15) 15_665
Sn10 Sn15 2.8524(15) 2_665
Sn10 Cs4 4.0007(14) 15_665
Sn10 Cs4 4.0007(14) 9_665
Sn10 Na1 4.087(12) 11_566
Sn10 Cs2 4.557(3) .
Sn10 Cs1 4.561(3) 3_545
Sn11 Sn1 2.8445(14) 10
Sn11 Sn7 2.8477(14) 10
Sn11 Sn9 2.8564(9) 9_665
Sn11 Sn11 2.8879(19) 10
Sn11 Cs4 3.9793(15) .
Sn11 Cs3 4.118(2) 15_765
Sn11 Cs3 4.169(2) 7
Sn11 Cs3 4.6599(10) 13_675
Sn12 Sn14 2.802(2) 11_666
Sn12 Sn4 2.8294(13) 2_665
Sn12 Na2 3.37(4) 11_666
Sn12 Cs5 3.8975(10) 3_554
Sn12 Cs4 4.0200(15) .
Sn12 Cs2 4.299(2) 11_666
Sn12 Cs1 4.5389(16) 11_676
Sn12 Na2 5.19(5) 4
Sn12 Na2 5.69(5) 12_666
Sn13 Sn17 2.716(7) .
Sn13 Sn1 2.8719(16) 9_665
Sn13 Sn1 2.8719(16) 2_665
Sn13 Sn5 2.887(2) 9_665
Sn13 Na1 3.386(18) .
Sn13 Cs2 4.052(2) 12_666
Sn13 Cs2 4.052(2) 3_554
Sn13 Cs4 4.311(2) 9_665
Sn13 Cs3 4.728(3) 15_665
Sn14 Na2 1.44(6) .
Sn14 Sn14 2.668(6) 2
Sn14 Sn16 2.739(4) .
Sn14 Sn12 2.802(2) 6_455
Sn14 Sn12 2.802(2) 12_656
Sn14 Na2 3.31(6) 10
Sn14 Na2 3.80(5) 2
Sn14 Cs5 4.172(3) .
Sn14 Cs1 4.282(4) 9_655
Sn14 Cs1 4.282(4) 1_455
Sn14 Cs2 4.677(4) .
Sn14 Na2 4.83(5) 9
Sn15 Sn17 2.661(5) 3_655
Sn15 Sn10 2.8524(15) 2_665
Sn15 Na1 3.403(12) 3_655
Sn15 Cs3 3.967(2) 13_676
Sn15 Cs4 4.2897(16) .
Sn15 Cs1 4.350(3) 11_676
Sn15 Cs2 4.882(3) 2_665
Sn16 Na2 1.31(5) 10
Sn16 Na2 1.31(5) .
Sn16 Sn14 2.739(4) 10
Sn16 Sn8 2.845(2) 7
Sn16 Cs2 4.091(4) .
Sn16 Cs2 4.091(4) 10
Sn16 Cs1 4.661(4) 9_655
Sn16 Cs1 4.661(4) 1_455
Sn16 Na2 5.52(5) 9
Sn16 Na2 5.52(5) 2
Sn17 Na1 1.217(7) .
Sn17 Sn17 2.418(13) 15_665
Sn17 Sn15 2.661(5) 4_464
Sn17 Sn15 2.661(5) 11_576
Sn17 Cs2 4.387(5) 12_666
Sn17 Cs2 4.387(5) 3_554
Sn17 Cs1 4.551(7) 9_665
Sn17 Cs3 4.650(7) 15_665
Na1 Sn17 1.217(7) 15_665
Na1 Sn13 3.386(18) 15_665
Na1 Sn15 3.403(12) 6_465
Na1 Sn15 3.403(12) 4_464
Na1 Sn15 3.403(12) 13_575
Na1 Sn15 3.403(12) 11_576
Na1 Sn10 4.087(12) 12_666
Na1 Sn10 4.087(12) 3_554
Na1 Cs2 4.127(18) 12_666
Na1 Cs2 4.127(18) 3_554
Na1 Cs1 4.52(3) 9_665
Na1 Sn5 5.09(3) 9_665
Na1 Sn5 5.09(3) 7
Na1 Sn7 5.3665(17) 4_464
Na1 Sn7 5.3665(17) 6_465
Na1 Sn7 5.3665(17) 13_575
Na1 Sn7 5.3665(17) 11_576
Na1 Sn1 5.506(13) 16
Na2 Na2 2.11(11) 10
Na2 Sn14 3.31(6) 10
Na2 Sn12 3.37(4) 6_455
Na2 Sn12 3.37(4) 12_656
Na2 Sn8 3.45(4) 7
Na2 Sn14 3.80(5) 2
Na2 Cs2 4.08(5) .
Na2 Cs1 4.32(3) 9_655
Na2 Cs1 4.32(3) 1_455
Na2 Sn6 4.49(2) 6_455
Na2 Sn6 4.49(2) 12_656
Na2 Na2 4.64(11) 2
Na2 Sn14 4.83(5) 9
Na2 Na2 5.10(11) 9
Na2 Sn12 5.19(5) 3_544
Na2 Sn12 5.19(5) 13_565
Na2 Cs2 5.39(5) 10
Cs1 Sn14 4.283(4) 9_655
Cs1 Sn14 4.282(4) 1_655
Cs1 Sn14 4.282(4) 10_655
Cs1 Sn14 4.282(4) 2_655
Cs1 Na2 4.32(3) 9_655
Cs1 Na2 4.32(3) 1_655
Cs1 Na2 4.32(3) 10_655
Cs1 Na2 4.32(3) 2_655
Cs1 Sn15 4.350(3) 14_755
Cs1 Sn15 4.350(3) 12_756
Cs1 Sn15 4.350(3) 5_645
Cs1 Sn15 4.350(3) 3_644
Cs1 Sn6 4.4386(12) 14_755
Cs1 Sn6 4.4386(12) 12_756
Cs1 Sn6 4.4386(12) 5_645
Cs1 Sn6 4.4386(12) 3_644
Cs1 Na1 4.52(3) 9_665
Cs1 Sn12 4.5389(16) 14_755
Cs1 Sn12 4.5389(16) 12_756
Cs1 Sn12 4.5389(16) 5_645
Cs1 Sn12 4.5389(16) 3_644
Cs1 Sn17 4.551(7) 7
Cs1 Sn17 4.551(7) 9_665
Cs1 Sn10 4.561(3) 4_554
Cs1 Sn10 4.561(3) 11_666
Cs1 Sn8 4.5626(17) 1_655
Cs1 Sn8 4.5626(17) 15_655
Cs1 Sn4 4.6213(14) 11_666
Cs1 Sn4 4.6213(14) 4_554
Cs1 Sn16 4.661(4) 1_655
Cs2 Sn13 4.052(2) 5_545
Cs2 Sn13 4.052(2) 11_566
Cs2 Sn5 4.053(2) 13_566
Cs2 Sn5 4.053(2) 3_545
Cs2 Sn3 4.1081(18) 7
Cs2 Na1 4.127(19) 11_566
Cs2 Sn8 4.135(2) 7
Cs2 Sn12 4.299(2) 6_455
Cs2 Sn12 4.299(2) 12_656
Cs2 Sn17 4.387(5) 5_545
Cs2 Sn17 4.387(5) 11_566
Cs2 Sn1 4.4713(11) 6_455
Cs2 Sn1 4.4713(11) 12_656
Cs2 Sn7 4.5931(17) 15_665
Cs2 Sn7 4.5931(17) 2_665
Cs2 Sn6 4.6647(18) 6_455
Cs2 Sn6 4.6647(18) 12_656
Cs2 Sn15 4.883(3) 15_665
Cs2 Sn15 4.883(3) 2_665
Cs2 Na2 5.39(5) 10
Cs2 Cs2 5.887(4) 10
Cs2 Cs2 6.217(4) 10_556
Cs2 Cs5 6.699(2) .
Cs3 Sn15 3.967(2) 13_575
Cs3 Sn15 3.967(2) 6_465
Cs3 Sn6 4.0166(18) 13_575
Cs3 Sn6 4.0166(18) 6_465
Cs3 Sn11 4.118(2) 8_675
Cs3 Sn11 4.118(2) 15_675
Cs3 Sn11 4.169(2) 7
Cs3 Sn11 4.169(2) 16
Cs3 Sn9 4.3110(12) 5
Cs3 Sn9 4.3110(12) 13_675
Cs3 Sn8 4.404(2) 7_565
Cs3 Sn7 4.4814(15) 13_575
Cs3 Sn7 4.4814(15) 6_465
Cs3 Sn1 4.5280(15) 6_465
Cs3 Sn1 4.5280(15) 13_575
Cs3 Sn3 4.533(3) 7_565
Cs3 Sn7 4.566(2) 15_675
Cs3 Sn7 4.566(2) 8_675
Cs3 Sn1 4.598(2) 7
Cs3 Sn1 4.598(2) 16
Cs3 Sn17 4.650(7) 15_665
Cs3 Sn11 4.6599(10) 13_576
Cs3 Sn11 4.6599(10) 6_464
Cs3 Sn13 4.728(3) 15_665
Cs3 Cs3 6.141(3) 9_675
Cs3 Cs1 6.565(3) 9_665
Cs3 Cs4 6.751(2) 15_675
Cs3 Cs4 6.7624(10) 13_575
Cs3 Cs4 6.7624(10) 13_576
Cs4 Sn4 3.8057(14) 9_665
Cs4 Sn4 3.8057(14) 2_665
Cs4 Sn7 3.8485(14) 10
Cs4 Sn1 3.8717(14) 10
Cs4 Sn11 3.9792(15) 10
Cs4 Sn6 3.9967(11) 10
Cs4 Sn10 4.0007(14) 2_665
Cs4 Sn10 4.0007(14) 9_665
Cs4 Sn2 4.0167(18) 9_665
Cs4 Sn12 4.0200(15) 10
Cs4 Sn3 4.0863(19) 9_665
Cs4 Sn15 4.2898(16) 10
Cs4 Sn13 4.311(2) 9_665
Cs4 Cs5 6.0930(13) 3_554
Cs4 Cs4 6.143(3) 7
Cs4 Cs2 6.7489(17) 4_554
Cs4 Cs2 6.7489(17) 11_666
Cs4 Cs3 6.751(2) 15_765
Cs4 Cs3 6.7625(10) 13_676
Cs4 Cs3 6.7625(10) 13_675
Cs4 Cs3 6.882(2) 7
Cs4 Cs2 6.922(2) 2_665
Cs4 Cs2 6.922(2) 9_665
Cs5 Sn4 3.8084(14) 12_656
Cs5 Sn4 3.8084(14) 4_455
Cs5 Sn4 3.8084(14) 11_566
Cs5 Sn4 3.8084(14) 3_545
Cs5 Sn12 3.8975(10) 13_566
Cs5 Sn12 3.8975(10) 5_545
Cs5 Sn12 3.8975(10) 11_566
Cs5 Sn12 3.8975(10) 3_545
Cs5 Sn12 3.8975(10) 14_656
Cs5 Sn12 3.8975(10) 6_455
Cs5 Sn12 3.8975(10) 12_656
Cs5 Sn12 3.8975(10) 4_455
Cs5 Sn5 4.0264(14) 11_566
Cs5 Sn5 4.0264(14) 5_545
Cs5 Sn5 4.0264(14) 3_545
Cs5 Sn5 4.0264(14) 13_566
Cs5 Sn14 4.172(3) 10_556
Cs5 Sn14 4.172(3) 2
Cs5 Sn14 4.172(3) 9_556
Cs5 Na2 5.51(6) 10_556
Cs5 Na2 5.51(6) 2
Cs5 Na2 5.51(6) 9_556
Cs5 Cs4 6.0930(13) 13_566
Cs5 Cs4 6.0930(13) 5_545
Cs5 Cs4 6.0930(13) 11_566
Cs5 Cs4 6.0930(13) 3_545
Cs5 Cs2 6.699(2) 10_556
